Concrete Pavement Design,
Construction, and Performance
Also available from Taylor & Francis
Reynolds’s Reinforced Concrete Designer Handbook
T. Threlfall et al. Hb: ISBN 978–0–419–25820–9
Pb: ISBN 978–0–419–25830–8
Reinforced Concrete 3rd edn
P. Bhatt et al. Hb: ISBN 978–0–415–30795–6
Pb: ISBN 978–0–415–30796–3
P. Mondorf Hb: ISBN 978–0–415–39362–1
Concrete Mix Design, Quality Control and
Specification 3rd edn
K. Day Hb: ISBN 978–0–415–39313–3
Binders for Durable and Sustainable Concrete
P.-C. Aïtcin Hb: ISBN 978–0–415–38588–6
Aggregates in Concrete
M. Alexander et al. Hb: ISBN 978–0–415–25839–5
Concrete Pavement Design Guidance Notes
G. Griffiths et al. Hb: ISBN 978–0–415–25451–9
Information and ordering details
For price availability and ordering visit our website www.sponpress.com
Alternatively our books are available from all good bookshops.
Concrete Pavement Design,
I dedicate this book to my late father, Norbert
Delatte Sr., who taught me to love books.
List of Figures ix
List of Tables xiii
1 Introduction 1
2 Types of concrete pavements 25
3 Performance 46
4 Subgrades, subbases, and drainage 69
5 Selection of concrete materials 95
6 Mixture design and proportioning 111
7 Design fundamentals 129
8 Highway pavement design 155
9 Light duty pavement design 172
10 Airport pavement design 199
11 Industrial pavement design 221
12 Transitions, special details, and CRCP reinforcement 231
13 Subgrade and subbase construction 249
14 Paving 262
15 Finishing, texturing, curing, and joint sawing and sealing 279
16 Concrete pavement maintenance 306
17 Rehabilitation 315
18 Overlays and inlays 330
1.1 Dowel and tie bar baskets placed in preparation for
slipform paving (photo courtesy of The Great Lakes
Construction Company, Hinckley, Ohio). 7
1.2 (a) and (b) Slipform pavers (photo courtesy of The Great
Lakes Construction Company, Hinckley, Ohio). 8
1.3 Finishing slipformed pavement around a banked curve
(photo courtesy of The Great Lakes Construction
Company, Hinckley, Ohio). 9
2.1 Jointed plain concrete pavement (JPCP) (courtesy:
2.2 Jointed reinforced concrete pavement (JRCP) (courtesy:
2.3 Continuously reinforced concrete pavement (CRCP)
(courtesy: ACPA). 29
2.4 Dowel basket assembly with corrosion resistant
epoxy-coated dowels (photo by author). 31
2.5 Doweled joint (FAA 2004: 86, 86–1). 32
2.6 Tie bar basket assemblies with corrosion resistant
epoxy-coated tie bars – dowel baskets are also shown
(photo by author). 33
2.7 Longitudinal joint (FAA 2004). 34
2.8 Header and dowel basket for a transverse construction joint
(photo by author). 34
2.9 Expansion joint detail (FHWA 1990a). 36
2.10 RCC pavement construction – Columbus, Ohio (photo by
2.11 Permeability of a pervious pavement demonstration
project – Cleveland, Ohio (photo by author). 45
3.1 Corner breaks (ACPA 1996a: VIII-16). 47
3.2 High severity D-cracking (Miller and Bellinger 2003: 37). 49
3.3 High severity longitudinal crack (Miller and Bellinger
2003: 39). 50
3.4 High severity transverse crack in JRCP (Miller and
Bellinger 2003: 41). 50
3.5 High severity transverse joint spalling (ACPA 1996a:
3.6 Map cracking (Miller and Bellinger 2003: 48). 53
3.7 Scaling (Miller and Bellinger 2003: 48). 54
3.8 Polished aggregate surface (Miller and Bellinger 2003: 49). 55
3.9 Blowup (Miller and Bellinger 2003: 52). 56
3.10 Faulted transverse joint (photo by author). 57
3.11 Water bleeding and pumping (Miller and Bellinger 2003: 58). 60
3.12 High severity punchout (Miller and Bellinger 2003: 79). 61
4.1 Roadway geometry inputs for concrete pavement drainage
4.2 Computation of inflow. 88
4.3 Determining the permeability of the base. 89
4.4 Designing the base by the depth-of-flow method. 89
4.5 Checking the base design by the time-to-drain method. 90
4.6 User-defined subgrade material. 91
4.7 Checking need for a separator layer. 91
4.8 Edge-drain design. 93
5.1 Combined aggregate relationship (coarseness factor) chart
(courtesy: Shilstone and Shilstone 2002). 102
6.1 Comparison of PCA 1984 and StreetPave fatigue
7.1 Curling stress correction factors for a finite slab (after
Bradbury 1938). 133
7.2 Corner, edge, and interior loading. 135
7.3 Maximum joint spacing based on slab thickness D
and modulus of subgrade reaction k for L/ ≤5 0 in
(a) U.S. customary units and (b) metric units. 144
8.1 WinPAS solution to design problem. 162
8.2 Spreadsheet solution to AASHTO 1998 design example. 164
8.3 Spreadsheet faulting check for AASHTO 1998 design. 165
8.4 Sensitivity analysis for AASHTO 1998 design. 166
9.1 StreetPave traffic major arterial traffic category. 178
9.2 StreetPave life cycle cost module input screen. 181
9.3 Design example traffic inputs. 182
9.4 Design example pavement inputs. 183
9.5 Concrete pavement design. 184
9.6 Design example fatigue and erosion table. 185
9.7 Rounding considerations. 185
9.8 Sensitivity of slab thickness to k-value. 186
9.9 Quadrant construction at an urban intersection in
Cleveland, Ohio (photo by the author). 196
10.1 FAA R805FAA.xls rigid airport pavement design
10.2 FAA R805FAA.xls rigid airport pavement design
spreadsheet frost design. 211
10.3 FAA R805FAA.xls rigid airport pavement design
spreadsheet computation of composite k-value. 212
10.4 Determining critical aircraft. 213
10.5 LEDFAA basic input screen. 214
10.6 Sample rigid pavement section from the LEDFAA
samples file. 215
10.7 Aircraft traffic mix. 216
10.8 Example problem rigid pavement section as designed. 218
11.1 RCCPave vehicle library. 224
11.2 RCCPave design results for example 1. 226
11.3 RCCPave design inputs for example 2. 227
12.1 Combination chair and transverse steel detail
1 in = 25 4 mm (FHWA 1990b). 243
12.2 Lug anchor treatment 1 in = 25 4 mm 1 ft = 305 mm
(FHWA 1990b). 245
12.3 Recommended WF steel beam terminal joint design
1 in = 25 4 mm 1 ft = 305 mm (FHWA 1990b). 247
14.1 Slipform paving train (ACPA 1996a: VI-6). 264
14.2 Concrete pavement produced by slipforming (ACPA
1996a: VI-6). 265
14.3 Stringline and paver sensing wand (ACPA 1996a: VI-15). 266
14.4 The pad line (ACPA 1996a: VI-20). 267
14.5 Vibrators (ACPA 1996a: VI-26). 268
14.6 Dowel basket (ACPA 1996a: VI-88). 269
14.7 Dowel bar inserters (ACPA 1996a: VI-32). 270
14.8 CRCP steel installation with tube feeders (ACPA 1996a:
14.9 Fixed form paving (ACPA 1996a: VI-68). 272
14.10 Steel forms for fixed form paving (ACPA 1996a: VI-72). 273
14.11 Blockouts for utility, drainage, and similar structures
(ACPA 1996a: VI-91). 274
15.1 Transverse tining to provide macrotexture (ACPA 1996a:
15.2 Burlap drag to provide microtexture (ACPA 1996a: VI-53). 280
15.3 Transverse joint initial and widening cut (ACPA 1996a:
15.4 Properties of rough asphalt concrete subbase. 301
15.5 Concrete mixture proportions. 302
15.6 Construction inputs. 303
15.7 Environmental inputs. 304
15.8 Results of analysis. 304
15.9 Evaporation rate predictions. 305
16.1 Effect of delay in applying a maintenance treatment. 307
16.2 Falling weight deflectometer (photo by the author). 310
17.1 Hole prepared for a full depth repair at a joint (ACPA
1996a: VIII-28). 317
17.2 Partial depth repair (ACPA 1996a: VIII-57). 318
17.3 Full depth repair with dowels and fiberboard for isolation
(ACPA 1996a: VIII-41). 320
17.4 Dowel bar retrofit (ACPA 1996a: VIII-66). 323
17.5 Diamond grinding (ACPA 1996a: VIII-11). 325
17.6 Grout injection for slab stabilization (ACPA 1996a:
18.1 Joint mismatching (Smith et al. 2002: 4–9). 333
18.2 Lane widening options (Smith et al. 2002: 4–12). 334
18.3 Unbonded overlay on two lanes with a third lane paved at
the same time (photo courtesy: Dale Crowl). 335
18.4 A transition detail for bridge approaches and overpasses
for unbonded overlays (Smith et al. 2002: 4–13). 335
18.5 Saw cutting for whitetopping with ruts (figure courtesy:
ACPA, Smith et al. 2002: 5–12). 343
18.6 A transition detail for bridge approaches and overpasses
for whitetopping (figure courtesy: ACPA, Smith et al.
2002: 5–9). 343
18.7 Output of ACPA UTW calculator
18.8 UTW placed as an inlay (photo by the author). 347
18.9 Failure of UTW by panel sliding (photo by the author). 348
18.10 UTW-thickened end transition detail (figure courtesy:
ACPA, Smith et al. 2002: 6–7). 349
4.1 Recommended k-value ranges for various soil types
(adapted from Hall et al. 1997: 80, AASHTO 1998: 6) 72
4.2 Effect of untreated subbases on k-values (PCA 1984: 6) 75
4.3 Effect of cement-treated subbases on k-values (PCA 1984: 6) 75
4.4 Effect of untreated subbases on k-values (FAA 2004: 15) 75
4.5 Effect of stabilized subbases on k-values (FAA 2004: 57) 76
4.6 Conditions where no subbase is required (FAA 2004: 55,
Table 3.10) 77
6.1 Sample concrete mixture designs for early opening to traffic
(Van Dam et al. 2005: A-1–A-2) 127
7.1 Dowel bar diameter recommendations (ACPA 1998: 27,
ACI Committee 2002 325: 15) 149
7.2 Tie bar spacing recommendations in mm (in) 152
8.1 Reliability and standard normal deviate ZR (AASHTO
1993, I-62 and II-9) 158
8.2 Drainage coefficients Cd (AASHTO 1993, II-26) 159
8.3 Load transfer coefficients J by pavement type (AASHTO
1993, II-26) 159
8.4 Input values for design example (AASHTO 1993, II-45) 161
8.5 Sensitivity analysis – effect of design parameters on
thickness D 162
9.1 Street and parking lot traffic classifications from ACI
325.12R-11 and ACI-330R-6 (ACI Committee 325 2002:
11, ACI Committee 330 2001: 6) 174
9.2 StreetPave traffic categories from help file 177
9.3 Traffic categories – axles per 1000 trucks 179
9.4 Pavement thickness design tables, aggregate interlock joints,
no edge-support 187
9.5 Pavement thickness design tables, aggregate interlock joints,
supported edges 190
9.6 Pavement thickness design tables for pervious concrete 192
10.1 Landing gear type conversion factors (FAA 2004: 25) 203
10.2 Forecast traffic and equivalent annual departures (FAA
2004: 26) 203
10.3 Maximum joint spacing for unstabilized base (FAA
2004: 87) 207
10.4 FAA dowel bar recommendations (FAA 2004: 88) 208
10.5 Traffic mix for LEDFAA design example 217
12.1 AASHTO CRCP percent steel design example (AASHTO
1993 II-56–II-62) 238
12.2 Recommended longitudinal reinforcement sizes (FHWA
12.3 Recommended WF beam dimensions (FHWA 1990b) 246
15.1 Joint sealing materials (ACPA 1996a: VII-32) 292
15.2 Typical values for PCC CTE (modified from AASHTO
1993: II-29) 294
15.3 Typical values for PCC coefficient of shrinkage
(modified from AASHTO 1993: II-29) 294
There are too many people to thank for helping me with this book, but I
will try anyway. To begin with, the members of American Concrete Insti-
tute Committees 325, Concrete Pavements, Committee 327, Roller Com-
pacted Concrete Pavements, Committee 330, Concrete Parking Lots and Site
Paving, and Committee 522, Pervious Concrete, have helped me consider-
ably with discussions during committee meetings and over beers afterward.
James Shilstone, Sr. (Jim) and James Shilstone, Jr. (Jay) supplied material
for Chapter 5, and Juan Pable Covarrubias supplied material for Chapter 9.
Tim Smith of the Cement Association of Canada, Dale Crowl of the Ohio
Department of Transportation, and George Palko of The Great Lakes Con-
struction Company supplied photographs. In addition to my colleagues, I’d
like to thank my students in courses at Cleveland State University and at
the University of Alabama at Birmingham over the years, because teaching
them challenged me to research and synthesize the material. Finally, I need
to thank my wife Lynn and our children, Isabella and Joe, for their patience
while I was drafting this manuscript.
Figures 2.1, 2.2, 2.3, and 18.7 are reprinted by permission of the Ameri-
can Concrete Pavement Association, Skokie, IL.
Figures 3.1, 3.5, 14.1–14.11, 15.1–15.3, 17.1–17.6, and Table 15.1 are
reprinted from course materials developed by the American Concrete Pave-
ment Association and used in National Highway Institute (NHI) training.
NHI is a part of the Office of Professional and Corporate Development,
Federal Highway Administration.
Concrete pavements have been used for highways, airports, streets, local
roads, parking lots, industrial facilities, and other types of infrastructure.
When properly designed and built out of durable materials, concrete pave-
ments can provide many decades of service with little or no maintenance.
“Concrete generally has a higher initial cost than asphalt but lasts longer
and has lower maintenance costs” (Hoel and Short 2006: 26).
In some cases, however, design or construction errors or poorly selected
materials have considerably reduced pavement life. It is therefore impor-
tant for pavement engineers to understand materials selection, mixture
proportioning, design and detailing, drainage, construction techniques, and
pavement performance. It is also important to understand the theoretical
framework underlying commonly used design procedures, and to know the
limits of applicability of the procedures.
The first concrete pavement was built in Bellefontaine, Ohio, in 1891, by
George Bartholomew. He had learned about cement production in Germany
and Texas and found pure sources of the necessary raw materials, limestone
and clay, in central Ohio. Because this was the first concrete pavement,
the city council required him to post a $5,000 bond that guaranteed the
pavement would last 5 years. Over 100 years later, part of his pavement
was still in use. Details of the history of the project are provided by Snell
and Snell (2002).
The American Concrete Pavement Association (ACPA) “100 Years
of Innovation” website (http://www.pavement.com/PavTech/AbtConc/His-
tory/Introduction.html) notes that the pavement “was an immediate success.
Local businessmen petitioned to have the entire block around the Square
paved with concrete. In 1893, Court Avenue and Opera Street were paved.
Columbus Avenue and the remainder of Main Street followed in 1894.” At
that time, the term “concrete” was not yet in general use, so the material
was called “artificial stone” and mixed by hand in 1.5 m (5 ft) square
forms. Other early concrete pavements included Front Street in Chicago,
which was built in 1905 and lasted 60 years, and Woodward Avenue in
Detriot (1909) which was the first mile of concrete pavement.
There may have been even earlier concrete pavement experiments. Pasko
(1998) notes “according to Blanchard’s American Highway Engineers’
Handbook of 1919, in 1879 in Scotland, a concrete was used with port-
land cement for binding. ‘The surface was very good, but when the road
commenced to break, it went to pieces very fast.’ Blanchard goes on to say
that the first portland cement concrete (PCC) pavement in the United States
was put down in 1893 on South Fitzhugh Street in Rochester, N.Y., by
J.Y. McClintock, Monroe county engineer. This was a section of portland
cement grouted macadam, a forerunner of the modern concrete pavement
of the Hassam type. The cost of this pavement was $1 per square yard
(per 0.84 square meters). However, the pavement soon deteriorated.” In
spite of this possible earlier history, it is clear the Bellefontaine was the first
successful, long-lasting concrete pavement.
In 1913, 37 km (23 miles) of concrete pavement was built near Pine Bluff,
Arkansas, at a cost of one dollar per linear foot. It became known as the
“Dollarway.” The pavement was 2.7 m (9 ft) wide and 125 mm (5 in) thick.
The remains of Dollarway are preserved as a rest area along US 6. This was
followed, in 1914, by 79 kms (49 miles) of concrete pavement for rural county
roads in Mississippi, and by the end of 1914, a total of 3,778 km (2,348 miles)
of concrete pavement had been built in the United States (ACPA 2006).
Despite the growing importance of the automobile, it was in fact a bicy-
clists’ association that was organized and effective enough to press for the
passage of the first Federal-Aid Highway Act in 1916. In the same year, the
Portland Cement Association was organized to promote the use of portland
cement and concrete. The concrete industry paved “seedling miles” with
the hope that the public would demand they be linked together with more
Early road tests
To supplement theory in the quest to develop design procedures for con-
crete pavements, many road tests were held over the years. It is believed
that the first controlled evaluation of concrete pavement performance was
conducted in 1909 by the Public Works Department of Detroit. Steelshod
shoes and heavy iron wheels were mounted at opposite ends of a pole,
revolving around a circular track, to simulate horse and wagon traffic of
the day. Test sections included concrete, granite, creosote block, and cedar
block. Based on this study, Wayne County, Michigan paved Woodward
Avenue with concrete and then paved sixty more miles of concrete roads in
the following 2 years (ACPA 2006).
After 1916, concrete roads were being built 125–225 mm (5–9 in) thick,
but little was known about thickness requirements. During 1912–1923,
the State of Illinois conducted the Bates Road Test. Using old World War
I trucks with wheel loads from 454 to 5,900 kg (1,000 to 13,000 lbs),
traffic was applied to test sections of different materials and thicknesses.
The concrete sections of uniform cross-section were 100–225 mm (4–9 in)
thick while thickened-edge sections were 229-125-229 mm and 229-152-
229 mm (9-5-9 and 9-6-9 in), some with edge bars. The results showed
that of the 22 brick, 17 asphalt, and 24 concrete sections in the test, one
brick, three asphalt, and 10 concrete sections satisfactorily withstood the
truck loadings. As a result, several design formulations were developed for
Illinois to use in building its first state highway system (ACPA 2006). The
Bates Road Test provided basic data that was used by design engineers for
many years (Yoder and Witczak 1975: 4).
Until 1922, many pavements had been built with no joints and a thick-
ened center section in an attempt to prevent the formation of an erratic
longitudinal crack that developed in 4.9–5.5 m (16–18 ft) wide pavements.
Based on the results of the Bates Road Test, center joints to eliminate
longitudinal cracking were adopted (ACPA 2006).
Other road tests followed. The Pittsburg, California Road Test of 1921–
1923 compared reinforced concrete pavement to plain concrete (ACPA
2006). This test showed no particular advantage to reinforcement, but the
test pavements were built without joints and did not reflect modern practice
(Ray 1981: 5).
In 1950 and 1951, the Bureau of Public Roads (now FHWA) with the
Highway Research Board (now the Transportation Research Board),
several states, truck manufacturers, and other highway-related indus-
tries conducted Road Test One – MD just south of Washington, D.C.
An existing 1.1 mi (1.8 km) of two-lane highway was carefully invento-
ried, instrumented, and traversed by 1,000 trucks per day. The results
showed the value of good load transfer between slabs, the effects of
speed and axle weights, and the problems caused by pumping. It pro-
duced the first dynamic wheel equivalence factors.
This road test evaluated a section of US 301 consisting of two 3.66 m (12 ft)
wide lanes with a 229-178-229 mm (9-7-9 in) thickened edge cross-section.
The pavement had been built in 1941. The slabs were reinforced with wire
mesh, and had 12.2 m (40 ft) contraction joint spacing and 36.6 m (120 ft)
expansion joint spacing (Yoder and Witczak 1975: 597).
Truck loads of 80 and 100 kN (18,000 and 22,400 lb) single axles
and 142 and 200 kN (32,000 and 44,800 lb) tandem axles were applied
between June and December 1950 (Huang 2004: 19–20). The primary aim
of this road test was not road design, but to determine proper tax allocation
between trucking and railroads.
These road tests applied accelerated traffic to pavements, simulating a
lifetime of traffic within a few months. However, it was not possible to
accelerate environmental effects in the field. Pasko (1998) notes “One also
needs to look at the effects of uncontrolled variables (environment) on
pavement performance. A good example is the Road Test One – MD where
controlled testing during July and August produced negligible damage. In
September, the area had very heavy rains. In August, eight joints were
pumping compared to 20 and 28 in September and October, respectively.
The edge pumping was 162 ft (50 m) in August, 462 ft (140 m) in September,
and 380 ft (116 m) in October after the heavy rain.”
At the Maryland Road Test, progression of cracking was definitely linked
to the development of pumping. Pumping was found to be greatest at expan-
sion joints. Pumping occurred on plastic clay soils, but not on granular
subgrades with low percentages of silt and clay. Deflections due to temper-
ature curling and warping were also measured, and found to be significant
(Yoder and Witczak 1975: 598).
The first concrete airfield pavement was built in 1928 at Ford Field in
Dearborn, Michigan. Lunken Field in Cincinnati, Ohio, was constructed
a year later. Like many early highway pavements, these airfields used a
thickened-edge section, with the pavement at the edge 50 mm (2 in) thicker
than at the centerline. Throughout the 1930s, the predominant aircraft
was the relatively light DC-3, so the trucks that delivered fuel to the air-
craft controlled the design. Early airfield concrete pavements were generally
152 mm (6 in) thick. The advent of the B-29 Superfortress bomber in World
War II required 305 mm (12 in) pavements, so existing pavements were
overlaid with 152–178 mm (6–7 in) of new concrete. With larger post-
war bombers, pavement thickness increased to 508–686 mm (20–27 in)
The work of the US Army Corps of Engineers in concrete pavement
development was significant, particularly for airfields. With the B-29 in late
World War II and progressively heavier postwar long range bombers, the
Corps faced the difficult task of designing pavements around the world
for very heavy loadings. In 1975, Yoder and Witczak noted that the
“Corps has for the past 20 years conducted extensive research programs
on prototype pavements as well as pavement test sections” (Yoder and
Witczak 1975: 4).
Ray (1981: 4–8) summarized the advances in pavement design and per-
formance that were made between 1945 and 1980.
• Based on observations of pavement deformation due to expansion or
shrinkage of highly expansive soils in the late 1930s, treatments for
these soils with cement or lime were developed.
• Mechanisms of frost heave were identified and analyzed, and meth-
ods to address frost heave through careful subgrade construction and
relatively thin granular subbase layers were adopted.
• Pumping was identified as a potential failure mechanism for concrete
pavement joints, and soils and conditions susceptible to pumping were
identified. Pumping may be controlled through use of granular subbases
and doweled joints.
• Inadequate drainage or nonuniform compaction can lead to problems
with thin granular subbases.
• Cement-treated bases (CTBs) or subbases provide excellent support and
• Under the right conditions, thin concrete pavements can provide satis-
factory service. Some 150 mm (6 in) airfield pavements lasted 30 years
or more as long as the design aircraft wheel loads were not exceeded.
Similarly, Iowa rural farm-to-market roads only 110 mm (4½ in) thick
carried traffic for 30 years.
• Even if slab stresses are not high, excessive deflections can lead to
pavement performance problems by aggravating curling and warping
• Most agencies switched exclusively to jointed plain concrete pave-
ment (JPCP) from jointed reinforced concrete pavement (JRCP) due
to spalling, blowups, and broken reinforcement at intermediate cracks
that form in JRCP slabs.
• Problems with undoweled JPCP joints led to wider adoption of dowels
for highway and airport pavements.
• JPCP with short joint spacing on the order of 4.6 m (15 ft) provides
the lowest life cycle costs for most applications.
• Concrete shoulders tied to mainline concrete pavements reduce deflec-
tions and stresses and improve safety and surface drainage and reduce
• Properly designed and built overlays – either bonded, unbonded, or
whitetopping – can provide many years of service.
The AASHO road test
The Dwight D. Eisenhower Federal-Aid Highway Act of 1956 created
the 66,000 km (41,000 mile) interstate highway system. Sixty percent
of the system was paved with concrete. There was obviously a need for
research to support this construction effort. The AASHO Road Test, a
$27-million study, was undertaken near Ottawa, Illinois. Six different test
loops were built and loaded around the clock for 2 years. Twelve dif-
ferent combinations of axles and many thicknesses of asphalt and con-
crete were evaluated in order to establish performance histories and trends
Pasko (1998) notes that
At the AASHO Road Test, there were two distinctive failure modes for
concrete pavements. The very thin pavements failed with continuous
edge pumping that caused edge-cracking that coalesced into a longitu-
dinal edge crack. The thicker pavements failed by joint pumping that
caused transverse cracking starting particularly in the traffic leave side
of the joints. The data from both were averaged together in the road
test analysis to develop a performance equation. Even so, of the 84
pavement test sections greater than 8 in (200 mm) in thickness, only
seven sections had a serviceability index of less than 4.0 at the end of
the testing. In fact, only three sections could actually be considered as
having failed. Hence, one can conclude that even though the AASHO
data is the best that we have, it hardly predicts failure of the thicknesses
of pavement that are now being built (greater than 8 in). Additionally,
at the road test, there were no punchthroughs (shear failure) such as
those produced at the Pittsburg Road Test under steel wheels, nor were
there other types of environmentally induced failures such as blow-ups,
CRCP punchouts, and so forth.
Early concrete pavements often suffered distress due to freezing and thawing
cycles, or scaling due to deicing salts, or subgrade pumping. These problems
were addressed during the 1930s, with air entrainment of concrete to attack
the durability problems. The conditions likely to lead to pumping were
identified – subgrade soil with fines that could go into suspension, water in
the subgrade, and frequent heavy axle loads. Where these conditions exist,
subbase layers between the concrete pavement and the subgrade are used
to prevent pumping.
During this period, improvements to concrete paving equipment had been
relatively minor, with motorized mixers replacing hand mixers. Pavements
were placed using relatively expensive side forms. The slipform paver was
developed in Iowa between 1946 and 1949 by two state highway engineers,
James W. Johnson and Bert Myers. The innovation was first used in 1949 to
pave a 2.7 m (9 ft) wide, 150 mm (6 in) thick county road. By using two pavers
side by side, a county road could be paved in one pass. By 1955, the Quad City
Construction Company had developed an improved, track propelled paver
that could place 7.3 m (24 ft) wide slabs 250 mm (10 in) thick, and over time
even larger pavers were developed. During this time, sawn joints began to
replace hand-tooled joints and improve pavement smoothness.
Construction practices also improved. “The 1960’s and Interstate con-
struction also saw a number of advances in concrete pavement construction
technology. Electronic controls were added to slipform pavers. Subgrade
trimmers were introduced for better grade control. Tied concrete shoulders,
first tested in Illinois in 1964, were found to add significant structural value
to concrete pavements. Concrete saws were increased in size and capability.”
(ACPA 2006). Central mixing plants increased production capacity by a
factor of 10 over the previous dry batch process. The net result of this work
was dramatic improvements in speed of construction.
Elements of modern slipform roadway paving are shown in Figures 1.1
through 1.3. In Figure 1.1, dowel and tie bars have been placed and secured
in baskets in order to provide load transfer across sawn joints. Figure 1.2
Figure 1.1 Dowel and tie bar baskets placed in preparation for slipform paving (photo
courtesy of The Great Lakes Construction Company, Hinckley, Ohio).
Figure 1.2 (a) and (b) Slipform pavers (photo courtesy of The Great Lakes Cons-
truction Company, Hinckley, Ohio).
Figure 1.3 Finishing slipformed pavement around a banked curve (photo courtesy of The
Great Lakes Construction Company, Hinckley, Ohio).
illustrates the extrusion of concrete from the slipform paver itself, along
with finishing operations. Figure 1.3 shows how slipforming can be used
around a banked curve.
Evolution of design
Yoder and Witczak note that in the early development of concrete pave-
ments, they were built directly on subgrade regardless of subgrade type or
drainage conditions. Typical slab thicknesses were 152–178 mm (6–7 in).
With increasing traffic after World War II, pumping became an increasingly
important phenomenon, although it had been described as early as 1932
(Yoder and Witczak 1975: 596).
Thickened edge sections were common in the 1930s and 1940s. For
example, a pavement would be built 152 mm (6 in) thick in the center
and 203 mm (8 in) thick along the edges, which was described as an 8-6-8
design. Pavements were typically only 5.5–6.1 m (18–20 ft) wide (Yoder
and Witczak 1975: 596–597).
As designs evolved, pavements were built over granular subbases to pre-
vent pumping. In northern climates, thick bases were also used for frost
protection. Pavement thickness was increased to 229–254 mm (9–10 in) for
highways (Yoder and Witczak 1975: 596–597). In modern practice, thicker
designs are often used for heavily traveled highways.
The long term pavement performance program
The last and greatest road test of all began in 1987 and continued for
the next two decades (and in fact continues today). This was the Federal
Highway Administration long term pavement performance (FHWA LTPP)
program, which is part of the strategic highway research program (SHRP).
The LTPP experiment encompassed rigorous field tests of more than 2,400
500 m (1,640 ft) asphalt and concrete pavement sections across the United
States and Canada (FHWA LTPP 2006).
The program consisted of both pavements that were in service at the
beginning of the test, termed general pavement studies (GPS) sections, and
pavement sections that were constructed specifically for the LTPP, termed
specific pavement studies (SPS) sections. SPS sections were constructed to
a specific experimental design within each experiment. In the original pro-
gram, there were 777 GPS sites and 234 SPS sites (Huang 2004: 26). An
additional experiment was the seasonal monitoring program (SMP) that
focused on environmental effects.
Within the GPS program, GPS-3, GPS-4, and GPS-5 analyzed JPCP,
JRCP, and continuously reinforced concrete pavement (CRCP), respectively.
Two other experiments analyzed concrete overlays on concrete pavements,
with GPS-8 for bonded overlays and GPS-9 for unbonded overlays (Huang
2004: 25–26). However, the GPS-8 bonded concrete overlay program was
Five of the nine SPS programs were relevant to rigid pavements. These
were SPS-2, structural factors, SPS-4, preventive maintenance effectiveness,
SPS-6, rehabilitation, SPS-7, bonded concrete overlays, and SPS-8, study
of environmental effects in the absence of heavy loads (Huang 2004: 26).
Because few states were willing to construct bonded concrete overlay test
sections, only four sites were built, and the SPS-7 experiment was termi-
All sites had original inventory information and materials samples col-
lected. LTPP pavement sites are visited periodically by contractors for data
collection. Data collected includes traffic, profile, smoothness, distress, fric-
tion, and falling weight deflectometer (FWD) readings. Detailed climate
information is also gathered (Huang 2004: 25–26).
The LTPP program offered many advantages over previous road tests. The
previous tests were limited to a single geographical location, and generally
used accelerated traffic loading. Accelerated traffic tends to obscure the
importance of environmental effects. In contrast, the LTPP program is
nearly two decades old, and realistic traffic and environmental conditions
have been monitored over that time.
The LTPP program produced a large number of research reports and
design and analysis tools, including the spreadsheet-based 1998 Ameri-
can Association of State Highway and Transportation Officials (AASHTO)
rigid pavement design procedure (AASHTO 1998). However, the greatest
importance of the LTPP program was in the development and calibration
of models for the new AASHTO Mechanistic-Empirical Pavement Design
In order to make LTPP data more accessible to users, the FHWA pub-
lished several versions of DataPave software. For several years, the LTPP
data and DataPave software were used for a student contest (Delatte
2002). The software has been superseded by DataPave Online, a website
that allows users to access and analyze LTPP data. “The LTPP DataPave
Online is a major effort to make the LTPP data more accessible to world-
wide transportation community” (FHWA DataPave 2006). The Trans-
portation Research Board (TRB) also has a program for LTPP studies
Economy, service life, and life cycle costs
Highway agencies have reported service lives for concrete pavements of
as much as 25–40 years, or generally 11/2–2 times the service life of
asphalt pavements designed and built to similar standards. In general,
concrete is selected for heavily trafficked pavements and typically carries
four times as much daily truck traffic as asphalt pavements. Respective
life cycle costs of pavement designs depend greatly on material costs at
the time of construction, but concrete pavements often have significantly
lower maintenance costs although initial construction costs may be higher
Challenges for the future
The interstate highway system was a monumental and historic undertaking.
However, in some respects, the engineers and builders of the early highways
and the interstate highway system had an easier task than those of today. As
the highway system has become built out, it must be maintained, repaired,
and reconstructed while, in many cases, allowing traffic to continue to
use the roadway. Much tighter environmental controls are now in place,
and quality raw materials for use in highway construction are becoming
increasingly scarce in many areas. Concrete overlays of various types have
an important part to play in the upgrading and maintaining of the overall
network. Accelerated or “fast track” paving materials and techniques have
been developed to get traffic onto pavements more quickly.
Maintenance and rehabilitation
Even the best designed and built concrete pavements will eventually wear
out and require maintenance or rehabilitation. Concrete pavement perfor-
mance and distress are addressed in Chapter 3. Maintenance techniques and
maintenance management are discussed in Chapter 16, and rehabilitation
techniques in Chapter 17. It is important to recognize that timely main-
tenance, or pavement preservation, can substantially extend pavement life
and delay the need for rehabilitation. When major work becomes necessary,
overlays, as discussed in Chapter 18, may be used.
An effective maintenance and rehabilitation program, however, also
requires a deeper understanding of how pavements behave. The basic design
aspects discussed in Chapter 7 can provide insight as to whether a partic-
ular pavement distress may be due to inadequate pavement thickness, an
unstable subbase material, or excessive joint spacing.
Meeting congestion and safety challenges
“Rehabilitation of today’s highways requires traffic management, con-
tracting and construction techniques that are quick and efficient and that
result in a pavement with superior rideability and service life” (ACPA
2000c: 1). Pavement maintenance and rehabilitation are particularly chal-
lenging for high volume pavements, particularly in congested urban areas.
The American Concrete Pavement Association (ACPA) has published Traf-
fic Management – Handbook for Concrete Pavement Reconstruction and
Rehabilitation (ACPA 2000c) to address some of these issues. Some impor-
tant points made in that document include:
• On many urban freeway reconstruction projects, the road user delay
costs may exceed $50,000 per day.
• Concrete pavement does not require a curing time of 5–14 days
before opening to traffic – mixtures are available that allow traffic in
• Limiting contractors to single lane closures or nighttime work hours
may be unwise for both safety and productivity.
• The public generally prefers a short project with major disruptions to
a long project with smaller disruptions. The slogan is “get in, get out,
• Issues that should be addressed include scope of the project, traf-
fic management, safety, construction requirements, innovative bidding,
constructability, emergency planning, and public information and coor-
• Innovative bidding and contracting practices, such as incen-
tives/disincentives and A+B bidding (bidding both price and time),
motivate and challenge contractors to finish projects and open them to
public traffic more quickly.
• Bridge abutments and clearances may constrict the range of available
work zone configuration options, and should be considered early in the
• Recycling paving materials in place, as discussed later in this chapter,
reduces project duration.
• Availability and capacity of detour routes and access for work vehicles
are key considerations. Pavements and bridges on detour routes that
will carry significant increases in traffic require structural evaluation.
• It is important to communicate with the public about the impacts,
future benefits, and progress of the project to establish and maintain
Non-destructive testing technologies such as maturity or ultrasonic pulse
velocity can estimate in-place pavement strength for opening to traffic.
ACPA (2000c: 28) provides a table for determining the strength necessary
to open the concrete pavement to public traffic.
Safety in US highway construction work zones is addressed in Part VI of
the Manual on Uniform Traffic Control Devices (FHWA 2003). Conges-
tion and capacity may be analyzed using Highway Capacity Manual 2000
Accelerated concrete pavement construction and reconstruction are also
addressed by the American Concrete Institute (ACI) committee report Accel-
erated Techniques for Concrete Paving, ACI 325.11R-01 (ACI Committee
325 2001). It is important to note that accelerated paving does not always
require high early strength concrete. With materials and mixtures in use
today, conventional paving concrete generally achieves sufficient strength
to carry traffic in 2–4 days, so if opening to traffic can be delayed that long
there is no need to use high early strength concrete. Small weekend closure
projects such as urban intersections can be built with conventional paving
concrete. If all concrete is placed by Saturday evening, it will have a day
and a half to cure for a Monday morning opening.
One interesting case study is the reconstruction of heavily trafficked
Interstate Highway 15 in Southern California. The concrete truck lanes
were badly deteriorated, and a 4.5 km (2.8 mile) section was rebuilt in
only two nine day closures. Because this is the main highway between Los
Angeles and Las Vegas, it has heavy traffic on weekends. The project is
discussed in detail by Lee et al. (2005). Some of the key features of the
• The pavement was rebuilt in nine day closures as opposed to overnight
closures, because the longer closures had been found to yield much
higher contractor productivity.
• Longer closures reduce the overall disruption to the traveling public,
provide greater life expectancy for the pavement, improve safety, and
significantly reduce construction costs.
• The existing pavement of 200 mm (8 in) of concrete over 100 mm
(4 in) of CTB over 300 mm (12 in) of aggregate base was replaced with
290 mm (11½ in) of concrete over 150 mm (6 in) of asphalt over half of
the reused aggregate base. The pavement grade was not changed. The
outer truck lane was widened by 600 mm (2 ft) to reduce edge-loading
• Caltrans went to considerable effort to communicate to the public how
the selected strategy would reduce the overall project duration and
minimize disruption to the traveling public. An automated work zone
information system gave the public travel time and detour informa-
tion on changeable message signs. Public outreach materials included
comprehensive project brochures and flyers, a construction advisory
electronic bulletin, and a project information hotline. A project website
was used to communicate information to the public and also to gather
feedback. Several public meetings were held for local communities.
• Rapid strength gain concrete with type III cement allowed opening the
pavement to traffic in 12 hours. About 50 percent of the project was
able to use a more conventional concrete with type II cement, as long
as 24 hours of curing was available.
• Project completion time incentives and disincentives and late opening
penalties were specified in the contract.
On larger projects, the bulk of the project may be paved with regular
concrete with small amounts of high early strength concrete used for small
final closure strips. This approach was adopted for critical taxiway tie-
ins during new runway construction at Cleveland Hopkins International
Airport, although it was found that with proper planning the conventional
concrete achieved sufficient early strength and it was not necessary to use
high early strength concrete (Peshkin et al. 2006b).
Case studies of similar projects can provide valuable insights into avail-
able techniques and strategies. Peshkin et al. (2006a,b) review a number of
airport case studies. The ACPA report Traffic Management – Handbook
for Concrete Pavement Reconstruction and Rehabilitation (ACPA 2000c:
iii, 50) discusses highway and street case studies:
• Reconstruction of the Eden’s Expressway in north suburban Chicago
required the Illinois DOT to use a wide range of accelerated paving
techniques and provided much of the information for the ACPA Hand-
• In Denver, Colorado, 75 days were cut from a 200-day schedule for
construction of an urban arterial.
• In Johnson County, Kansas, a major intersection was repaved over a
weekend with a whitetopping overlay.
If high early strength concrete is used, it is important to consider durability.
Some mixtures that achieve strength in 6–8 hours have shown durabil-
ity problems, although not in all cases. Durability of high early strength
concrete is discussed in Chapter 6 and by Van Dam et al. (2005). It is
particularly frustrating to agencies and users when repairs fail quickly and
need to be repeated.
Recycling and reuse of materials
The construction of highways, bridges and buildings has been increasing
from the beginning of the past century, especially in areas of high
population density. These facilities need to be repaired or replaced
with the passing of time because their end of service life is reached or
the original design no longer satisfies the needs due to the growth in
population or traffic. These facts have generated two important issues.
First, a growing demand for construction aggregates and, second, an
increase in the amount of construction waste. Two billion tons of
aggregate are produced each year in the United States. Production is
expected to increase to more than 2.5 billion tons per year by the
year 2020. This has raised concerns about the availability of natural
aggregates and where we will find new aggregate sources. On the other
hand, the construction waste produced from building demolition alone
is estimated to be 123 million tons per year. Historically, the most
common method of managing this material has been through disposal
in landfills. As cost, environmental regulations and land use policies for
landfills become more restrictive, the need to seek alternative uses of the
waste material increases. This situation has led state agencies and the
aggregate industry to begin recycling concrete debris as an alternative
(FHWA 2004: 5–6)
Pavements with steel reinforcement may also be recycled, and equipment has
been developed to economically remove reinforcement and dowels without
the need for hand labor. Continuous steel or mesh is usually removed at
the demolition site, while dowels and tie bars may be removed at a plant
where the material is processed (ACPA 1993c). Any reinforcing steel in the
concrete has to be removed.
Existing concrete can be crushed and recycled into concrete pavement,
either as new concrete pavement or as a base or subbase course under
concrete pavement. Crushing and processing may occur at or very near
to the construction site. The recycled concrete aggregate (RCA) offers a
number of advantages:
• reduces the need for virgin aggregates;
• reduces the volume of waste materials brought to landfills;
• reduces transportation costs as well as the number of trucks that must
maneuver in and out of the work zone, which can reduce project dura-
tions as well as costs;
• residual cementitious properties as well as the angularity of crushed
concrete particles can enhance the stability and stiffness of a recycled
concrete base or subbase;
• when old concrete is crushed to a smaller size, susceptibility to D-
cracking is reduced.
There are also some risks and cautions associated with the re-use of existing
• Existing concrete often has unknown properties. Construction debris
may contain unwanted bricks, wood, steel, ceramics, glass, or other
materials. As a result, some agencies only allow concrete from their
previous agency or DOT projects to be recycled for their new projects.
• Use of RCA in new concrete can create workability problems unless
the moisture content of the material is controlled.
• Some RCA needs to be washed before being used in new concrete,
which adds to cost.
• Fines in unwashed RCA may reduce concrete compressive strength.
• RCA generally has a higher absorption and lower specific gravity than
the original aggregate used in the concrete, due to the inclusion of
mortar made of cement, water, and air. It is best to keep stockpiles in
saturated surface dry (SSD) condition.
• When used as a base or subbase, the RCA should be kept wet to limit
dust and excess working should be avoided to prevent segregation. The
material should be compacted in a saturated condition.
• Concerns about leaching remain when RCA is used in a drainage layer
or near a water source.
The Federal Highway Administration Recycling Team performed a national
review of the state of the practice in Transportation Applications of Recy-
cled Concrete Aggregate. The study identified 41 states recycling concrete
aggregate, with 38 using it as aggregate base and 11 as an aggregate for PCC.
The report reviewed and summarized state practices in Texas, Virginia,
Michigan, Minnesota and California. Texas, Minnesota, and California
reported that RCA performed better than virgin aggregate as a base. One
value engineering proposal in Michigan saved $114,000 on a $3 million
project through use of RCA. Michigan has also used recycled concrete
as backfill for edge-drains. Two developments that make the use of RCA
more attractive are the use of mobile crusher units that can be moved to
stockpiles of construction debris, and mobile units that crush pavement in
place into base or subbase material (FHWA 2004). The FHWA has estab-
lished a website at http://www.fhwa.dot.gov/pavement/recycling/index.cfm
to provide information on recycling.
An important thing to remember is that concrete often fails for a reason.
If the concrete failed due to fatigue, there is little risk involved in recycling
the material. On the other hand, if the failure was due to a material-related
distress such as alkali-silica reaction (ASR), recycling the material into new
concrete simply sets the stage for a future failure. One cautionary tale
on the problems that can occur when crushed concrete is recycled in an
environment prone to sulfate attack is discussed in detail by Rollings et al.
(2006) and reviewed briefly in Chapter 5. It may be prudent to carefully
examine the existing concrete for ASR or D-cracking problems to determine
whether recycling is an option (ACPA 1993c).
When the concrete pavement has a thin asphalt overlay, it is possible
to crush the two together if it is to be used as a base or a subbase, but
not in new concrete. The asphalt in the material is not harmful, and it is
not necessary to mill off the overlay. Minnesota allows up to 3 percent
asphalt cement or approximately 50 percent reclaimed asphalt pavement
(RAP) in the crushed base material. California goes further and allows any
combination of RCA and RAP (FHWA 2004: 26).
The ACPA has published Recycling Concrete Pavement, Technical Bul-
letin TB–014.P, which discusses concrete pavement recycling from old pave-
ment removal, to concrete crushing, to replacing the new pavement. The
bulletin covers critical aspects of mix design for RCA in fresh concrete. It
may be necessary to determine the optimum rate of recycled concrete fines
in the mixture, and to pay special attention to control of water content.
A guide specification is included in the Bulletin (ACPA 1993c).
Road and airport construction and the production of concrete and other
construction materials have environmental impacts. For the most part, the
impacts of development on the landscape are similar regardless of the pave-
ment type, with the exception of pervious pavements. Also, both asphalt and
concrete pavements require large quantities of aggregate, so their impact
through aggregate mining and production are similar.
The production of portland cement impacts the environment due to the
large amounts of energy required and the release of CO2 into the atmo-
sphere. Concrete production requires approximately 3.4 GJ per cubic meter
(Mindess et al. 2003: 5). “As a major part of the world economy, the con-
crete industry must play an active role in sustainable development. Because
there are few new technologies on the horizon that can reduce CO2 emis-
sions from the manufacturing of portland cement, however, the answer to
reducing CO2 emissions lies in minimizing the output of cement clinker”
(Malhotra 2006: 42).
The total worldwide annual production of fly ash is about 900 million
tonnes (990 million tons), principally in China, India, and the US. China
alone produces two-thirds of the worldwide amount. Use of coal in power
plants, and therefore production of fly ash, is expected to increase substan-
tially in these countries over the next few decades. These countries currently
use approximately 10–15 percent of the fly ash in concrete. In the United
States, fly ash is separately batched at concrete plants, whereas overseas
the fly ash is often blended into the cement at a rate of about 20 percent
(Malhotra 2006: 42–43).
Not all fly ash meets specifications for use in concrete. Most of the fly
ash that does is type F, which is a by-product of combustion of anthracite
or bituminous coal, and has pozzolanic but not cementitious properties.
High calcium fly ash, type C, which has cementitious properties as well
as pozzolanic properties, is produced from lignite or sub-bituminous coal.
“Technologies are available, however, that can beneficiate fly ash that fails
to meet fineness and carbon content requirements – the two most important
parameters of fly ash used in concrete. These technologies include removal
of carbon by electrostatic and floatation methods. Grinding and air classifi-
cation methods have also been used to produce fly ash with high fineness”
(Malhotra 2006: 43).
Malhotra (2006: 45) suggests reducing CO2 emissions using the following
• “Using less portland cement;
• Using more supplementary cementitious materials;
• Using less unit water content by using more water-reducing admixtures
and HRWRAs [high-range water reducing admixtures];
• Incorporating recycled aggregates in concrete;
• Where possible, specifying strength acceptance criteria at 56 or 91 days
instead of 28 days.”
For paving concrete, then, the strategies for reducing cement use and thus
CO2 emissions are:
• maximize the aggregate structure as discussed in Chapter 6 to minimize
the overall paste volume;
• use water reducers to reduce the amount of water and thus the cementi-
tious material content required to maintain the same water/cementitious
materials (w/cm) ratio; and
• replace as much cement as practicable with fly ash or ground granulate
blast furnace slag (GGBFS).
Malhotra (2006: 43–44) has developed high volume fly ash (HVFA) con-
crete where as much as half or more of the cement is replaced by fly ash.
To date, HVFA concrete has not been used for pavement, to the author’s
Some other supplementary cementitious materials that could be used in
paving concrete are GGBFS, natural pozzolans, rice-husk ash, silica fume,
and metakaolin. GGBFS is already extensively used in paving concrete,
but availability is limited. Only about 25 million tonnes (28 million tons)
are produced a year. Rice-husk ash is not yet commercially available, but
the estimated worldwide potential is 20 million tonnes (22 million tons).
Silica fume and metakaolin are only available worldwide in relatively small
quantities (Malhotra 2006: 44). To date, silica fume and metakaolin have
not been widely used for pavements. Silica fume has been used for dense
concrete bridge deck overlays, and could be used for pavement bonded
Sustainable development is of increasing interest, and was written into
the American Society of Civil Engineers Code of Ethics in 1996. This
was added as item 1e – “Engineers should seek opportunities to be of
constructive service in civic affairs and work for the advancement of
the safety, health and well-being of their communities, and the protec-
tion of the environment through the practice of sustainable development”
Sustainable development is defined as “the challenge of meeting human
needs for natural resources, industrial products, energy, food, transporta-
tion, shelter, and effective waste management while conserving and protect-
ing environmental quality and the natural resource base essential for future
development” (ASCE 2006). Another term for sustainable development is
Pavements represent an important potential application area for sus-
tainability concepts. “As the world’s non-renewable resources such as fos-
sil fuels and roadway aggregates decrease in availability, it is important
for all levels of government to begin considering paving structures on a
sustainability basis rather than just a first cost basis” (Smith and Jolly
Some of the environmental and sustainability benefits of concrete pave-
• Reductions of 2.4–30 percent in energy requirements for pavement
construction and maintenance, with higher savings for more heavily
• Reduced heavy vehicle fuel consumption and greenhouse gas produc-
tion (particularly CO2) because concrete pavement has less rolling resis-
tance, therefore requiring lower vehicle power. Fuel reductions of up
to 20 percent have been observed.
• Concrete pavements use less granular material or aggregate throughout
the pavement structure because base layers are not needed. Asphalt
pavements may use twice as much. These materials are growing scarcer,
and hauling aggregates represents a significant fraction of the environ-
mental impact of highway construction.
• Supplementary cementitious materials – fly ash, ground granulated blast
furnace slag, and silica fume – are industrial by-products and their use
in concrete reduces volumes of waste.
• Concrete pavements reduce the heat island effect. Urban areas tend to
be 5 C 9 F warmer than the surrounding countryside because dark
pavements and roofs retain heat. Concrete pavement has a lighter color
and reflects light, reducing the heat island effect. Black surfaces can be
21 C 38 F warmer than the most reflective white surfaces. Reducing
the heat island effect can also reduce smog and ozone in urban areas.
• Because concrete is more reflective than asphalt, lighting requirements
are lower for concrete parking lots, reducing energy consumption
(Smith and Jolly 2005: 585–606).
An US Environmental Protection Agency (EPA) website on the heat island
effect states “For millions of Americans living in and around cities, heat
islands are of growing concern. This phenomenon describes urban and sub-
urban temperatures that are 2 to 10 F (1 to 6 C) hotter than nearby rural
areas. Elevated temperatures can impact communities by increasing peak
energy demand, air conditioning costs, air pollution levels, and heat-related
illness and mortality” (EPA 2006). Lighter colored and porous paving mate-
rials are recommended by the EPA for reducing the heat island effect.
One way of addressing sustainability in constructed facilities is through
the leadership in energy and environmental design (LEED) program.
Although LEED primarily applies to buildings, it provides principles that
are relevant to sustainability in general, and applies to parking facilities
and industrial pavements. Under LEED, buildings are eligible for points
that may be used to achieve different levels of certification. Potential LEED
points applicable to ready-mixed concrete include storm water manage-
ment, landscape paving, managing construction waste, use of recycled
materials, and reductions in the use of portland cement (RMC Research
Possible LEED strategies include:
• use of pervious concrete pavement, discussed in Chapter 2;
• concrete parking lots to reduce the heat island effect;
• diversion of construction debris from landfills through recycling or
salvage, which primarily applies to overlays, discussed in Chapter 18;
• use of by-products as supplementary cementitious materials, such as
fly ash, GGBFS, silica fume, or rice-husk ash. Use of these materials in
concrete usually reduces the amount of portland cement needed;
• use of local materials to reduce transportation costs (RMC Research
The Environmental Council of Concrete Organizations (ECCO) (www.
As a nearly inert material, concrete is an ideal medium for recycling
waste or industrial byproducts. Many materials that would end up in
landfills can be used instead to make concrete. Blast furnace slag, recy-
cled polystyrene, and fly ash are among materials that can be included
in the recipe for concrete and further enhance its appeal. Waste prod-
ucts such as scrap tires and kiln dust are used to fuel the manufacture
of cement. And even old concrete itself can be reborn as aggregate for
new concrete mixtures.
Another environmental plus for concrete is energy efficiency. From
manufacture to transport to construction, concrete is modest in its
energy needs and generous in its payback. The only energy intensive
demand is in the manufacture of portland cement, typically a 10–15%
component of concrete. Since the materials for concrete are so readily
available, concrete products and ready-mixed concrete can be made
from local resources and processed near a jobsite. Local shipping min-
imizes fuel requirements for handling and transportation.
Sources for information, research reports,
guidelines, and standards
A number of organizations publish references that are useful to the concrete
pavement engineer. Many of these references were consulted during the
development of this book and are listed in the bibliography. Although many
of these organizations are in the United States, their documents are often
used and referenced worldwide.
The websites will be useful to readers who would like to pursue the topics
discussed. Also, readers who wish to keep up with the latest developments
or contribute to the state of the practice may wish to participate in one or
more of these organizations.
One of the oldest organizations to develop information for concrete pave-
ments is the Portland Cement Association (PCA), website www.cement.org.
The PCA developed a number of important pavement design guides
up through the 1980s. The American Concrete Pavement Association
(ACPA), website www.pavement.com, subsequently has assumed most
of the PCA’s concrete pavement work. At present, the ACPA publishes
design and construction documents for highways, parking lots, streets
and local roads, airports, and industrial pavements. The ACPA and PCA
also sell a number of concrete pavement design computer programs.
The PCA continues to publish literature on roller-compacted concrete
(RCC) pavements as well as cement-stabilized base and subbase layers, as
well as a key publication on Design and Control of Concrete Mixtures
(Kosmatka et al. 2002).
The National Ready Mixed Concrete Association (NRMCA), website
http://www.nrmca.org/, is at present the primary source for information on
pervious concrete pavements. NRMCA also provides a number of certifica-
tions for concrete suppliers and contractors. The PCA, ACPA, NRMCA are
all industry associations that are supported and financed by their members.
All three of these organizations employ engineers to draft their technical
documents and also contract for outside research.
The American Concrete Institute (ACI), website www.concrete.org,
works to advance concrete knowledge through a large number of techni-
cal committees. The four technical committees most directly relevant to
concrete pavement are 325 Concrete Pavements, 327 Roller Compacted
Concrete Pavements, 330 Concrete Parking Lots and Site Paving, and 522
Pervious Concrete. The technical committee membership includes members
of industry associations, government agency representatives (e.g. FHWA,
FAA, and USACE, discussed below), academics, and consulting engineers.
Documents are produced through a rigorous consensus process, which
means they take longer to develop but are often more authoritative than
those from other sources. The documents of the four pavement committees,
as well as many others with direct application to pavements (e.g. mix-
ture proportioning, testing, and curing), are contained in the six volume
Manual of Concrete Practice and may also be purchased separately. ACI
also has a number of certification programs for testing laboratories and
ACI, APCA, and PCA publications are particularly relevant for concrete
pavement types that are not addressed by governmental organizations such
as FHWA, AASHTO, or PCA. These include parking lots, streets and local
roads, RCC, pervious concrete, and industrial pavements.
The American Society for Testing and Materials (ASTM), website
www.astm.org, works through technical committees in a similar manner to
ACI. There is also some overlap of membership between the two organiza-
tions. ASTM publishes testing protocols and materials standards.
The Transportation Research Board (TRB) is a division of the National
Research Council. The TRB website is www.trb.org. The National Research
Council is jointly administered by the National Academy of Sciences, the
National Academy of Engineering, and the Institute of Medicine. TRB is a
very large organization with international membership that covers a broad
array of transportation topics, including concrete and concrete pavement.
Concrete pavement research results are often presented at the TRB annual
meeting, and papers are published in Transportation Research Record
(TRB). Like ACI and ASTM, TRB works through constituent committees.
TRB was formerly the Highway Research Board.
The International Society for Concrete Pavements (ISCP), website
http://www.concretepavements.org/, is a relatively young organization
whose main activity has been to organize the International Conferences
on Concrete Pavements. Eight of these conferences have been held every 4
years, and the conference proceedings are a valuable source of information.
Many ISCP members also participate in TRB and ACI.
Under the United States Department of Transportation, the Federal
Highways Administration (FHWA), website http://www.fhwa.dot.gov/, is
responsible for highways. FHWA pavement research reports may be down-
loaded free from http://www.fhwa.dot.gov/pavement/pub_listing.cfm. The
FHWA also has a computer program for pavement drainage design, which
may also be downloaded free and is discussed in detail in Chapter 4.
The American Association of State Highway and Transportation Officials
(AASHTO), website http://www.transportation.org/, sells pavement design
guides and materials and test standards. AASHTO standards are often sim-
ilar or identical to ASTM standards. Many AASHTO documents, including
the pavement design guides, are developed under contract research through
the National Cooperative Highway Research Program (NCHRP), which
is under TRB. NCHRP online publications may be downloaded free from
Many US state Departments of Transportation have websites with
research reports and standards. There are obviously too many to list here.
In the United States, civil aviation is governed by the Federal Aviation
Administration (FAA), website http://www.faa.gov/. The FAA’s design and
construction standards are published in the Series 150 Advisory Circulars
and may be downloaded free from http://www.faa.gov/airports_airtraffic/
airports/resources/ recent_advisory_circulars/. The FAA also has free design
computer programs that may be downloaded. These are discussed in
The Innovative Pavement Research Foundation (IPRF), website
www.iprf.org, has published a number of research reports on airfield pave-
ments. IPRF reports may be downloaded free from the website.
For US military facilities, standards and guidelines are developed by
the US Army Corps of Engineers (USACE) and published as unified
facilities criteria (UFC) documents on the web at http://18.104.22.168/
report/doc_ufc.html. These include UFC 3-250-02 (2001a) “Standard Prac-
tice Manual for Rigid Pavements,” and UFC 3-260-02 (2001b) “Pavement
Design for Airfields.”
Types of concrete pavements
There are a number of different types of concrete pavements that have been
built. However, for the most part, they have two features in common. First,
they resist traffic loads through flexure of the concrete. If reinforcement is
used, it is used for crack control and not to carry load. The second element
is that concrete pavements contract due to drying shrinkage of the concrete,
and expand and contract due to thermal effects, and these movements must
be dealt with. Different types of pavements use joints, reinforcing steel,
The term “conventional concrete pavements” is generally taken to mean
either jointed plain, jointed reinforced, or continuously reinforced concrete
pavements (the first three categories described below) but not other types.
Design and detailing of joints is important for these pavements. All three
conventional pavement types have been used as overlays, although jointed
plain overlays are most common.
Prestressed and precast concrete pavements are used for similar applica-
tions as conventional concrete pavements, but have been used infrequently.
Other types of concrete pavement include roller compacted concrete (RCC)
and pervious or porous concrete, which are generally used for specialized
industrial or parking lot applications.
Jointed plain concrete pavement
Jointed plain concrete pavement, or JPCP, consists of unreinforced con-
crete slabs 3.6–6.0 m (12–20 ft) in length with transverse contraction joints
between the slabs. The joints are spaced closely enough together so that
cracks should not form in the slabs until late in the life of the pave-
ment. Therefore, for JPCP, the pavement expansions and contractions are
addressed through joints. JPCP is illustrated in Figure 2.1.
One important performance issue with JPCP is load transfer across the
joints. If joints become faulted, then drivers encounter bumps at the joints
and experience a rough ride. Two methods are used to provide load transfer
across JPCP joints – aggregate interlock and dowels.
26 Types of concrete pavements
Subbase or base
or rideability Thickness design
Figure 2.1 Jointed plain concrete pavement (JPCP) (courtesy: ACPA).
Aggregate interlock joints are formed during construction by sawing
1/4−1/3 of the way through the pavement to create a plane of weakness. A
crack then propagates through the remaining thickness of the pavement as
the concrete contracts. This crack has a rough surface because it propagates
around the aggregates through the green cement paste, and as long as
it remains narrow the joint can transfer load from one slab to another
through bearing stress of the aggregate particles against each other across
the crack. Load transfer is compromised if the joint opens too widely or if
the aggregates wear away. The quality and erosion resistance of the material
supporting the slab at the joint also affect load transfer.
Types of concrete pavements 27
When the pavement carries heavy vehicle traffic, particularly at high
speeds, aggregate interlock will break down over time and will not prevent
faulting over the life of the pavement. In this case, dowels are provided
across the joint for load transfer. Dowels are smooth rods, generally plain-
or epoxy-coated steel, which are usually greased or oiled on side to allow
the joints to open and close without resistance.
JPCP is the most commonly used type of concrete pavement because it is
usually the cheapest to construct. A 1999 survey by the American Concrete
Pavement Association identified 38 US states as constructing JPCP (ACPA
1999c). It is economical because there is no need to pay for any reinforcing
steel in the slabs or for labor to place the steel. In most regions, also, contrac-
tors will have more familiarity with JPCP than with other types of concrete
pavement. In those regions where corrosion of steel is a problem, the absence
of steel reinforcement means an absence of steel corrosion issues, although
the steel dowels can still corrode. To address dowel corrosion, a variety of
different dowel materials and coatings have been investigated (Snyder 2005).
JPC pavements, like other conventional concrete pavements, often use tie
bars to connect adjacent traffic lanes. Tie bars are deformed reinforcing steel
and, unlike dowels, are not intended to allow the joints to open and close.
Tie bars are used to separate lanes for highway pavements. In contrast,
airfield JPC pavements generally use dowels at all joints.
Most of this book’s design and construction guidelines primarily address
JPCP because it is the predominant concrete pavement type by far. Special
considerations for transitions between pavements and bridges and CRCP
details are discussed in Chapter 12.
Key performance issues of JPCP include:
• initial pavement smoothness, which is a function of construction
• adequate pavement thickness to prevent mid-slab cracking;
• limiting the joint spacing, also to prevent mid-slab cracking; and
• adequate joint design, detailing, and construction.
Jointed reinforced concrete pavement
Jointed reinforced concrete pavement, or JRCP, is distinguished from JPCP
by longer slabs and light reinforcement in the slabs. This light reinforcement
is often termed temperature steel. JRCP slab lengths typically range from
7.5 to 9 m (25–30 ft), although slab lengths up to 30 m (100 ft) have been
used. With these slab lengths, the joints must be doweled. The slab steel
content is typically in the range of 0.10–0.25 percent of the cross-sectional
area, in the longitudinal direction, with less steel in the transverse direction.
Either individual reinforcing bars or wire fabrics and meshes may be used.
Because the steel is placed at the neutral axis or midpoint of the slab, it
28 Types of concrete pavements
Figure 2.2 Jointed reinforced concrete pavement (JRCP) (courtesy: ACPA).
has no effect on the flexural performance of the concrete and serves only
to keep cracks together. JRCP is illustrated in Figure 2.2.
Although JRCP was widely used in the past, it is less common today.
The only advantage that JRCP has over JPCP is fewer joints, and this is
outweighed by the cost of the steel and the poor performance of the joints
and the cracks. Because the joints are spaced further apart than JPCP, they
open and close more, and load transfer suffers as joints open wider. JRCP
joints always use dowels. Furthermore, even though the slabs are longer,
the cracks still form at the same interval as JPCP, and therefore JRCP slabs
generally have one or two interior cracks each. The light steel reinforcement
across these cracks is generally not enough to maintain load transfer, and
therefore the cracks fault as well as the joints. As a result, the latest proposed
AASHTO M-EPDG procedure does not have provisions for JRCP. A 1999
survey by the American Concrete Pavement Association identified only nine
US states as constructing JRCP, and several of those are states that have
small highway networks (ACPA 1999c).
Continuously reinforced concrete pavement
Continuously reinforced concrete pavement, or CRCP, is characterized by
heavy steel reinforcement and an absence of joints. Much more steel is used
for CRCP than for JRCP, typically on the order of 0.4–0.8 percent by volume
in the longitudinal direction. Steel in the transverse direction is provided in a
lower percentage as temperature steel. CRCP is illustrated in Figure 2.3.
Cracks form in CRCP approximately 0.6–2 m (2–6 ft) apart. The rein-
forcement holds the cracks tightly together and provides for aggregate
interlock and shear transfer. CRC pavements require anchors at the begin-
ning and end of the pavement to keep the ends from contracting due to
shrinkage, and to help the desired crack pattern develop. Special CRCP
Types of concrete pavements 29
Figure 2.3 Continuously reinforced concrete pavement (CRCP) (courtesy: ACPA).
design considerations, including determination of the proper reinforcement
percentage, are discussed in Chapter 12.
Use of CRCP dates back to the 1921 Columbia Pike experimental road
in Virginia, with over 22,500 km (14,000 miles) of two-lane highway built
in the United States by 1982. CRCP has also been used for major airports
around the world (CRSI 1983: 1).
Because of the steel reinforcement, CRCP costs more than JRCP, and is
thus used less frequently in most regions. However, it provides a smoother
ride and a longer life than any other type of pavement, and is therefore a
preferred type in Texas and Illinois. A 1999 survey by the American Con-
crete Pavement Association identified only eight US states as constructing
CRCP (ACPA 1999c).
In many regions, the performance of CRCP has been excellent. A 2000
study of concrete pavement performance in the Southeastern US used the
LTPP database to investigate 14 CRCP sections in the states of Alabama,
Florida, Georgia, Mississippi, North Carolina, and South Carolina. At
the time of the study the sections were 21–30 years old and had carried
heavy traffic, but were generally in very good to excellent condition. With
three exceptions, the pavements had serviceability indices of 4 or better,
despite the fact that they had already exceeded their 20-year design lives
(Delatte et al. 2000: 4-3–4-6).
Key performance considerations for CRCP include:
• initial pavement smoothness;
• adequate pavement thickness to prevent excessive transverse cracking;
• adequate reinforcing steel to hold cracks together and prevent pun-
chouts. Punchouts are a distress mechanism distinct to CRCP and are
discussed in Chapter 3.
30 Types of concrete pavements
Conventional pavement joints
Conventional pavements (JPCP, JRCP, and CRCP) make use of several
types of transverse and longitudinal joints. Transverse contraction joints
are used in JPCP and JRCP, usually with dowels. At the end of each daily
paving operation, or for a significant delay in paving, transverse construc-
tion joints are placed, generally at the location of a planned contraction
joint for JPCP or JRCP. Transverse expansion or isolation joints are placed
where expansion of the pavement would damage adjacent bridges or other
drainage structures. Longitudinal contraction joints are created where two
or more lane widths or shoulders are paved at the same time. In contrast,
longitudinal construction joints are used between lanes or shoulders paved
at different times (ACPA 1996a: VII-9–VII-10).
The performance of concrete pavements depends to a large extent upon
the satisfactory performance of the joints. Most jointed concrete pave-
ment failures can be attributed to failures at the joint, as opposed to
inadequate structural capacity. Distresses that may result from joint
failure include faulting, pumping, spalling, corner breaks, blowups, and
mid-panel cracking. Characteristics that contribute to satisfactory joint
performance, such as adequate load transfer and proper concrete con-
solidation, have been identified through research and field experience.
The incorporation of these characteristics into the design, construction,
and maintenance of concrete pavements should result in joints capable
of performing satisfactorily over the life of the pavement. Regardless
of the joint sealant material used, periodic resealing will be required
to ensure satisfactory joint performance throughout the life of the
pavement. Satisfactory joint performance also depends on appropriate
pavement design standards, quality construction materials, and good
construction and maintenance procedures.
Transverse contraction joints
A transverse construction joint is defined as “a sawed, formed, or tooled
groove in a concrete slab that creates a weakened vertical plane. It reg-
ulates the location of the cracking caused by dimensional changes in the
slab, and is by far the most common type of joint in concrete pavements”
Lightly loaded jointed pavement contraction joints may rely only on
aggregate interlock across joints. More heavily loaded pavements almost
always use load transfer dowels in the joints. Dowels prevent vertical
movement or faulting between slabs, but allow the joint to open and
close to relieve stress buildup due to moisture and temperature changes in
the concrete pavement. A dowel basket assembly with corrosion resistant
Types of concrete pavements 31
Figure 2.4 Dowel basket assembly with corrosion resistant epoxy-coated dowels (photo
epoxy-coated dowels is shown in Figure 2.4. Dowel baskets are also shown
in Figure 1.1.
For jointed highways, transverse joints (usually doweled) are used perpen-
dicular to traffic, and longitudinal joints are used parallel to traffic, between
traffic lanes. Airport pavements are much wider, and jointed airport pave-
ments often use square or nearly square panels with dowels around all four
sides. Figure 2.5 shows a cross-section view of a doweled transverse joint.
The primary purpose of transverse contraction joints is to control the
cracking that results from the tensile and bending stresses in concrete
slabs caused by the cement hydration process, traffic loadings, and the
environment. Because these joints are so numerous, their performance
significantly impacts pavement performance. A distressed joint typically
exhibits faulting and/or spalling. Poor joint performance frequently
leads to further distresses such as corner breaks, blowups, and mid-
panel cracks. Such cracks may themselves begin to function as joints and
develop similar distresses. The performance of transverse contraction
joints is related to three major factors: joint spacing, load transfer across
the joint, and joint shape and sealant properties.
32 Types of concrete pavements
T/2 ± d/2
Paint and oil one end of dowel
Sealant material 1/4" – 3/8"
(6–10 mm) below surface
1 1/4" (32 mm)
T/4 ± 1/4"
Rod backup material
Figure 2.5 Doweled joint (FAA 2004: 86, 86–1).
Pavement distresses, including joint distresses, are discussed in Chapter 3.
Joint spacing and load transfer are discussed in Chapter 7, and joint shape
and sealants are discussed in Chapter 15.
A longitudinal joint is defined as
a joint between two slabs which allows slab warping without apprecia-
ble separation or cracking of the slabs Longitudinal joints are used
to relieve warping stresses and are generally needed when slab widths
exceed [4.6 m] 15 feet. Widths up to and including [4.6 m] 15 feet
have performed satisfactorily without a longitudinal joint, although
there is the possibility of some longitudinal cracking. Longitudinal
joints should coincide with pavement lane lines whenever possible, to
improve traffic operations. The paint stripe on widened lanes should be
at [3.7 m] 12 feet and the use of a rumble strip on the widened section
Types of concrete pavements 33
is recommended Load transfer at longitudinal joints is achieved
through aggregate interlock.
To aid load transfer, tie bars are often used across longitudinal joints. Tie
bars are thinner than dowels, and use deformed reinforcing bars rather than
smooth dowel bars. Design of longitudinal joints and tie bars is discussed
in Chapter 7. Tie bars in basket assemblies between lanes are shown in
Figures 1.1 and 2.6, along with dowel baskets. The tie bars are longer
and thinner than the dowel bars, and are also epoxy coated for corrosion
protection. Figure 2.7 shows a cross-section view of a longitudinal joint
with tie bars.
Longitudinal joints may be sawn or built as construction joints. If they
are sawn, basket assemblies as shown in Figures 1.1 and 2.6 are used and
the joint is sawn in a manner similar to transverse contraction joints. If
built as construction joints, tie bars are used to connect the new and old
For crowned pavements, it is important to provide a properly detailed
longitudinal joint at the crown. Otherwise, a crack is almost certain to form
there (Rollings 2001, 2005).
Figure 2.6 Tie bar basket assemblies with corrosion resistant epoxy-coated tie bars –
dowel baskets are also shown (photo by author).
34 Types of concrete pavements
T/2 ± d/2
Tie bar 30" (76 cm) Long on 30" (76 cm) Centers
Figure 2.7 Longitudinal joint (FAA 2004).
A construction joint is defined as “a joint between slabs that results when
concrete is placed at different times. This type of joint can be further broken
down into transverse and longitudinal joints” (FHWA 1990a). A header and
dowel basket for a transverse construction joint are shown in Figure 2.8.
After paving up to the header, the header will be removed. The next
paving day will start with the new concrete butted up against the old
Figure 2.8 Header and dowel basket for a transverse construction joint (photo by author).
Types of concrete pavements 35
Transverse construction joints should normally replace a planned con-
traction joint. However, they should not be skewed, as satisfactory
concrete placement and consolidation are difficult to obtain. Transverse
construction joints should be doweled and butted, as opposed to
keyed. Keyed transverse joints tend to spall and are not recommended.
It is recommended that transverse construction joints be sawed and
sealed. The reservoir dimensions should be the same as those used for
the transverse contraction joints.
Longitudinal construction joints with tie bars are discussed below.
It is essential that the tiebars be firmly anchored in the concrete. Tiebars
should be either mechanically inserted into the plastic concrete or
installed as a two-part threaded tiebar and splice coupler system. It is
recommended that periodic pullout tests be conducted to ensure the
tiebars are securely anchored in the concrete Bending of tiebars is
not encouraged. Where bending of the tiebars would be necessary, it is
recommended that a two-part threaded tiebar and splice coupler system
be used in lieu of tiebars. If tiebars must be bent and later straight-
ened during construction, Grade 40 [less than 276 MPa or 40 ksi yield
strength] steel should be used, as it better tolerates the bending. It may
be necessary to reapply a corrosion-resistant coating to the tiebars after
they have been straightened. When pullout tests are performed, they
should be conducted after the tiebars have been straightened. It is rec-
ommended that longitudinal construction joints be sawed and sealed.
The reservoir dimensions should be the same as those used for the
Keyed longitudinal joints have been used in the past but are now less
common. These joints use a sort of tongue and groove configuration where
one slab has a formed slot and the adjacent slab has a key that fits in the
slot to transfer shear. “The decision to use keyed longitudinal construction
joints should be given careful consideration. The top of the slab above the
keyway frequently fails in shear. For this reason, it is recommended that
keyways not be used when the pavement thickness is less than [250 mm]
10 inches. In these cases, the tiebars should be designed to carry the load
transfer” (FHWA 1990a).
An expansion joint is defined as “a joint placed at a specific location
to allow the pavement to expand without damaging adjacent structures
36 Types of concrete pavements
or the pavement itself” (FHWA 1990a). These are generally needed at
bridge abutments and at embedded utility structures in streets. For example,
Figure 2.4 shows a utility structure blockout adjacent to a dowel basket.
The embedded utility structure will require expansion joints.
Early pavement designs used transverse expansion joints as well as con-
traction joints, but performance was poor. One early design combined
expansion joints at 28 m (90 ft) intervals supplemented with contraction
joints at 9 m (30 ft) intervals in between. The expansion joints closed and
allowed the contraction joints to open too widely (Ray 1981: 6).
Good design and maintenance of contraction joints have virtually elim-
inated the need for expansion joints, except at fixed objects such as
structures. When expansion joints are used, the pavement moves to
close the unrestrained expansion joint over a period of a few years.
As this happens, several of the adjoining contraction joints may open,
effectively destroying their seals and aggregate interlock. The width
of an expansion joint is typically [19 mm] 3/4 inch or more. Filler
material is commonly placed [19 to 25 mm] 3/4 to 1 inch below
the slab surface to allow space for sealing material. Smooth dowels
are the most widely used method of transferring load across expan-
sion joints. Expansion joint dowels are specially fabricated with a
cap on one end of each dowel that creates a void in the slab to
accommodate the dowel as the adjacent slab closes the expansion
This detail is shown in Figure 2.9.
At bridges, expansion joints are very important, because an expand-
ing pavement can build up considerable force and damage bridge super-
structures and abutments. Expansion joints at bridges are discussed in
Joint filler materialJoint sealant material
Figure 2.9 Expansion joint detail (FHWA 1990a).
Types of concrete pavements 37
Pressure relief joints are intended to serve the same purpose as expansion
joints, except that they are installed after initial construction to relieve
pressure against structures and to alleviate potential pavement blowups.
Pressure relief joints are not recommended for routine installations.
However, they may be appropriate to relieve imminent structure damage
or under conditions where excessive compressive stresses exist.
Concrete pavements may also be used as overlays for either existing asphalt
or concrete pavements. For each of the two existing pavement types, there
are two overlay classifications based on whether the overlay is bonded to
the existing pavement, or whether the bond is either ignored or prevented,
and thus not considered in the design. A complete discussion of concrete
overlays is provided by Smith et al. (2002) and ACI Committee report
ACI 325.13R-06, Concrete Overlays for Pavement Rehabilitation (ACI
Committee 325 2006). Overlays are discussed in detail in Chapter 18.
The oldest type of concrete overlay over an existing asphalt pavement
is termed whitetopping. Generally, no special measures are taken to either
achieve or prevent bond between the new concrete and the old asphalt.
Many of these were constructed in the United States when existing asphalt
highways were added to the Interstate Highway system and upgraded. For
all practical purposes, these are designed and built as conventional concrete
pavements, using the existing asphalt as a high quality base. Special details
may be needed when the new concrete must be wider than the existing
asphalt. Traditionally, whitetopping overlay designs do not consider any
reduction in flexural stress in concrete due to bond.
However, for some time it has been recognized that the concrete bonds
to asphalt, and thinner overlays have been developed to take advantage
of that fact. Ultra-thin whitetopping (UTW) was developed in the United
States in the early 1990s, with overlays between 50 and 100 mm (2 and
4 in) in thickness. In order to reduce curling stresses in such thin pavements,
they are typically cut into squares 0.6–2 m (2–6 ft) on a side. Conventional
whitetopping overlays are typically at least 200 mm (8 in) thick.
Subsequently, thin whitetopping overlays have been developed to fill the
gap between light traffic UTW and conventional whitetopping. These are
generally 100–200 mm (4–8 in) thick, with 1.2–2 m (4–6 ft) squares. As with
UTW, thin whitetopping overlays rely on bond to reduce the flexural stress
in the concrete. A complete discussion of thin and ultrathin whitetopping
is provided by Rasmussen and Rozycki (2004).
Unbonded concrete overlays are constructed over existing concrete pave-
ments with specific measures taken to prevent bonding between the two
layers. Most commonly, the bond breaker is a thin layer of hot-mix asphalt.
The reason for the bond breaker is to keep cracks and other damage in the
38 Types of concrete pavements
existing pavement from propagating up through the new pavement – this
propagation is termed “reflective cracking.” With the bond breaker layer,
the existing pavement functions as a high quality base of support for the
new pavement, so there are similarities to conventional whitetopping.
Bonded concrete overlays have also been constructed. For these overlays,
the existing concrete pavement is carefully prepared to facilitate bond. These
measures are discussed in detail by Delatte et al. (1996a,b). These can be
as thin as 50 mm (2 in) because of the composite action with the existing
pavement. However, because any damage in the base concrete pavement will
reflect through the overlay, bonded concrete overlays are limited to exist-
ing pavement in good condition. This is probably the main reason that these
overlays remain rare – they are only suitable for pavements in relatively
good condition, and agencies are reluctant to invest in these pavements and
tend to allocate funds to pavements in worse condition. The other reason
they are rare is that if bond is not achieved, the thin overlays will fail rapidly.
A third type of concrete overlay on concrete pavement, the partially
bonded overlay, has been used in the past. For these overlays, no special
measures are taken to either prevent or achieve bond – the new concrete
is simply placed on top of the old. Some of these overlays were US Army
Corps of Engineers airfields, with thick overlays placed over thin existing
pavements. As a result, the contribution of the existing pavement may have
been very small. There seems to be very little recent construction of partially
bonded concrete overlays. In theory, at least, partially bonded overlays
would seem to be susceptible to reflective cracking.
Prestressed and precast concrete pavement
All conventional concrete pavements rely on the flexural strength of the
concrete to resist traffic loads over time. By using prestressing tendons to
induce a net compressive force in the pavement section it is possible to
considerably decrease the thickness of the pavement, because the traffic
loads must overcome the compressive stress before inducing a net tensile
stress and flexural fatigue into the pavement.
In addition to prestressed pavements for original construction or overlays,
precast concrete sections with either conventional or prestressed reinforce-
ment have been used as full depth patches. Precast sections may be left in
place as a permanent pavement, or may be temporary to allow traffic until
a permanent full depth patch is placed.
Pasko (1998) stated
prestressed concrete was introduced in the late 1940s and was used first
in airport pavements. About 1959, two-way prestressed slabs were used
Types of concrete pavements 39
at Biggs military airfield in Texas. The 24-in (610-mm) plain pavement
was replaced with 9-in (230-mm) post-tensioned slabs. Unfortunately,
the fear of the unknown, the need to use more skilled labor, and the
reluctance of mile-a-day slipform contractors to embrace this unproven
technology have held this concrete-saving technology back. About a
dozen highways with prestressed concrete pavements of various designs
were built in the United States between 1970 and 1990.
The first known prestressed test highway pavement was a short section in
Delaware in 1971. Other demonstration projects were at Dulles Airport,
along with two in Pennsylvania (Huang 2004: 16).
Another demonstration project, an unbonded overlay at Chicago O’Hare
International Airport, on Runway 8R-27L, was documented in the FAA
Engineering Brief No. 24. The base pavement was 305 mm (12 in) thick
CRCP on a 457 mm (18 in) thick crushed limestone base. The prestressed
overlay was 203 mm (8 in) thick on the western half and 228 mm (9 in)
thick on the eastern half, based on Boeing 747 aircraft. The dimensions
of the overlay were 244 m (800 ft) by 46 m (150 ft). The pavement was
prestressed in both the longitudinal and transverse directions (FAA 1981).
The 1993 AASHTO Pavement Design Guide discusses the design of pre-
stressed pavements. Prestressed pavement’s potential advantages include
more efficient use of construction materials (due to reduced pavement thick-
ness) and fewer joints and cracks, with reduced maintenance and longer
pavement life. Items addressed include:
• The pavement may be prestressed only longitudinally (with the pave-
ment unreinforced or conventionally reinforced transversely), pre-
stressed both longitudinally and transversely, or prestressed at an angle.
• Although prestressed pavement should work with low strength support,
fairly high strength subbases of 54 MPa/m (200 psi/in) or more have
generally been used.
• Much longer slabs may be used than conventional pavements – gener-
ally on the order of 122 m (400 ft) although slabs as long as 300 m
(1,000 ft) have been built in Europe.
• Prestress levels are typically 689–2,070 kPa (100–300 psi) in the longi-
tudinal direction and 0–1,380 kPa (0–200 psi) in the transverse direc-
• Typical tendons are 15 mm (0.6 in) strand stressed to 80 percent of
yield, spaced at two to four times slab thickness longitudinally and
three to six times slab thickness transversely.
• Because little is known about fatigue of prestressed pavements, and
because little warning may precede failure, designers should use con-
servative fatigue safety factors.
40 Types of concrete pavements
• Prestressed pavement thickness is on the order of 40–50 percent of con-
ventional concrete pavement thickness, or about 100–150 mm (4–6 in)
• Subgrade friction restraint is an important factor, and friction reducing
layers such as sand over building paper or polyethylene sheeting are
• Prestress losses on the order of 15–20 percent should be considered in
the design (AASHTO 1993: II-65–II-67).
The FAA notes that
Prestressed concrete pavements have been used in airport applications in
Europe and to a limited extent in the United States. Prestressed concrete
airport pavements are usually post-tensioned with high strength steel
strands. These pavements are usually considerably thinner than plain,
jointed reinforced, or continuously reinforced concrete pavements yet
provide high load carrying capacity. Slab lengths on the order of 400–
500 ft (120–150 m) are generally used.
(FAA 2004: 102)
Some of these projects had prestressing strand in only one direction, and
tended to have cracks form parallel to the strand due to lack of pre-
stress in the transverse direction. A 150 mm (6 in) pavement with pre-
stressing in both directions, 1.6 km (1 mile) long, was built on I-35 in
Texas and was still in excellent condition after 17 years (Merritt et al.
Recently there has been renewed interest in precast and prestressed pave-
ment systems. Tyson and Merritt (2005) described the following projects:
• A Texas Department of Transportation project, completed in 2002,
near Georgetown, TX, to demonstrate the viability of constructing a
pavement using precast prestressed concrete. TxDOT placed approxi-
mately 700 meters (2,300 feet) of two-lane pavement (plus shoulders)
on the frontage road along Interstate 35.
• The California Department of Transportation (Caltrans) built a demon-
stration project in April 2004. This was built at night on an interstate
with a low tolerance for lane closure. The agency placed approximately
76 m (250 ft) of two-lane (plus shoulder) pavement on Interstate 10
in El Monte, CA. This project is discussed in detail in Merritt et al.
At the time the article was written in 2005, additional demonstration
projects were planned for Missouri and Indiana.
Types of concrete pavements 41
The system described by Tyson and Merritt (2005) consists of the fol-
• Individual precast, prestressed pavement panels approximately 200 mm
(8 in) thick are constructed ahead of time. These are roughly equivalent
in traffic capacity to conventional pavement 355 mm (14 in) thick. The
panels are cast at the full pavement width.
• Three types of panels are used – joint, central stressing, and base panels.
Joint panels are located at the ends of each posttensioned section
and contain dowelled expansion joints to absorb horizontal slab
movements. The central stressing panels are placed at the middle
of each posttensioned section and contain large pockets or block-
outs where the posttensioning strands are fed into the ducts and
stressed. The base panels make up the majority of the pavement,
placed between the joint panels and stressing panels. During a single
construction operation, workers must place at least one complete
section of panels from joint panel to joint panel.
(Tyson and Merritt 2005)
• Panels were placed over a hot-mix asphalt leveling course.
• Shear keys along the edges of the panels facilitate vertical alignment
during construction and ensure satisfactory ride quality by preventing
Precast pavement panels
Precast concrete panels have been used in two ways for concrete pavement
rehabilitation. These are:
• temporary replacement for removed panels until concrete can be placed
during the next scheduled closure; and
• permanent pavement (selective panel replacement).
Potential advantages of precast concrete panels include higher quality con-
crete, better curing, less risk of weather disruption, and reduced delay before
opening to traffic (Lane and Kazmierowski 2005: 771). Important issues
include leveling the panels to avoid bumps at panel edges, and load transfer
between precast panels or between precast panels and existing pavement.
Precast panels are generally reinforced with mild steel, primarily to prevent
damage during transportation and handling.
Precast panels were used for temporary closure during runway intersec-
tion reconstruction at Charleston (SC) International Airport in 1990 and
42 Types of concrete pavements
Savannah/Hilton Head International Airport in 1996. Both pavement inter-
sections were reconstructed during multiple eight-hour overnight closures,
using concrete with proprietary high early strength cement. During each
closure, two 7.6 by 7.6 m (25 by 25 ft) sections were excavated and two
were filled with concrete. Precast panels approximately 3.8 m (12½ ft)
square (four per section) or 3.8 m by 2.4 m (12½ by 8 ft) (six per section)
were cast before construction, to fulfill several functions:
• Producing the precast panels allowed the contractor to gain experience
with and verify the properties and workability of the high early strength
• Panels could be used to open the runway to traffic in the event of an
• Panels were used to speed production – following each overnight clo-
sure, one section was filled with precast panels. On the next closure,
the panels were removed and the new concrete was placed as two more
panels were removed.
The contractor for the Savannah project was able to observe the Charleston
project and made improvements to the process (Drinkard 1991, McGovern
1998, Peshkin et al. 2006b).
Precast panels were evaluated on 12-lane Highway 427 in Toronto,
Canada. This is a major north–south commuter route through Toronto. All
replacement slabs were reinforced with epoxy-coated reinforcement. Three
different methods were tested, including two patented methods. All three
methods performed well, despite a relatively inexperienced contractor (Lane
and Kazmierowski 2005).
In October and November 2003, 157 distressed slabs were rehabilitated
with precast panels at 18 locations along I-25 north of Denver, Colorado.
The slabs were stabilized and slab jacked to match the elevation of the
existing pavement using high density polyurethane foam, and the joints
were backfilled with a joint bonding material. Fiber glass thin tie bars were
used instead of dowels across panel joints, but some panels cracked next
to the tie bars. Productivity increased substantially as the workers became
more familiar with the technology. It proved to be necessary to diamond
grind most of the panels to produce an acceptable ride (Buch et al. 2005).
Overall, precast slabs were found to be a satisfactory way to accommodate
short lane closures, in the same manner as the Charleston and Savannah
An innovated compression joint system has been developed in Japan
and used to construct 800 square meters (8,600 square feet) of taxiway
pavement at the Sendai Airport. The individual slabs are 14.5 m long by
2.5 m wide by 240 mm thick (47.6 ft by 8.2 ft by 9.4 in) and are prestressed.
The joints are connected with prestressing tendons which are tensioned to
Types of concrete pavements 43
provide load transfer. The existing pavement was badly distressed asphalt.
All of the work was completed during a 9 pm–7 am overnight closure
(Hachiya et al. 2001).
Roller compacted concrete
Roller compacted concrete (RCC) pavements are described in detail by
ACI Committee 325 in report ACI 325.10R (ACI 1995). RCC is a very
dry mixture that can be produced as ready-mixed concrete but is often
produced in a pugmill. RCC is also extensively used for dam construc-
tion and rehabilitation, although the mixtures and construction methods
are different. It is a low to no slump mixture that is closer in some
respects to cement treated aggregate base than a conventional, flowing
The construction process resembles that of hot-mix asphalt pavements.
The material is delivered by dump trucks, placed into an asphalt paver, and
then rolled with steel wheel rollers. The RCC is then cured. The pavement
may be allowed to crack naturally, or joints may be cut. Because RCC
shrinks less than conventional concrete, the joints or cracks are further
apart than those for JPCP.
Traditionally, the construction process has left RCC pavements with
rough surfaces which are not suitable for high speed traffic. Unsurfaced
RCC pavements have many industrial applications – multimodal freight
transfer facilities, automobile plants, and military facilities. Recent large
scale industrial projects have included Honda and Mercedes facilities in
Alabama (Delatte et al. 2003).
RCC pavements have also been constructed with hot-mix asphalt riding
surfaces. These have been widely used for new subdivision construction in
Columbus, Ohio, and for streets and roads in Quebec province, Canada.
Figure 2.10 illustrates RCC pavement construction in Columbus for a new
Some small state demonstration projects have been conducted in South
Carolina and Tennessee. The state of Georgia also used RCC to replace
deteriorated asphalt shoulders on Interstate 285 around Atlanta (Bacon
2005). Information on these and other projects has been made avail-
able by the Southeast Cement Promotion Association on the web at
RCC pavements have proven to be very economical to construct. Com-
pared to JPCP pavements, RCC pavements do not require forms, dowels
or tie bars, or labor for texturing and finishing, so construction costs are
lower. Maintenance costs also tend to be lower than other pavement types.
The flexural strength of RCC is typically equal to or better than that
of conventional concrete. A recent review of RCC in service documented
44 Types of concrete pavements
Figure 2.10 RCC pavement construction – Columbus, Ohio (photo by author).
excellent long-term performance (Piggott 1999). For high speed applica-
tions, the use of bonded concrete overlays on RCC has been investigated,
and a trial pavement has been built at an industrial facility in Michigan
All of the concrete pavement types discussed above provide impervious
cover. Except for small amounts of infiltration through joints and cracks,
precipitation runs off of the pavement surface and must be handled by a
separate drainage system.
However, in many regions developers are limited in the amount of imper-
vious cover allowed on a site. This has led to increasing interest in per-
vious or porous pavements – pavements that allow rapid water flow into
and through the pavement structure. Different types of porous pavements,
including pervious concrete, are described by Ferguson (2005). Figure 2.11
shows the permeability of a pervious concrete pavement demonstration
project constructed in Cleveland, Ohio, in August 2005.
Pervious concrete generally has much lower strength than conventional
concrete. Niethelath et al. (2005) discussed the potential benefits of pervious
Types of concrete pavements 45
Figure 2.11 Permeability of a pervious pavement demonstration project – Cleveland, Ohio
(photo by author).
concrete for reducing pavement noise, but did not address the structural
aspects of producing a durable mainline highway pavement. The solution
would most likely be a conventional concrete pavement structure with a
pervious pavement overlay.
Procedures for design and construction of pervious concrete pavements
have recently been published by ACI Committee 522 (ACI Committee
522 2006). Information about pervious concrete has been made avail-
able by the Southeast Cement Promotion Association on the web at
Because pervious concrete has a much lower flexural strength than con-
ventional concrete, it has been most widely used for parking lots and light-
traffic streets and roads. For these applications, a pavement thickness of
150 mm (6 in) has generally been found to be adequate. In the future,
however, the use of pervious concrete pavement will probably be expanded
to heavier traffic. Pervious pavement parking lots may be used as part
of building construction projects to accrue LEED points (RMC Research
Foundation 2005: 6–13).
Concrete pavement engineering is the selection of design, materials, and
construction practices to ensure satisfactory performance over the projected
life of the pavement. Pavement users are sensitive to the functional per-
formance of pavements – smoothness and skid resistance – rather than
structural performance. Pavements, as a general rule, develop distresses
gradually over time under traffic loading and environmental effects. An
exception is when poor material choices or construction practices cause
defects before or shortly after the pavement is put into service.
As part of the LTPP Program, the FHWA has developed a Distress Identi-
fication Manual (Miller and Bellinger 2003). This manual provides descrip-
tions and photographs to identify the different distress types and classify
This manual lists the following distress types for JPCP and JRCP:
• Cracking – divided into corner breaks, durability (“D”) cracking, lon-
gitudinal cracking, and transverse cracking.
• Joint deficiencies – joint seal damage (transverse or longitudinal), and
joint spalling (transverse or longitudinal).
• Surface defects – divided into map cracking, scaling, polished aggre-
gates, and popouts.
• Miscellaneous distresses – classified as blowups, faulting of transverse
joints and cracks, lane-to-shoulder dropoff, lane-to-shoulder separa-
tion, patch deterioration, and water bleeding and pumping.
This manual lists the following distress types for CRCP:
• Cracking – as above, except CRCP cannot have corner breaks.
• Surface defects – as above.
• Miscellaneous distresses – as above, with the addition of punchouts,
transverse construction joint deterioration, and longitudinal joint seal
damage. Also, CRCP does not have joints, so joint faulting does
Another manual for concrete condition assessment is provided by the ACI
Committee 201 report 201.1R-92 Guide for Making a Condition Survey of
Concrete in Service (ACI Committee 201 1992).
Cracks may form in concrete pavements due to a one time overload or due
to repeated fatigue loading. The exception is tight, closely spaced transverse
cracks formed intentionally in CRCP.
Corner breaks only occur at corners of JPCP or JRCP. A triangular piece
of concrete, from 0.3 m (1 ft) to half the width of the slab, breaks off
(Miller and Bellinger 2003: 36). These are more likely with longer slabs,
because as the slabs warp or curl upward the slab corners may become
unsupported and break off when heavy vehicles travel across them. Huang
(2004: 378) notes that “load repetitions combined with loss of support, poor
load transfer across the joint, and thermal curling and moisture warping
stresses usually cause corner breaks.” Corner breaks may be avoided by
limiting slab lengths, particularly with stiffer subbases, and by providing
load transfer to adjacent slabs through dowels and tie bars. A moderate
severity corner break is shown in Figure 3.1.
Figure 3.1 Corner breaks (ACPA 1996a: VIII-16).
Durability (“D”) cracking
Durability or “D” cracking occurs near joints, cracks, and free edges, and
is manifested as a “closely spaced crescent-shaped hairline cracking pat-
tern” (Miller and Bellinger 2003: 37). The cracks are often darker than the
remaining uncracked concrete. Yoder and Witczak (1975: 636) note that
the phenomenon is regional and due to use of non-durable materials and/or
severe climatic conditions. It is a progressive failure mechanism than may
eventually result in nearly total disintegration of the slab.
According to Huang (2004: 387), it is caused by freeze-thaw expansion
of some types of coarse aggregate. Mindess et al. (2003: 503) note that
the problem occurs frequently with limestones in midwestern states in the
United States. There is also a critical size for many aggregates below which
they are not susceptible to fracture (Mindess et al. 2003: 502). There-
fore, D-cracking may be prevented by avoiding susceptible aggregates or, if
only susceptible aggregates are available, by using smaller maximum coarse
aggregate size. For some poorly consolidated sedimentary rocks, this critical
dimension may be as small as 12–25 mm (1/2–1 in) (Mindess et al. 2003:
140). High severity D-cracking is shown in Figure 3.2.
Longitudinal cracks are defined as those parallel to the pavement centerline
(Miller and Bellinger 2003: 38). Huang (2004: 380) suggests that longitu-
dinal cracks are caused by a combination of heavy load repetitions, loss
of foundation support, and curling and warping stresses, or by improper
construction of longitudinal joints. If longitudinal cracks are not in vehicle
wheel paths and do not fault appreciably, the effect on pavement perfor-
mance may not be significant. Longitudinal cracks are also likely to occur
at the crowns of crowned pavements if longitudinal joints are not pro-
vided (Rollings 2001, 2005). A high severity longitudinal crack is shown in
Transverse cracks are defined as those perpendicular to the pavement center-
line (Miller and Bellinger 2003: 40). They are a key JPCP concrete pavement
performance measure, because once a transverse crack forms its faulting and
deterioration leads to severe roughness. JPCP does not have steel across the
crack to hold it together. The cracking can progress and lead to a shattered
slab, requiring slab replacement (Hoerner et al. 2001: 70). Huang (2004:
384) notes that transverse cracks are “usually caused by a combination of
heavy load repetitions and stresses due to temperature gradient, moisture
gradient, and drying shrinkage.” A high severity transverse crack in JRCP
is shown in Figure 3.4.
Figure 3.2 High severity D-cracking (Miller and Bellinger 2003: 37).
Figure 3.3 High severity longitudinal crack (Miller and Bellinger 2003: 39).
Figure 3.4 High severity transverse crack in JRCP (Miller and Bellinger 2003: 41).
Yu et al. (1998) found that transverse cracking risk is higher in drier
climates with longer joint spacings, due to the higher temperature gradi-
ents that develop in these climates. Overall, increased joint spacing greatly
increases transverse cracking. Determining proper joint spacing is discussed
in detail in Chapter 7.
In JRCP and CRCP, transverse cracks are expected to form. The key
difference is how the cracks perform. With CRCP, there is enough steel to
keep cracks tightly closed unless they progress to punchouts. With JRCP,
there is not enough steel to prevent crack deterioration and faulting.
As only JPCP and JRCP have joints, these pavement types alone can have
joint deficiencies. These are classified as seal damage or spalling.
Joint seal damage (transverse or longitudinal)
Joint seals are used to keep incompressible materials and water from pen-
etrating joints. Incompressible materials can lead to stress concentrations
when open pavement joints close, causing some of the concrete to spall off.
Water leads to deterioration in the pavement and underlying layers.
Typical types of joint seal damage include extrusion (seal coming up out
of joint), hardening, adhesive failure (loss of bond), cohesive failure (split-
ting), complete loss of sealant, intrusion of foreign material, or weed growth
in the joint (Miller and Bellinger 2003: 44). Joints must be periodically
cleaned out and resealed, and this type of damage usually indicates a need
to maintain the joints.
Transverse joint seal damage is only an issue with JPCP or JRCP. Longi-
tudinal joint seal damage may occur with any type of conventional concrete
Joint spalling (transverse or longitudinal)
Joint spalling is defined as “cracking, breaking, chipping, or fraying of slab
edges within 0.3 m (1 foot) from the face of the joint” (Miller and Bellinger
2003: 45–46). Spalls are a surface phenomenon and are generally caused
by incompressible materials creating stress concentrations in joints as they
close due to slab expansion or traffic loading. They may also be caused
by “poorly designed or constructed load transfer devices” (Huang 2004:
382). Therefore, the best way to avoid spalls is to properly maintain joints.
Spalls may also be caused by poor construction practices, such as failing to
properly cure pavement joints after saw cutting. High severity transverse
joint spalling is shown in Figure 3.5.
Figure 3.5 High severity transverse joint spalling (ACPA 1996a: VIII-47).
Unlike cracking and joint deficiencies, surface defects are usually unrelated
to design. They are due to either poor materials selection or poor construc-
tion practices, or both.
Map cracking is defined as “a series of cracks that extend only into the upper
surface of the slab. Larger cracks frequently are oriented in the longitudinal
direction of the pavement and are interconnected by finer transverse or
random cracks” (Miller and Bellinger 2003: 47). According to Huang (2004:
387), it is usually caused by overfinishing of concrete. Mindess et al. (2003:
507) note that map cracking can either be caused by excessive bleeding and
plastic shrinkage from finishing too much or too early, which leads to fine
cracks, or by ASR, which leads to coarse cracks. Map cracking is shown in
It is useful to distinguish between map cracking due to finishing problems,
which is unlikely to progress further, and map cracking due to ASR, which is
likely to progress and lead to eventual destruction of the pavement. ASR is an
increasingly important problem for concrete pavements, and is difficult to fix.
ASR is one of two types of alkali-aggregate reactions in concrete, the
other being alkali-carbonate reaction. ASR is due to an expansive reaction
Figure 3.6 Map cracking (Miller and Bellinger 2003: 48).
between alkalis in cement paste and certain reactive forms of silica within
aggregate. The reactive aggregate components include opal, silica glass,
chalcedony, cristobalite tridymite, and quartz, which can occur in siliceous
and volcanic rocks and quartzite. Problems were observed in the United
States in structures built between the late 1920s and early 1940s, and
problems have been noted primarily in western and southwestern parts of
the country. Factors that affect ASR include nature, amount, and particle
size of the reactive silica, amount of available alkali, and the presence of
moisture. Since concrete pavements cannot be kept free of moisture, the
solution is to either use low alkali cements or non-reactive aggregates. In
some regions, however, non-reactive aggregates may not be economically
available. Fly ash, GGBFS, and silica fume have been found to reduce the
effects of ASR. Class F fly ash typically provides adequate protection at
15–20 percent replacement of cement, but class C fly ash is usually less
effective (Mindess et al. 2003: 142–152).
Similar reactions include a form of ASR in sand-gravel aggregates from
some river systems in the states of Kansas, Nebraska, Iowa, Missouri,
and Wyoming, and alkali-carbonate reactions. Alkali-carbonate reactions
involve carbonate rocks in some midwestern and eastern states as well as
eastern Canada (Mindess et al. 2003: 153–154). ASR and other alkali-
aggregate reactions are discussed in detail in ACI 221.1R-98, Report on
Alkali-Aggregate Reactivity (ACI Committee 221 1998).
Scaling is defined as “the deterioration of the upper concrete slab surface,
normally 3–13 mm (1/8-1/2 inch), and may occur anywhere over the pave-
ment” (Miller and Bellinger 2003: 47). Scaling may progress from map
cracking (Huang 2004: 387). Scaling is shown in Figure 3.7.
Scaling may also occur with repeated application of deicing salts. This
type of scaling may be prevented by using an adequately air entrained low
permeability concrete with a low water/cement (w/c) ratio. Risk of scaling
is higher on concrete surfaces that have not been finished properly (Mindess
et al. 2003: 504–505).
Polished aggregate problems refer to “surface mortar and texturing worn
away to expose coarse aggregate” (Miller and Bellinger 2003: 49). This
typically leads to a reduction in surface friction. The reduction in surface
friction can make pavements unsafe, particularly in wet weather. A polished
aggregate surface is shown in Figure 3.8.
Because cement paste does not have good abrasion resistance, the wear
resistance of concrete depends on the hardness of aggregates used. Poor
finishing practices may also lead to a weak surface layer and lower abrasion
resistance (Mindess et al. 2003: 470–471). Skid resistance may be restored
Figure 3.7 Scaling (Miller and Bellinger 2003: 48).
Figure 3.8 Polished aggregate surface (Miller and Bellinger 2003: 49).
by diamond grinding, but with soft aggregates the treatment may have to
be repeated in a few years.
Popouts are “small pieces of pavement broken loose from the surface,
normally ranging in diameter from 25–100 mm (1–4 inches), and depth
from 13–50 mm (1/2–2 inches)” (Miller and Bellinger 2003: 50). Popouts
may be caused by “expansive, nondurable, or unsound aggregates or by
freeze and thaw action” (Huang 2004: 387). Popouts and D-cracking are
caused by similar mechanisms (Mindess et al. 2003: 503).
Blowups are “localized upward movement of the pavement surface at trans-
verse joints or cracks, often accompanied by shattering of the concrete in
that area” (Miller and Bellinger 2003: 52). Blowups are buckling failures
due to compressive stresses in the concrete pavement. They may occur
in hot weather if a transverse joint or crack does not allow expansion,
typically when joints have been allowed to become full of incompressible
material. They may also occur at utility cut patches and drainage inlets, or
if D-cracking has weakened the concrete at the joint (Huang 2004: 376).
A blowup is shown in Figure 3.9.
The most common way of preventing blowups is by maintaining joints so
(Yoder and Witczak 1975: 640). Expansion joints may be used at bridges,
and isolation joints may be used at utility cut patches and drainage inlets.
Under most conditions, properly designed, constructed, and maintained
transverse joints will allow enough movement to prevent blowups. This is
because the slab contraction due to drying shrinkage will generally be more
than enough to overcome any subsequent thermal expansion. Exceptions
may occur if pavements are constructed in cold weather, with very high
temperatures over the following summers. Blowups may also occur with
excessively long joint spacing, as with JRCP, because the joint movement
is directly proportional to the slab length.
Faulting of transverse joints and cracks
Faulting is defined as a “difference in elevation across a joint or crack”
(Miller and Bellinger 2003: 53). It represents a failure of the load-transfer
Figure 3.9 Blowup (Miller and Bellinger 2003: 52).
Figure 3.10 Faulted transverse joint (photo by author).
system. Faults have a considerable effect on ride and are particularly objec-
tionable to the traveling public. Figure 3.10 shows a faulted transverse
crack. Faulting is difficult to capture in a photograph, but is readily noted
by the traveling public.
Faulting is most likely for pavements with aggregate interlock joints, or at
mid-slab cracks in JPCP. Generally, the approach slab (upstream in traffic)
will be higher than the leave slab (Yoder and Witczak 1975: 641). As traffic
moves across the joint it imposes impact loads on the leave slab, forcing
loose materials from under the leave slab to under the approach slab. This
phenomenon is termed pumping (Huang 2004: 380).
Dowels of adequate size are effective for preventing faulting. If dowels
are too small, high bearing stresses on the concrete may cause the dowels
to wear away the opening and become loose. The light steel used in JRCP
may not be enough to prevent faulting of mid-slab cracks. However, there
is generally enough steel in CRCP to prevent faulting of the narrow, closely
spaced transverse cracks.
Other important factors that affect faulting are drainage, the quality of
the subbase or subgrade materials, and the joint spacing. Pumping requires
moisture. Certain unstabilized materials under the pavement are also more
susceptible to pumping. If the subgrade material is poor, the use of a higher
quality subbase material may help prevent pumping. Longer joint spacings
lead to more joint movement, and make it more difficult to maintain load
Traditionally, aggregate interlock joints have been used for JPCP where
vehicle weights or speeds are low. If aggregate interlock joints are used,
faulting will be reduced if joint spacing is reduced and if larger size and/or
harder coarse aggregates are used in the concrete.
Khazanovich et al. (1998: 182–184) found that JPC pavements in wet-
freeze climates are more susceptible to faulting, particularly with fine-
grained soil subgrades. Placing a thick granular layer beneath the subbase
may improve drainage and reduce faulting, particularly for undoweled pave-
ments. Wider slabs also reduce corner deflections and reduce faulting by
about 50 percent. Increasing slab thickness alone will not solve joint faulting
Lane-to-shoulder dropoff is a “difference in elevation between the edge of
slab and outside shoulder; [and] typically occurs when the outside shoulder
settles” (Miller and Bellinger 2003: 54). Dropoff is unlikely to occur if
concrete shoulders are used and are connected to the mainline pavement by
tie bars. However, concrete pavements may also have asphalt, granular or
soil shoulders. These shoulder types can undergo consolidation, settlement,
or pumping of underlying soils. They may also have heave, due to frost
action or swelling soils, as well as dropoff (Huang 2004: 371). Dropoffs
and heaving represent a safety hazard for vehicles that have to go onto the
shoulder, and may be corrected by maintaining or replacing the shoulders.
Lane-to-shoulder separation is “widening of the joint between the edge of
the slab and the shoulder” (Miller and Bellinger 2003: 55). It should not
be considered a distress if the joint is sealed well enough to keep water out
(Huang 2004: 387). Causes are similar to those of lane-to-shoulder dropoff.
The most common remedy is to seal the separation as a joint.
Patch deterioration refers to “a portion, greater than 0 1 m2
all of the original concrete slab that has been removed and replaced, or
additional material applied to the pavement after original construction”
(Miller and Bellinger 2003: 56). Patch deterioration may be caused by
traffic, poor materials, or poor construction practices (Huang 2004: 387).
Proper patching procedures are discussed in Chapter 16. It is usually easier
and cheaper to build the pavement properly in the first place, rather than
to resort to premature patching.
Water bleeding and pumping
Water bleeding and pumping is “seeping or ejection of water from beneath
the pavement through cracks. In some cases, detectable by deposits of fine
material left on the pavement surface, which were eroded (pumped) from
the support layers and have stained the surface” (Miller and Bellinger 2003:
58). Water bleeding and pumping may occur at joints, cracks, and pavement
edges. Figure 3.11 illustrates water bleeding and pumping.
Yoder and Witczak (1975: 341) provide an excellent discussion of pump-
ing. Active pumping is most pronounced directly after rainfall, and was first
noticed when pavements were built directly on plastic clay soils. Compres-
sion of the soil under traffic opens up a void space under the pavement,
which collects water. This water, combined with a pumpable material such
as a high plasticity clay, is then forced out under traffic loading. This
process may be gradual and not noticed until years after construction.
The muddy water ejected often causes telltale staining on the pavement
Huang (2004: 12) notes that for pumping to take place, the material
under the concrete slab must be saturated, there must be frequent heavy
wheel loads, and the material under the slab must be erodible. If wheel
loads are light, slow moving, or infrequent, pumping may never become a
problem even with wet erodible materials. However, for highways and other
high volume, high speed pavements, proper drainage should be provided.
It may also be necessary to stabilize the soil or subbase under the slab.
Figure 3.11 Water bleeding and pumping (Miller and Bellinger 2003: 58).
Punchouts, which only occur with CRCP, are rectangular chunks of con-
crete broken loose and punched down below the surface of the adjacent
pavement. The LTPP distress manual description for punchout is “the area
enclosed by two closely spaced (usually <0 6 m [2 foot]) transverse cracks,
a short longitudinal crack, and the edge of the pavement or a longitudinal
joint. Also includes “Y” cracks that exhibit spalling, breakup, or faulting”
(Miller and Bellinger 2003: 78). Punchouts generally occur at pavement
edges. Figure 3.12 shows a high severity punchout.
Punchouts are the key structural distress for CRCP. They start with a
loss of aggregate interlock at two of the closely spaced transverse cracks.
The portion between the cracks then begins to flex as a cantilever beam
until a fatigue crack forms. The cracks break down under repeated loading,
the steel ruptures, and pieces of concrete punch down into the subbase and
subgrade (Huang 2004: 384–385).
CRCP generally has an excellent performance history where punchouts
have been prevented. However, if they occur, punchouts are difficult to
repair properly. Full depth repair of punchouts is discussed in Chapter 17.
Punchouts may be avoided by designing reinforcement so that transverse
cracks are fine enough and far apart enough to stop aggregate interlock
break-down. Khazanovich et al. (1998: 189–190) found that punchout
Figure 3.12 High severity punchout (Miller and Bellinger 2003: 79).
distress was reduced with higher steel percentages and cement-treated sub-
bases as opposed to asphalt-treated or granular subbases.
Transverse construction joint deterioration
Transverse construction joint deterioration is a “series of closely spaced
transverse cracks or a large number of interconnecting cracks occurring
near the construction joint” (Miller and Bellinger 2003: 73). It is a “break-
down of the concrete or steel at a CRCP construction joint primary
causes are poorly consolidated concrete and inadequate steel content
and placement” (Huang 2004: 388).
The traveling public – the pavement users – are most concerned about
the pavement surface conditions. The surface conditions are initially “built
in” to the pavement during construction, but change over time, generally
for the worse. The various distresses discussed above often degrade the
pavement surface condition. It is also useful to discuss the contributions of
the pavement microtexture and macrotexture to the surface characteristics.
Traditionally, smoothness has been expressed in terms of serviceability,
which is “the ability of a specific section of pavement to serve traffic in
its existing condition” (Huang 2004: 389). The concept of serviceability
was developed by Carey and Irick at the AASHO Road Test. Initially,
a present serviceability rating from 0 to 5 (very poor to very good) was
used by a panel of raters riding in a vehicle over the pavement. These
ratings were correlated to objective measurements of pavement condition
to develop a regression equation for present serviceability index (PSI). For
rigid pavements, the regression equation used slope variance (a summary
statistic for wheelpath roughness) and the sum of cracking and patching.
Slope variance was found to be the dominant variable (Yoder and Witczak
1975: 648–653, Huang 2004: 389–398).
The World Bank developed the international roughness index (IRI) as a
quantitative measure of smoothness. According to Huang (2004: 399):
The IRI summarizes the longitudinal surface profile in the wheelpath
and is computed from surface elevation data collected by either a topo-
graphic survey or a mechanical profilometer. It is defined by the average
rectified slope (ARS), which is a ratio of the accumulated suspension
motion to the distance traveled obtained from a mathematical model
of a standard quarter car transversing a measured profile at a speed of
50 mph (80 km/h). It is expressed in units of inches per mile (m/km).
In other words, IRI is a not a direct measure of pavement roughness,
but a measure of vehicle response to that roughness. General methods for
measuring IRI are specified by ASTM E1170 (ASTM E1170 2001).
Agencies have used several types of devices for measuring pavement
smoothness. These range from simple straightedges to high-speed, iner-
tial profilers equipped with laser sensors to record elevation measure-
ments (Grogg and Smith 2002: 3). Smoothness measurements are often
taken immediately after construction, to determine whether the pavement
is acceptable and whether the contractor should be assessed penalties or
awarded bonuses. It is also necessary to have devices capable of travel-
ing at highway speeds to monitor network roughness conditions for asset
Profilographs consist of a rigid beam or frame with a system of support
wheels that serve to establish a datum from which deviations can be mea-
sured using a “profile” wheel located at the center of the unit (Woodstrom
1990). The two basic models used are the California and Rainhart profilo-
graphs. Profilographs are used exclusively for construction quality control
and are light enough to be used to measure pavements 1 day after paving
(Grogg and Smith 2002: 3–4).
Response-type road roughness measuring systems (RTRRMS) measure
the dynamic response of a mechanical device. Common devices include the
Mays ridemeter, the Bureau of Public Roads (BPR) roughometer, and the
PCA ridemeter. They are used mainly for network assessment of existing
pavements (Grogg and Smith 2002: 4–6).
Inertial road profiling systems (IRPS) are high-speed devices using non-
contact sensors (ultrasonic, laser, infrared, or optical) to measure relative
displacement between the vehicle frame and the road surface. Due to their
accuracy and rapidity, they have largely supplanted RTRRMS for network
assessment. Traditionally, these vehicles were too heavy to drive onto freshly
constructed pavement. Recently, however, lightweight (golf cart or all ter-
rain vehicle type) profilers have been developed that can drive on day-old
concrete pavement with speeds up to 32 kph (20 mph) (Grogg and Smith
The profile index, or PI, has traditionally been used for quality control
of new pavements, with the IRI used for network monitoring. The PI is
computed from a profilograph trace of the pavement surface, using manual
or computer techniques. It is the sum of all individual high and low values
exceeding a predetermined value. The predetermined value is termed the
blanking band and has historically been 5 mm (0.2 in) for the California
profilograph, although some agencies omit the blanking band. Due to the
limited span of the profilograph, wavelengths over 15 m (50 ft) cannot be
captured, even though those affect ride quality. Because correlation between
PI and IRI has been found to be poor, some highway agencies have adopted
IRI for construction acceptance testing (Grogg and Smith 2002: 7). The
ACPA Technical Bulletin TB–006.0-C (ACPA 1990a) provides an example
of a profilograph trace and PI computation.
One of the best ways to provide a smooth pavement over the entire
service life is to build it smooth in the first place. Khazanovich et al. (1998:
183–184) found a strong correlation between initial IRI and IRI over time.
A good working platform, such as a stabilized subbase, makes it easier
to build a smoother pavement. For JPCP, joint faulting is an important
contributor to roughness – joints with 38 mm (1½ in) dowels have very
little faulting. For CRCP, using higher steel percentages lowered IRI and
prevented localized failures.
Pavement skid resistance is important for safety. Skid resistance is neces-
sary to allow vehicles to stop safely and avoid crashes, particularly in wet
weather. For a concrete pavement, the skid resistance depends on the tex-
ture provided when the pavement is built as well as subsequent wear due
to vehicle tires.
Texture affects both noise and friction characteristics; these properties
must be considered together It is also imperative that texture/friction
be specifically addressed to reduce the currently unacceptable level of
almost 43,000 fatalities and 3 million injuries annually in highway
crashes and to minimize the resultant traffic delays. It has been esti-
mated that poor pavement conditions currently contribute to 13,000
deaths annually. A small but significant portion of the poor pavement
condition is due to poor surface texture or friction characteristics.
(Larson et al. 2005: 506)
One important issue identified by Larson et al. (2005) is the durability of
the surface – the ability to retain favorable friction characteristics over time.
If the surface becomes polished and loses skid resistance, the texture may be
restored through diamond grinding or grooving as discussed in Chapter 17.
On occasion, new concrete pavements are diamond ground to meet
smoothness specifications. Because only the high spots are ground, the pave-
ment surface may become a mixture of ground and unground surfaces.
“Spot grinding to remove bumps can result in differential friction qualities
and can also result in non-uniform appearance” (Larson et al. 2005: 503).
Kohn and Tayabji (2003: 79) note there are two primary functions of sur-
face texture. The first is to provide paths for water to escape from beneath
the tires of aircraft or other vehicles. The second is to provide enough
sharpness for the tire to break through the residual film remaining after the
bulk water has escaped. Huang (2002: 401) lists some factors that affect
skid crashes, including polishing of the pavement surface and inadequate
cross-slope drainage which allows water to pond on the pavement surface.
Skid resistance is defined using the skid number (abbreviated SK or SN).
It is 100 times the kinetic or sliding coefficient of friction measured using
a locked-wheel trailer of known weight with standardized tires, riding on
wet pavement. Devices for measuring SN include the locked-wheel trailer,
Yaw mode trailer, and British Portable Tester. Locked-wheel trailers are
the most commonly used devices (Garber and Hoel 2002: 1081).
Research results indicate that up to 70 percent of wet weather crashes
could be prevented with improved texture/friction. Given that wet
weather crashes represent about 14 percent of the total fatal crashes,
this potential could result in a 10 percent total reduction in fatal
and serious injury crashes and also could significantly reduce travel
delays However, a little recognized fact is that 80 to 86 percent of
total fatal crashes occur on dry roadways. In the past, most of the
emphasis has been on wet weather crashes, with the friction (or macro-
texture) on dry roadways often assumed to be adequate To provide
safer roads, the effect of increasing texture/friction on reducing crashes
on both wet and dry roadways must be considered.
(Larson et al. 2005: 510)
Locked-wheel trailer testing is performed according to ASTM E274 (ASTM
E274 2006). The test is performed at 64 kph (40 mph) with water applied
in front of the test wheel. The trailer wheels are then locked and the friction
force generated by the trailer is measured. SN decreases with increasing
vehicle speed (Huang 2004: 402–403).
Karamihas and Cable (2004: 16) point out that ASTM E274 may be
carried out with two types of standard test tires, ribbed or smooth. The
two types of tires may rank skid resistance of roads differently, because
ribbed tires provide channels for water to escape. Therefore, using ribbed
tires may put pavements with good surface drainage at a disadvantage.
Surface texture is attained during construction by dragging various mate-
rials or tools across the fresh concrete. This process builds undulations or
grooves into the surface before the concrete hardens. The spacing, width
and depth of the grooves affect surface friction, skid resistance and tire/road
noise. The purpose of a surface texture is to reduce wet-weather accidents
caused by skidding and hydroplaning.
The different surface types produced during construction include drags
and tining. Drag textures result from dragging brooms, artificial turf, or
burlap across the fresh concrete surface. Tined surfaces are produced with
metal rakes, and may be either longitudinal or transverse to the pavement
centerline. These are illustrated in Chapter 15. Concrete pavement sur-
face textures are discussed in Concrete Pavement Surface Textures, Special
Report SR902P (ACPA 2000b).
Exposed aggregate is used mainly in Europe, and consists of applying a set
retarder to the new concrete surface, and then washing away surface mortar
to expose durable chip-size aggregates. This process requires uniformly
applying chips to fresh surface and washing away the still-wet mortar. This
technique may be used to improve the appearance of city streets.
Hardened concrete may also be textured, either to improve a newly
constructed pavement that is not acceptable or will not earn the contractor
a bonus, or to rehabilitate an existing pavement with inadequate surface
characteristics. The surface may be diamond ground, diamond grooved, or
abraded with steel shot (shot blasting). These techniques are discussed in
The interaction between pavement texture and vehicle tires produces noise
both inside and outside of the vehicle. If the noise is exceptionally loud or
high pitched, it will be objectionable to drivers and/or citizens living next
to the highway. Noise is becoming an issue of increasing importance in
concrete pavement engineering. Hanson and Waller (2005: iv) state that
“Noise is the generation of sounds that are unwanted traffic noise can
be considered an environmental pollution because it lowers the standard of
Two key studies on texturing and noise are NCHRP Synthesis 268
(Wayson 1998) and a comprehensive multistate study by Kuemmel et al.
(2000). These and other reports and technical papers may be found on
the website of the International Grooving & Grinding Association at
NCHRP Synthesis 268 (Wayson 1998: 1) found that, for concrete pave-
Transverse tining causes the greatest sideline (roadside) noise levels
and may lead to irritating pure tone noise. Randomized spacing and
changing the tine width have been found to reduce the pure tone that is
generated and reduce overall noise levels. Texture depth of transverse
tining also seems to play an important role in sideline noise levels
• Studies show that sound generation varies with speed. The pave-
ment with the best results for noise may be different with varying
speeds. In addition, the most quiet pavement surface was found to
be different for automobiles than for trucks.
• Construction quality is an important consideration in the final
overall noise generation no matter which pavement type/texture is
• Texture depth of the transverse tining also seems to play an impor-
• The use of porous PCC pavement also results in a noise reduction
along the highway. This surface may provide noise attenuation
while also being more durable than asphaltic surfaces.
(Wayson 1998: 38–39)
Wayson (1998: 70) concludes that concrete pavements are more durable
and provide better skid resistance than asphalt pavements, but generate
Kuemmel et al. (2000) carried out an extensive study with 57 test sites
in six different US states. This included a number of new test sections
constructed in Wisconsin in 1997. The report (Kuemmel et al. 2000: 2–3)
• Tining depths vary tremendously among the pavements con-
structed, even within a single test section. This was found to be the
case throughout the states analyzed. In many cases, depths specified
by the highway agencies were not achieved.
• Uniform tined pavements exhibit discrete frequencies (a whine) and
should be avoided.
• For all transverse tined pavements, those with the widest and deep-
est textures were often among the noisiest.
• Longitudinal tined PCC pavements and an AC pavement exhibited
the lowest exterior noise while still providing adequate texture. The
performance of longitudinal tining in wet weather has not been
documented in any recent accident study.
• One AC pavement, and the longitudinally tined and random skew
tined (1:6 skewed) PCC pavements exhibit the lowest interior noise
while providing adequate texture. The random skewed can be easily
built and eliminates discrete frequencies.
• Random transverse tining can significantly reduce discrete frequen-
cies, but may still exhibit some discrete frequencies unless carefully
designed and constructed, and will not substantially reduce overall
• Diamond ground PCC pavements exhibited no discrete frequencies
and lower exterior noise levels (compared to random transverse)
approximately 3 dB.
These investigators documented the noise reductions of various concrete
pavement treatments over uniform transverse tining. They also recom-
mended improving quality control of macrotexture, and research to doc-
ument the amount of macrotexture necessary for satisfactory wet weather
performance of pavements. If noise considerations are paramount, longitu-
dinal tining with 19 mm (3/4 in) spacing may reduce noise while providing
adequate safety. Other treatments with potential include 1:6 skew or ran-
dom transverse tining, or diamond grinding (Kuemmel et al. 2000: 3–4).
Karamihas and Cable (2004: 2) note that “quiet pavement should never
be provided at the expense of safety. As such, the challenge is to provide
quiet pavement with sufficient drainage and without any reduction in fric-
tion.” They also found that transverse tining usually causes more noise
than random textures. A high-pitched whine may be produced by trans-
verse tining with constant spacing. There remains a problem of lack of
standardization of pavement noise measurements (Karamihas and Cable
Hanson and Waller (2005: 11) reported that, among concrete pavements,
diamond ground pavements were the quietest, followed by longitudinally
tined, longitudinally grooved, and transverse tined. All were noisier than
asphalt pavements. This was based on 300 test sections across the United
States Although diamond ground pavements were quieter, they also had
the highest variability of noise measurements, probably because grinding
does not affect low spots in the pavement. In Minnesota, a turf/broom drag
produced low noise levels that were comparable to asphalt (Hanson and
Waller 2005: 19–20).
Despite the fact that all of these sources are in agreement that concrete
pavements start with better skid resistance and maintain it longer than
asphalt pavements, the noise issue will remain a difficult challenge for
the concrete paving industry. While virtually all drivers and passengers
experience the noise differences while traveling on different pavements, only
an unfortunate minority will ever experience the differences in the locked-
wheel skid resistance of different types of pavements. Furthermore, some
of those who find the skid resistance to be inadequate will not be around
to testify on the issue. Therefore, more research into noise reduction for
concrete pavements is necessary.
Subgrades, subbases, and
Pavement performance is strongly influenced by the underlying soil layers,
particularly with respect to stability, bearing strength, consolidation over
time, and moisture susceptibility. Frequently one or more layers are placed
between the soil subgrade and the pavement.
In flexible or asphalt pavements, the layer directly under the pavement
is the base and the layer between the base and the subgrade is termed the
subbase. Base course materials have to meet tighter quality specifications
than subbase materials. Since subbase quality materials may be used directly
under a concrete pavement, this layer is typically termed the subbase. This
is the terminology used in the 1993 AASHTO Design Guide (AASHTO
Concrete pavements distribute loads much more widely than asphalt
pavements, and the pressures on the subbase and subgrade are low. As a
result, the bearing capacity of the underlying layers is less critical, and there
is no need to use stiff base materials except for pavements carrying the
In the literature, however, both terms, base and subbase, have been used
to describe the layer under a concrete pavement. It is rare for concrete
highway pavements to have both a base and a subbase layer. In contrast,
airfield pavements that handle heavy wide-body aircraft often have both a
base and a subbase (Kohn and Tayabji 2003: 41).
These layers may be unstabilized, or stabilized with portland or asphalt
cement. They may also be densely graded and relatively impermeable,
or deliberately gap graded to provide drainage. The PCA/ACPA publica-
tion Subgrades and Subbases for Concrete Pavements addresses selection
and construction of these layers (PCA/ACPA 1991). Another publica-
tion that discusses subbases and bases, specifically for airfields, is Design
and Construction Guide for Stabilized and Drainable Bases (Hall et al.
70 Subgrades, subbases, and drainage
Careful attention to the design and construction of subgrades and sub-
bases is essential to ensure the structural capacity and ride quality of
all types of pavements. For concrete pavements, the requirements may
vary considerably depending on subgrade soil type, environmental con-
ditions, and amount of heavy truck traffic. In any case, the objective
is to obtain a condition of uniform support for the pavement that will
prevail throughout its service life.
(PCA/ACPA 1991: 1)
As an example, a parking lot carrying only light vehicle traffic would
usually be built directly on the compacted subgrade. A subbase would
be used only to deal with unsuitable soil (ACI Committee 330 2001:
5). For streets and local roads, subbases are generally not used for res-
idential pavements, but would be used to prevent pumping for collec-
tor and arterial streets and local roads (ACI Committee 325 2002: 7).
For highways, AASHTO recommends the use of a subbase unless the
subgrade soils are equal in quality to subbase materials, or if the pro-
jected traffic is less than one million ESALs (AASHTO 1993: I-21).
ESALs, discussed in Chapter 8, are equivalent single axle loads of 80 kN
Airfield requirements are similar. For pavements serving only general avi-
ation aircraft, a subbase may not be necessary (ACPA 2002: 2). The FAA
requires a subbase under airport pavements with heavier traffic with the
exception of certain soil type, drainage, and frost susceptibility combina-
tions. For heavier aircraft, stabilized subbases which are essentially bases
are required (FAA 2004: 55).
The subgrade is the native roadbed soil at the site and the engineer must
generally work with what is available. If necessary, better materials may
be brought in or the subgrade may be stabilized, but this represents an
Two common soil classification methods are the ASTM or Unified Soil
Classification System (USCS) (ASTM D2487 2000) and the AASHTO clas-
sification system (AASHTO 2005). The AASHTO system is used for high-
ways in the United States, and the ASTM/USCS system is used for other
pavements. Soils are classified by the proportion of the coarse grained
fraction (gravels and sands) and the fine-grained fraction (silts and clays),
as well as the plasticity or response of the fine-grained fraction to mois-
ture. Classification of soil is described by many standard textbooks on
geotechnical or pavement engineering, including Garber and Hoel (2002:
Subgrades, subbases, and drainage 71
For concrete pavement engineering, the important parameters are the
quality of the support provided to the pavement, the moisture suscepti-
bility, and the frost susceptibility. The quality of support is characterized
by the modulus of subgrade reaction k, in units of MPa/m or psi/inch
(sometimes pci or pounds per cubic inch). This modulus represents the
spring constant of an imaginary spring or dense liquid foundation sup-
porting the slab. The subgrade reaction increases linearly with the deflec-
tion of the slab. It may be measured in the field using a plate bearing
test, or predicted from the soil classification or California bearing ratio
One commonly used chart for predicting k was developed by the PCA
(1966). This chart was used by the PCA 1984 method and is reproduced
by Garber and Hoel (2002: 1036) and Huang (2004: 328). It provides
approximate relationships for determining k based on ASTM/USCS soil
classification, AASHTO classification, FAA classification, resistance value
(R), bearing value, and CBR.
Recently Hall et al. (1997: 80) developed a revised k-value chart for
the AASHTO 1998 supplement design procedure. The k-values for dif-
ferent soil types are shown in Table 4.1. The AASHTO 1998 guide also
provides procedures for correlating k-values to CBR and dynamic cone
penetrometer (DCP) data. Charts are provided for fine-grained soils based
on moisture content – essentially linear relationships exist between the
minimum values shown in Table 4.1 at 100 percent saturation and the
maximum values at 50 percent saturation. Procedures are also provided
for finding k through back-calculation of FWD test results (AASHTO
As a practical matter, the design thickness of a concrete pavement is not
very sensitive to the k-value. The moisture susceptibility of the soil has a
much greater effect on pavement performance. Frost action may also be
For heavy duty highway or airport pavements, it is generally necessary to
remove any unsuitable material encountered. Unsuitable subgrade materials
include peat, organic silt, silt, and soil with high organic content (Kohn and
Tayabji 2003: 33).
Subgrades may need to be stabilized to improve low-strength soil,
reduce potential for swelling due to moisture, or to improve con-
struction conditions. If the project is on a tight schedule, stabilization
reduces the risk of construction delays due to wet weather. Subgrades
may be stabilized with lime or cement. Lime stabilization is most suit-
able for clayey soils with high moisture content. Cement stabilization
is used for coarse-grained soils or soils with high silt content. Lime
and cement stabilization are discussed in detail by Kohn and Tayabji
Subgrades, subbases, and drainage 73
Expansive subgrade soils
Excessive differential shrink and swell of expansive soils cause nonuni-
form subgrade support. As a result, concrete pavements may become
distorted enough to impair riding quality. Several conditions can lead
to this pavement distortion and warping:
1. If expansive soils are compacted when too dry or are allowed to dry
out prior to paving, subsequent expansion may cause high joints
and loss of crown.
2. When concrete pavements are placed on expansive soils with widely
varying moisture contents, subsequent shrink and swell may cause
bumps, depressions, or waves in the pavement.
3. Similar waves may occur where there are abrupt changes in the
volume-change capacities of subgrade soils.
(PCA/ACPA 1991: 3)
It is obviously important to identify potentially expansive soils before con-
struction. As a general rule, soils with high colloid content (percent of grains
be expected to expand the most. These are generally classified as CH, MH,
or OH by the ASTM classification method or A-6 or A-7 by the AASHTO
method. Concrete pavements can often tolerate clays with medium or low
degrees of expansion. The actual amount of expansion depends on the cli-
mate, the load conditions from the pavement layers above the subgrade,
and the moisture and density conditions at the time of paving (PCA/ACPA
1991: 3–4). Therefore, careful construction is important for control
of expansive soils. Construction considerations are discussed in Chapter 13.
Frost-susceptible subgrade soils
“For pavement design purposes, frost action can be evaluated by the effects
of (1) frost heave and (2) subgrade softening on spring thawing. Design
considerations for controlling frost heave are not necessarily identical to
those for controlling subgrade softening” (PCA/ACPA 1991: 7). Subgrade
softening is generally very damaging for asphalt pavements, but less dam-
aging for concrete pavements because they can bridge over soft soils during
the spring thaw period. The following material has been adapted from
PCA/ACPA Subgrades and Subbases for Concrete Pavements (1991: 7–8).
Frost heave is caused by the growth of ice lenses in the soil. Water moves
by capillary action through soil to ice crystals initially formed, and then
freezes. With enough available water, the crystals continue to grow and
form thick lenses that lift or heave the pavement. Frost action requires frost-
susceptible soil, freezing temperatures that penetrate the subgrade, and a
supply of water, usually with a water table within about 3 m (10 ft) of the
surface. All three must be present for frost action to occur.
74 Subgrades, subbases, and drainage
Frost-susceptible soils are often defined as having more than 3 percent of
particles smaller than 0.02 mm (0.0008 in). Low plasticity, fine-grained soils
with high silt content (0.05–0.005 mm, 0.002–0.0002 in) are particularly
susceptible to frost heave. Pore sizes must be small enough to develop
capillary action, but large enough to allow water to flow to form the lenses.
“Low plasticity silts are most susceptible to frost heave, followed by loams
and very fine sands, sandy loams, clay loams, and clays in decreasing order”
(PCA/ACPA 1991: 8).
FAA design procedures address the design of pavements for frost and
permafrost in detail in Chapters 2 and 3 of FAA document Pavement
Design, Advisory Circular (AC) 150/6320-6D (FAA 2004). This topic is
discussed in more detail in Chapter 10 of this book. Methods of dealing
with frost heave are discussed in Chapter 13.
In addition to the dramatic effect of moisture on the k-value of fine-
grained soils, moisture in soils also leads to pumping and the formation of
ice lenses. This risk can be reduced through the use of subbases.
Subbases and bases
The AASHTO Guide for Design of Pavement Structures (AASHTO 1993:
I-21) defines a subbase as “one or more compacted layers of granular or
stabilized material” between the subgrade and concrete pavement slab. The
Guide cites the following reasons for using subbases:
• “to provide uniform, stable, and permanent support,
• to increase the modulus of subgrade reaction k,
• to minimize the damaging effects of frost action,
• to prevent pumping of fine-grained soils at joints, cracks, and edges of
the rigid slab, and
• to provide a working platform for construction equipment.”
As noted previously, the Guide further states that a subbase is not necessary
if the traffic is relatively light (less than one million ESALs) and the roadbed
soil quality is equal to that of a subbase. Use of a subbase solely to increase
the k is not economical, in the absence of the other reasons (PCA 1984: 6).
As a practical matter, the last reason cited in the previous list may be the
strongest, because it helps avoid construction delays due to wet weather
and helps the contractor build a smoother pavement.
A key consideration is whether the subbase is expected to also func-
tion as subdrainage. Conventional subbases are densely graded and com-
pacted granular materials, and materials stabilized with suitable admixtures.
AASHTO soil classes A-1, A-2-4, A-2-5, and A-3 granular materials may
need to be treated with portland cement to make cement-treated subbases
(PCA 1984: 6).
Subgrades, subbases, and drainage 75
Use of a subbase will increase the k-value over that provided by the
subgrade soil. The PCA developed a chart to calculate the increase in k-value
due to aggregate (Table 4.2) and cement-treated subbase (Table 4.3) (PCA
The FAA has developed similar charts. For well-graded aggregate, results
are similar to Table 4.2. The k-values for bank run sand and gravel are
lower and are shown in Table 4.4. Values for all types of stabilized subbases
are provided in Table 4.5 (FAA 2004: 55–56).
The AASHTO Guide for Design of Pavement Structures (AASHTO 1993)
uses a more elaborate procedure to adjust the k-value upward based on
the subbase modulus and thickness, and possibly on a rigid foundation or
rock 3 m (10 ft) below the surface, adjust for seasonal effects, and then
adjust it downward based on the loss of support factor due to foundation
erosion or differential soil movements. That degree of refinement may not
be necessary, based on the limited importance of k-value to design and
Table 4.2 Effect of untreated subbases on k-values (PCA 1984: 6)
Subbase k-value, MPa/m (psi/in)Subgrade
(psi/in) 100 mm (4 in) 150 mm (6 in) 225 mm (9 in) 300 mm (12 in)
13.5 (50) 17.5 (65) 20 (75) 23 (85) 30 (110)
27 (100) 35 (130) 38 (140) 43 (160) 51 (190)
54 (200) 60 (220) 62 (230) 73 (270) 87 (320)
81 (300) 87 (320) 89 (330) 100 (370) 117 (430)
Table 4.3 Effect of cement-treated subbases on k-values (PCA 1984: 6)
Subbase k-value, MPa/m (psi/in)Subgrade
(psi/in) 100 mm (4 in) 150 mm (6 in) 225 mm (9 in) 300 mm (12 in)
13.5 (50) 46 (170) 62 (230) 84 (310) 107 (390)
27 (100) 76 (280) 108 (400) 141 (520) 173 (640)
54 (200) 127 (470) 173 (640) 218 (830) −
Table 4.4 Effect of untreated subbases on k-values (FAA 2004: 15)
Subbase k-value, MPa/m (psi/in)Subgrade k-value,
100 mm (4 in) 150 mm (6 in) 225 mm (9 in) 300 mm (12 in)
13.5 (50) 16.2 (60) 19 (70) 23 (85) 28 (105)
27 (100) 34 (125) 38 (140) 43 (160) 51 (190)
54 (200) 62 (230) 68 (250) 73 (270) 81 (300)
81 (300) 84 (310) 87 (320) 92 (340) 95 (350)
76 Subgrades, subbases, and drainage
Table 4.5 Effect of stabilized subbases on k-values (FAA 2004: 57)
Subbase k-value, MPa/m (psi/in)Subgrade
(psi/in) 100 mm (4 in) 150 mm (6 in) 225 mm (9 in) 300 mm (12 in)
13.5 (50) 23 (85) 30 (110) 46 (170) 60 (220)
27 (100) 46 (170) 62 (230) 73 (270) 87 (320)
54 (200) 76 (280) 84 (310) 100 (370) 107 (390)
81 (300) 95 (350) 103 (380) 113 (420) 116 (430)
given the difficulty of predicting potential erosion. Tables 4.2 and 4.3 are
There is one further comment worth making on k-values, particularly
when stiff cement- or asphalt-treated subbase materials are used. Typically,
in engineering, it is thought that more strength and stiffness is better and
it is conservative to ignore it. Following that philosophy, it would seem to
be conservative to design on the basis of a relatively low k-value regardless
of whether or not better materials were used or better compaction were
achieved in the field.
That approach would be correct for slab thickness design, but not for joint
spacing. As will be shown in Chapter 7, curling stresses increase as k-values
Thus, for determining maximum joint spacing, the k-value must be calculated
correctly or overestimated in order to achieve a conservative design.
For airfield pavements, subbases are made of natural or crushed granular
materials with CBR from 20 to 100. They are used to provide frost protec-
tion or drainage (Kohn and Tayabji 2003: 41). Similar materials are used
for highways, streets, and roads (PCA/ACPA 1991: 12–13).
The FAA Advisory Circular Airport Pavement Design and Evaluation
(FAA 2004) states that “the purpose of a subbase under a rigid pavement
is to provide uniform stable support for the pavement slabs. A minimum
thickness of 4 inches (100 mm) of subbase is required under all rigid pave-
ments, except as shown” in Table 4.6.
New airport pavements, particularly those that carry heavy aircraft with
gross aircraft loads of 45,250 kg (100,000 lb) or more, generally require
stabilized bases (Hall et al. 2005: 1, FAA 2004: 55). Bases used under
airfield pavements may be mechanically or chemically stabilized. Higher
quality materials are required for mechanically stabilized bases than for
subbases, in terms of crushed aggregate content, deleterious material, and
gradation, but they are otherwise similar (Kohn and Tayabji 2003: 42).
Subgrades, subbases, and drainage 77
Table 4.6 Conditions where no subbase is required (FAA 2004:
55, Table 3.10)
Soil classification Good drainage Poor drainage
No frost Frost No frost Frost
GW X X X X
GP X X X
X = no subbase required
Categories of chemically stabilized bases include soil cement, cement-
treated base (CTB), econocrete (lean concrete), and asphalt-treated base
(ATB). Soil cement and CTB are similar, but soil cement uses on-site sub-
grade or fill material while CTB is generally made from processed material
and is of higher quality. It is recommended that these materials be specified
not to exceed a certain maximum strength, or that other measures be taken,
in order to reduce cracking potential.
Mixture proportioning and test methods for soil-cement are discussed in
detail in the PCA publication Soil-Cement Laboratory Handbook, Engi-
neering Bulletin EB052.07S. This handbook covers determining the cor-
rect cement content and testing for freeze-thaw and moisture susceptibility
CTB typically has a seven-day compressive strength of 5.3 MPa (750 psi).
CTB is listed in the FAA document Standards for Specifying Construction of
Airports, AC 150/5370-10B (FAA 2005) as Item P-304 – Cement Treated
Cement treated base course, FAA Item P-304, is designed to have a
minimum seven-day compressive strength of 5,171 kPa (750 psi). In areas
subjected to a large number of freeze-thaw cycles, a durability criterion
may also apply. A bond breaker is recommended between the CTB and the
concrete pavement. The CTB is accepted based on density and smoothness
(Hall et al. 2005: 6).
Econocrete is similar to concrete but is made with marginal quality
materials. A typical minimum seven-day compressive strength is 5.3 MPa
(750 psi) with a 28-day maximum of 8.3 MPa (1,200 psi). The maximum
strength requirement is intended to prevent cracking of the econocrete, and
reduce the risk that these cracks will cause reflective cracks in the con-
crete pavement when it is placed. Base materials may also be treated with
asphalt. Stiff base materials, particularly econocrete, can increase k-value
and curling/warping stresses and therefore decreased joint spacing should
78 Subgrades, subbases, and drainage
be considered (Kohn and Tayabji 2003: 42–46). Econocrete is listed in
the FAA document Standards for Specifying Construction of Airports, AC
150/5370-10B (FAA 2005) as Item P-306 – Econocrete Subbase Course.
Lean concrete base (LCB), or Econocrete, Item P-306, is weaker than
CTB, with seven-and 28-day compressive strength requirements of 3,448
and 5,171 kPa (500 and 750 psi), respectively. To reduce the cracking
risk for the concrete pavement, an upper limit on compressive strength of
8,274 kPa (1,200 psi) may be specified. This limit may be waived if a good
bond breaker is used between the LCB and the concrete pavement. The
minimum cement content is 118 kg/m
, which is considerably
lower than conventional concrete. LCB is accepted based on consistency
(slump) air content, thickness, strength, and grade (Hall et al. 2005: 6–7).
ATB is similar to conventional hot mixed asphalt, and uses the same
FAA specification. ATB may use either Item P-401, which is the same as
conventional hot mix asphalt surface layers, or the newer Item P-403. P-403
was developed specifically for ATB and asphalt leveling courses. Mixture
design, construction, and acceptance are similar to conventional asphalt
pavements (Hall et al. 2005: 7).
Details on materials selection and mix design for CTB, LCB, and ATB
are provided by Hall et al. (2005: 35–42). Recycled, crushed, and graded
concrete may be used as an aggregate for CTB and LCB if it meets speci-
fications. Similarly, recycled asphalt pavement (RAP) may be used as part
Cement-treated subbases and lean concrete subbases are also used under
highway pavements. In many areas of the world, aggregates that meet
specifications for unstabilized subbases are becoming difficult to find. CTB
and lean concrete subbases allow greater use of local materials, substandard
aggregates, and recycled materials, generally saving materials and hauling
costs. CTB generally contains 4–5 percent cement by weight. Lean concrete
subbase has more cement than CTB, but less than conventional concrete
(PCA/ACPA 1991: 14–15).
Hall et al. (2005: 5) note that “a uniform, non-erodible base is preferred
over a high strength base in a rigid pavement system.” The base increases
foundation support and reduces stresses and deflections, and improves joint
load transfer. Therefore, cracking and faulting potential are reduced.
Selection of stabilized subbase/base type
Since CTB, LCB, and ATB may all be used as stabilized subbases or bases
under concrete pavement, it is useful to address the advantages and disad-
vantages of the materials. Hall et al. (2005: 30–32) discusses the relative
merits of these types of layers.
CTB is usually a good choice for a base under rigid airfield pavements.
Advantages include resistance to erosion and pumping, good load transfer
Subgrades, subbases, and drainage 79
efficiency, and improved foundation support (increased k-value). CTB can
generally be constructed quickly (Hall et al. 2005: 30). However, it is
important with CTB to control maximum strength and stiffness and use
bond breakers. Joint spacing may also need to be reduced.
LCB subbases and bases offer similar advantages to CTB, but may be
more cumbersome because they require slipform pavers and a longer curing
period. LCB has a rougher surface than CTB, so bond breakers are impor-
tant. Thickness and stiffness of the layer should be minimized to reduce
cracking risk. LCB may also be notched to control cracking, in a manner
similar to joint sawing in concrete pavement (Hall et al. 2005: 31).
ATB generally works as well as CTB or LCB, but has a much lower
stiffness. Therefore, friction and restraint are reduced, and a bond breaker
is not necessary. The lower stiffness of ATB layer allows it to deflect with
the slab and provide more uniform support. ATB layers are easily placed.
ATB seems to lead to a lower risk of slab cracking than CTB and LCB
layers (Hall et al. 2005: 31).
There are few disadvantages to using ATB layers, but in hot weather it
is important to whitewash the surface, to reduce the temperature before
placing concrete. Using ATB or asphalt-treated permeable base (ATPB)
layers requires mobilization of asphalt paving equipment.
Friction and bond breakers
Concrete slabs expand and contract with temperature and moisture changes.
Some high-strength stabilized base layers have a rough finished texture and
offer considerable frictional restraint to the concrete pavement movement.
This restraint, particularly at early ages when the concrete is weak, can lead
The high stiffness and rough finished texture of high-strength stabi-
lized bases, such as CTB and LCB, offer considerable restraint at the PCC
slab/base interface. Permeable bases, such as cement-treated permeable base
(CTPB), also offer restraint because the concrete penetrates into the open
surface. These factors increase the risk of early cracking in concrete pave-
ments built over these base types (Hall et al. 2005: 16).
Furthermore, bond between a concrete and a stiff base can create a
“composite slab” and problems with joint saw cutting. A normal saw cut
depth of 1/4 to 1/3 of the slab thickness is not deep enough to ensure that
the composite slab cracks at the desired joint location.
In order to prevent these friction and bond problems, it is necessary to
specify a bond breaker between the base/subbase and the concrete pavement.
The most effective bond breaker for CTB, LCB, or CTPB is a thin layer of
choke stone spread over the surface just prior to concrete placement. Choke
stone is uniformly graded, approximately 13–25 mm (1/2–1 in) in size. This
layer breaks bond and also prevents concrete penetration into CTPB and
80 Subgrades, subbases, and drainage
locking. The lower elastic modulus of asphalt generally offers less restraint
than cement-treated layers, so no bond breaker is usually necessary unless
the surface is milled. Milled surfaces may be treated with a single layer of
asphalt emulsion to reduce friction. For cement-based base/subbase layers,
waxed base curing compounds provide a bond breaker as well as helping
to cure the layer. However, these do not always effectively break bond, so
choke stone is preferred (Hall et al. 2005: 26).
For both ATB and ATPB, the black surface can absorb considerable heat
and increase the risk of cracking the concrete slab. Therefore, they should
be whitewashed with a lime-water solution to lower the surface temperature
(Hall et al. 2005: 23).
It is also helpful to limit the strength and stiffness of CTB or LCB layers.
A compressive strength of 2.4 MPa (350 psi) is sufficient to support con-
struction traffic. Minimum compressive strengths of 3.4 MPa (500 psi) and
maximum of 6.8 MPa (1,000 psi) are desirable. Higher strengths are asso-
ciated with increased risks of slab cracking. Although higher strengths have
often been specified to improve freeze-thaw durability, these are generally
not necessary (Hall et al. 2005: 18).
When CTB layers have high cement content and are not adequately
cured, they may develop surface plastic shrinkage cracks. These cracks may
propagate or reflect upward through freshly placed concrete pavement. If
shrinkage cracking is observed, medium to high density geotextile fabric
may be placed over the CTB as a crack relief layer (Hall et al. 2005: 23).
Recognition of the importance of pavement drainage has increased over
the years. In 1975, Yoder and Witczak devoted only a few pages to the
topic in their classic textbook (Yoder and Witczak 1975: 370–371). Later
textbooks devoted entire chapters to the topic (Garber and Hoel 2002:
739–823, Huang 2004: 334–367). Those textbooks cite the same references
and describe the same procedures discussed, as adapted from Mallela et al.
Garber and Hoel (2002: 739) cite two reasons for the importance of pave-
ment drainage. The first is that inadequate drainage often results, over time,
in severe damage to the pavement structure. The second is that standing
water seriously detracts from the safety and the efficiency of the pavement,
with increased risk of hydroplaning and loss of visibility. They note that
there are two sources of water – surface water from precipitation falling on
the pavement in the form of rain or snow, and ground water flowing in the
soil beneath the pavement.
The surface drainage system is comprised of those features that carry
water away from the pavement and right of way. These include transverse
slopes or the crown of the pavement, typically 2 percent for highways.
Subgrades, subbases, and drainage 81
Longitudinal slopes of at least 0.2 percent are also generally provided.
Longitudinal channels or ditches along highways carry away the water that
flows from the pavement surface. In urban areas, curbs and gutters control
runoff (Garber and Hoel 2002: 739–741).
Regardless of the efficiency of the surface drainage system, some water will
get into the pavement. All pavement surfaces, no matter how impermeable,
allow water to enter through joints and cracks, particularly as they age.
Unless the water is able to drain away quickly, it will weaken the pavement
structure and may cause or accelerate damage.
Some pavements make use of permeable base subdrainage layers. They
are generally more costly than conventional subbase layers, and unstabilized
granular materials are less stable than densely graded materials. This is
because in order to provide the desired permeability the fine portion of the
aggregate must be removed (Mallela et al. 2002: 4-2). There is, therefore, a
structural penalty paid when an unstabilized granular drainable base is used.
A densely graded, well-compacted, crushed limestone base is very stable,
but impermeable. In contrast, a uniformly graded, rounded aggregate, such
as pea gravel, is very permeable but highly unstable.
Kohn and Tayabji (2003: 46) note that
A balance between the need for stability and the need for porosity must
be considered in the design with stability taking precedence. The thick-
ness of the drainage layer is typically 100–150 mm (4–6 in). The use of
unstabilized open graded aggregate drainage layer is not recommended
for pavements used by wide bodied aircraft. These layers do not pro-
vide the necessary stability and construction related problems (rutting
due to construction traffic, etc.) are common. If an unstabilized open
graded layer is necessary, it should be placed deeper in the pavement
structure to reduce stresses on the layer.
Hall et al. (2005: 5) note that “a well designed and constructed permeable
base layer rapidly removes water from within the pavement structure. This
leads to a mitigation of PCC durability-related distresses (e.g. D-cracking)
and helps increase resistance to joint faulting.” However, they are not
directly addressed in FAA pavement design procedures. “The structural
contribution of permeable base layers is ignored in the design process since
they are relatively weak” (Hall et al. 2005: 7).
Aggregate drainage layers can provide a permeability of 300–1,500 m/day
(1,000–5,000 ft/day) with a minimum of 300 m/day (1,000 ft/day) typi-
cally recommended for high-type highways. This may be provided by using
ASTM/AASHTO No. 57 or No. 67 gradations (Mallela et al. 2002: 4–13).
82 Subgrades, subbases, and drainage
To compensate for the poor stability of open graded aggregate layers,
small amounts of asphalt or portland cement may be added. Asphalt- or
cement-stabilized bases have only slightly lower permeability than unstabi-
lized bases (Mallela et al. 2002: 4-2), although there is often a higher cost.
Hall et al. (2005: 7–8) discuss the use of stabilized permeable base layers
for concrete airport pavements.
The construction specifications for these layers are typically developed
by modifying existing guide specifications, such as Items P-401 or 402
for ATPB and Item P-304 for CTPB, etc. However, the open-graded
nature of these materials prevents the application of conventional tech-
niques for performing mix designs and specifying their construction.
For example, the ATPB mix designs often are specified on the basis
of a gradation and percent binder content. Permeability—an important
consideration for this base type—is seldom specified or monitored. Fur-
ifications. Acceptance of the mixture is done on the basis of thickness.
As can be noted, considerable empiricism is used to specify and construct
these mixes, some of which is unavoidable until further research is done.
For airfield pavements, which are difficult to drain because of their width
and gentle slopes, permeability values for drainage layers in the range of
150–450 m/day (500–1,500 ft/day) have been found to be adequate in
most situations. This can be achieved with a minimum cement content of
for CTPB and asphalt content of 2–3.5 percent by
mass for ATPB (Hall et al. 2005: 18–19). CTPB is discussed in Cement-
Treated Permeable Base for Heavy-Traffic Concrete Pavements, Informa-
tion Series IS404.01P (ACPA 1994c).
CTPB is open graded, and therefore weaker than stabilized bases. These
layers must be strong enough to withstand construction traffic without
deformation. Due to their inherent weakness, these layers should be used
only when there is a need for drainage (e.g. high rainfall, perched water
table, low permeability subgrade soils, heavy traffic). If designed and built
properly, CTPB layers can improve the long-term performance of pavements
by reducing moisture-related distress (Hall et al. 2005: 32). CTPB layers
have some of the same problems as CTB and LCB, and concrete paste can
penetrate into the open surface structure and create bond. Segregation may
also occur during placement.
ATPB layers have similar advantages as CTPB for pavements, but they
are generally weaker (less stiff). Due to the lower stiffness, interface restrain
is less of an issue and bond breakers are not necessary. “Significant concerns
when using ATPB include the overheating of the base in hot-weather paving
conditions (similar to ATB) and stripping and stability problems” (Hall
et al. 2005: 32).
Subgrades, subbases, and drainage 83
Details on materials selection and mix design for CTPB and ATPB are
provided by Hall et al. (2005: 42–45). Due to the low amount of binder,
the long-term stability of the mixture comes from the aggregate structure.
Therefore, aggregate quality is an important concern, more so for ATPB
than for CTPB.
If the subgrade under the permeable base has fines that are likely to
migrate into and clog the permeable base, it may be necessary to provide a
separator. This may be a granular layer or a geotextile.
Gharaibeh and Darter (2002: 6) note that permeable ATBs and CTBs
have seen limited use with CRCP, because the rough surface texture leads
to bonding and a composite pavement layer and reduces the effective steel
percentage. A geotextile may be used to prevent bond. Unstabilized drainage
layers do not present this problem.
Khazanovich et al. (1998: 184) found that JPCP with better subdrainage
had lower joint faulting and overall lower roughness. The effect was
stronger with non-doweled JPCP.
Subdrainage design software
The US FHWA has developed a computer program, DRIP 2.0, which
may be used to design pavement subdrainage and side drains. DRIP
stands for drainage requirements in pavements. This program, along
with its user manual, may be downloaded free from the FHWA web-
site: http://www.fhwa.dot.gov/pavement/software.cfm. The program may
be used with either SI or US customary units. Chapter 4 of the user manual
provides the technical background for the program as well as a useful and
thorough review of the topic (Mallela et al. 2002: 4-1–4-29).
The DRIP 2.0 user manual (Mallela et al. 2002: 4-1) outlines the major
steps in the design of subdrainage and side drains as:
1 quantifying water inflow;
2 designing the permeable base;
3 designing the separation layer;
4 quantifying flow to edge-drains;
5 computing outlet spacing;
6 checking outlet flow.
The first three items refer to the design of the permeable base, and the latter
three to the side drains.
Quantifying water inflow
Water inflow into the subdrainage system is due to surface infiltration,
water flow from high ground, groundwater seepage, and meltwater from
84 Subgrades, subbases, and drainage
ice lenses. Generally, infiltration is the single largest source of water flowing
into pavements (Mallela et al. 2002: 4–6). Water flowing from high ground
may be collected and carried off using intercepting drains to keep it away
from the pavement structure (Garber and Hoel 2002: 743–744). A pavement
subsurface drainage system is probably not an efficient way to deal with
groundwater, and the designer should seek assistance from geotechnical
specialists (Mallela et al. 2002: 4–8). Procedures for estimating meltwater
were developed by Moulton (1980) and are reviewed by Mallela et al.
(2002: 4-6–4-7). Meltwater inflow quantities may be calculated using the
DRIP 2.0 computer program.
Infiltration occurs through cracks and joints in the pavement surface.
Uncracked concrete is practically impermeable (Mallela et al. 2002: 4–5).
Two methods may be used to estimate infiltration – the infiltration ratio
method, developed by Cedergren et al. (1973), and the crack infiltration
method, developed by Ridgeway (1976). Although the DRIP 2.0 software
allows for calculations with both methods, the crack infiltration method is
recommended (Garber and Hoel 2002: 807, Mallela et al. 2002: 4-8–4-9).
The design infiltration rate in cubic meters of water per day per square
meter of pavement (cubic feet per day per square foot) is
qi = Ic
where Ic = crack infiltration rate, or the water-carrying capac-
ity of a crack or joint, suggested by Ridgeway (1976) as
0 223 m3
2 4 ft3
Nc = number of contributing longitudinal cracks or joints,
W = width of permeable base in m (ft),
Wc = length of contributing transverse cracks in m (ft), generally equal to
the width of the paved surface,
Cs = spacing of transverse cracks or joints in m (ft), and
Kp = rate of infiltration through the uncracked pavement in
, which is generally very low and may be assumed
to be zero or estimated from laboratory tests (Garber and Hoel 2002: 808).
For JPCP, the slabs should be designed to remain uncracked, so that the
joint spacing should be used for Cs. JRCP is likely to crack between joints,
so a Cs of 4.5–6 m (15–20 ft) is reasonable. For CRCP, it is conservative
to use the standard transverse crack spacing of 0.6–2 m (2–6 ft) for Cs, but
due to the smaller crack width it might also be reasonable to reduce the
crack infiltration rate Ic.
Designing the permeable base
The rapidity of water removal from a permeable base depends on the length
of the path that the water must travel and on the permeability of the base.
Subgrades, subbases, and drainage 85
Mallela et al. (2002: 4-2) provide an equation for computing the resultant
slope, SR, from the longitudinal slope and cross-slope
SR = S2 +S2
where S and Sx are the longitudinal and cross-slope, respectively, in m/m
(ft/ft). The resultant slope, SR, determined from equation 4.2 is then used to
compute the resultant length of the flow path through the permeable base
resultant slope, LR, in m (ft):
LR = W 1+
The permeability of the base material, expressed as a coefficient of per-
meability K, depends on the type of material and the degree to which it
is compacted. Generally, a small k is used as a symbol for permeability,
but in this text a capital K is used to avoid confusion with the modulus of
subgrade reaction. The key material characteristics are the effective grain
size D10 (corresponding to the 10 percent passing grain size), the porosity
n, and the percentage of fines passing the 0.075 mm sieve (No. 200 or 200
spaces per inch) (Mallela et al. 2002: 4-2).
Methods for calculating permeability are reviewed by Mallela et al. (2002:
4-2–4-5). The coefficient K may be computed using DRIP 2.0 software based
on the grain size distribution of the material, the in-place density or unit
weight in kg/m3
, the specific gravity of the solids, and the effective
porosity. The effective porosity may be determined from a simple test to
find the volume of water draining from a known volume of material, or
estimated based on the percent and type of fines (mineral filler, silt, or clay).
The DRIP 2.0 software provides a material library with ASTM/AASHTO
No. 57 or No. 67 gradations as well as granular permeable bases used by
a number of US states.
Once the resultant length of the flow path and the permeability of the
base material are known, it is necessary to determine the required thickness
of the permeable base. Two basic concepts are available for this design –
the depth of flow method, and the time to drain method (Mallela et al.
2002: 4-9–4-10). The DRIP 2.0 software may be used to design the layer
based on either method.
The depth-of-flow method was developed by Moulton (1980) and may
be used to either determine a minimum drainage layer thickness for a given
design inflow rate, permeability, and length and slope of flow path, or
to find a required coefficient of permeability for a given layer thickness.
Moulton’s equations and charts are reproduced by Mallela et al. (2002:
86 Subgrades, subbases, and drainage
The time-to-drain method was developed by Casagrande and Shannon
(1952) and is based on a specific time (2 hours to 1 month) and either 50
percent drainage or 85 percent saturation. The DRIP 2.0 software computes
time-to-drain by either the Casagrande and Shannon (1952) or Barber and
Sawyer (1952) equations. Mallela et al. (2002: 4–13) note that the time for
drainage is not sensitive to thickness, so these equations are more useful for
determining the required k.
Designing the separation layer
Mallela et al. (2002: 4-15) note that:
The separator layer may be a granular base material or an appropriate
geotextile. The separator layer must (a) prevent fines from pumping
up from the subgrade into the permeable base; (b) provide a stable
platform to facilitate the construction of the permeable base and other
overlying layers; (c) provide a shield to deflect infiltrated water over
to its edge-drain, thereby providing protection for the subgrade; and
(d) distribute live loads to the subgrade without excessive deflection.
Only an aggregate separator layer can satisfactorily accomplish (b) and
(d). The granular separator layer is preferred to the fabric since the
granular layer will provide the construction platform and distribution
of loads to the subgrade. When geotextiles are used as separator layers,
they are most often used in connection with stabilized subgrades, which
provide the construction platform and load distribution. Both granular
and geotextile materials can prevent pumping of fines if they satisfy the
filter requirements. The thickness of the granular separator is dictated
by construction requirements and can range from 100 to 300 mm (4 to
For concrete pavements, distribution of live loads (d) is not important
because the rigid concrete slabs significantly reduce pressure on the sub-
grade. What is important is keeping subgrade fines from migrating up and
clogging the permeable base.
Preventing clogging requires that an aggregate layer meets both of the
following criteria at the interface:
D15 (permeable base) ≤ 5 D85 subgrade (4.4)
D50 (permeable base) ≤ 25 D50 subgrade (4.5)
where D15 D50, and D85 represent the 15, 50, and 85 percentile particle
diameters from the gradation curve. If equations 4.4 and 4.5 are met at the
Subgrades, subbases, and drainage 87
permeable base – subgrade interface, then there is no need for a separator
layer. If not, then a separator layer should be used. The same two criteria
must be met at the separator layer and permeable base interface. Other
requirements for separator layer materials are provided by Mallela et al.
Geotextiles may also be used to separate the drainable base from the
subgrade. They must also meet filter and clogging criteria for the appar-
ent opening size of the geotextile. These are different for woven and
non-woven geotextiles and for different soil types (Mallela et al. 2002:
Mallela et al. (2002: 5-1–5-7) provide a design example for a drainable base
under a concrete pavement. The following design parameters are used:
• Pavement width and thickness – two 3.66 m (12 ft) lanes, 225 mm
(9 in) thick, with 3.05 m (10 ft) shoulders on each side. Transverse
joint spacing is 6.1 m (20 ft).
• Cross-slope – uniform, not crowned, sloped at 2 percent in both longi-
tudinal and transverse directions.
• Permeable base – same width as PCC pavement, AASHTO #57 material
with density/unit weight of 2 082 kg/m
(130 pcf), trial thickness
100 mm (4 in) based on construction considerations.
• Subgrade material – Georgia Red Clay, a well-graded clayey-silt, with
K = 0 001 m/day (0.0033 ft/day). The sieve analysis for the subgrade
material is 92 percent passing the 4.75 mm sieve (#4), 67 percent passing
the 2 mm sieve (#10), 55 percent passing the 850 m sieve (#20), 42
percent passing the 300 m sieve (#50), and 31 percent passing the
75 m sieve (#200).
Results of the roadway geometry calculations (Figure 4.1) provide SR =
0 0283 and LR = 10 35 m (33.94 ft).
Next, inflow is computed. The inflow computation by the crack
infiltration method (equation 4.1) is shown in Figure 4.2 as 1 48 ×
0 42 ft3
. If meltwater is included (not shown), it
would add about 10 percent to the inflow.
The permeable base is then designed by the depth-of-flow method.
First, the permeability of the base must be determined, using the gra-
dation, specific gravity, and unit weight. This is shown in Figure 4.3.
Based on a subgrade permeability of 122 m/day (400 ft/day), the required
base thickness is determined to be 194 mm (7.6 in), which is more than
the provided thickness of 100 mm (4 in) (Figure 4.4). Therefore, the
thickness should be increased to 200 mm (8 in). Alternatively, if the
Figure 4.1 Roadway geometry inputs for concrete pavement drainage design.
Figure 4.2 Computation of inflow.
Figure 4.3 Determining the permeability of the base.
Figure 4.4 Designing the base by the depth-of-flow method.
90 Subgrades, subbases, and drainage
compaction of the base were reduced so that the in-place density/unit
weight were 2 000 kg/m
(125 pcf), then the 100 mm (4 in) base
would be sufficient. This example shows the tradeoff between stability
and permeability, as well as the need to avoid overcompacting permeable
The time-to-drain for the base can also be checked, as shown in Figure 4.5.
Even at the lower permeability of 122 m/day (400 ft/day), the base would
drain to 50 percent in 4–5 hours, by either the Barber and Sawyer or
Casagrande and Shannon equations.
The next step is to determine if a separator is needed, by checking equa-
tions 4.4 and 4.5. The gradation curves are plotted for both the permeable
base and subgrade materials. Because the drainable base is a standard
material (AASHTO #57), the gradation is provided within the DRIP 2.0
software. The subgrade material must be input. The software interpolates
the gradation curve to determine D15 D50, and D85 for the two materials.
Figure 4.6 shows the gradation analysis for the user-defined subgrade mate-
rial. These values could also be determined by plotting a standard gradation
Next, the separator tab in DRIP 2.0 may be used to determine if the
criteria are met. Figure 4.7 indicates that they are for these two materials,
so there is no need for an aggregate or geotextile separator.
Figure 4.5 Checking the base design by the time-to-drain method.
Figure 4.6 User-defined subgrade material.
Figure 4.7 Checking need for a separator layer.
92 Subgrades, subbases, and drainage
Water that goes into a permeable base has to come out somewhere. Some
water will exit through the subgrade, but if this outflow were sufficient
there would be no need for a drainage layer in the first place. Therefore,
the drainage layer typically drains to the sides.
The drainage layer may terminate with longitudinal drains, or may extend
through the side slope (“daylighting”). Longitudinal drains are more reliable
because daylighted drainage layers are susceptible to contamination and
clogging. Longitudinal drains may have pipes or may be aggregate French
drains without pipes (Huang 2004: 338).
The DRIP 2.0 software includes the design of longitudinal collector pipes.
The edge-drains may be designed for pavement infiltration flow rate, peak
flow from the permeable base, or the average flow rate during the time to
drain the permeable base. It is recommended that the minimum capacity be
the peak capacity of the permeable base. It is usually conservatively assumed
that all flow is handled by the pipe, with no allowance for outflow through
the soil. Pipe flow capacity is computed using the Manning equation, as
detailed in many hydraulics and fluid mechanics textbooks (Mallela et al.
The capacity of the outlet pipes must also be checked, using the Manning
equation. The outlet drain slope should be at least 3 percent (Mallela et al.
Generally the only design variables for longitudinal edge-drains are the
type of pipe, pipe diameter, and outlet spacing. The type of pipe and
outlet spacing are often matters of policy within a transportation orga-
nization, and minimums may be specified based on maintenance require-
ments. Minimum pipe diameters of 75–100 mm (3–4 in) with outlet
spacings of 75–100 m (250–300 ft) are common (Mallela et al. 2002:
Separators may also be necessary with edge-drains. “The filter mate-
rial must be fine enough to prevent the adjacent soil from piping or
migrating into the edgedrains but coarse enough to allow the passage
of water with no significant resistance.” These functions may be per-
formed with aggregates, which may be difficult to place without contam-
ination, or with geotextiles. They must be met with regard to holes or
slots in perforated or slotted pipes (Mallela et al. 2002: 4–20). Prefab-
ricated geocomposite edge-drains may also be used (Mallela et al. 2002:
Continuing the previous design example, corrugated pipes with 100 mm
(4 in) diameter are tried, with the “permeable base” peak flow design
Subgrades, subbases, and drainage 93
Figure 4.8 Edge-drain design.
method. Results from DRIP 2.0 are shown in Figure 4.8, with a maximum
outlet spacing of 628 m (2,060 ft) (Mallela et al. 2002: 5-8–5-9). The
time-to-drain criterion may also be checked, but that results in a larger
maximum outlet spacing. The software also has a provision for design of
For an existing pavement, it is obviously impossible to retrofit a permeable
base. However, edge-drains can be installed along an existing pavement.
These will lower the water table in the vicinity of the pavement and reduce
the moisture content of the subgrade and subbase. According to Mallela
et al. (2002: 4-20–4-23), a 1989 FHWA study on retrofitting edge-drains
for pavement rehabilitation concluded that:
• The edgedrain should be located under the shoulder immediately
adjacent to the pavement/shoulder joint.
• By eliminating the filter fabric at the subbase/edgedrain interface,
eroded fines cannot clog the filter fabric.
94 Subgrades, subbases, and drainage
• Trench backfill should be permeable enough to transmit water to
the longitudinal edgedrain pipe; asphalt or cement treated backfill
increases stability with little or no loss of permeability.
• The most commonly used trench width was 300 mm (12 in); locat-
ing the top of the pipe at the bottom of the layer to be drained was
• Outlet spacing should not exceed 150 m (500 ft); additional outlets
should be provided at the bottom of sag vertical curves.
• Because of the tendency of flexible corrugated plastic pipe to curl,
use of rigid PVC pipe was recommended for outlet laterals; rigid
PVC pipe helps maintain proper outlet pipe grade and provides
protection from crushing.
• Headwalls protect the outlet pipe from damage, prevent slope ero-
sion, and ease in the locating of the outlet pipe.
Retrofitting edge-drains as a rehabilitation strategy is discussed in
Chapter 17. Maintenance of edge-drains, also important, is discussed in
Drainage of airport pavements is addressed in the FAA document Air-
port Drainage, Advisory Circular (AC) 150/5320-5B (FAA 1970). Surface
drainage or airport pavements is less effective than for highway pavements,
because airport pavements are much wider and must have much gentler
transverse and longitudinal slopes for safety reasons. Permeable bases are
therefore more useful and important.
Selection of concrete materials
The successful use of concrete as a construction material extends back two
millennia to the days of the Romans – and one of their greatest structures,
the Pantheon, is still providing excellent service (Delatte 2001). On the
other hand, some concrete structures and facilities built since then have
had considerably shorter service lives. Careful selection of concrete mate-
rials and careful mixture design and proportioning, combined with good
design and construction practices, is a key contributor to success. Durability
is addressed in Guide to Durable Concrete, 201.2R-01 (ACI Committee
Pasko (1998) states that
a good pavement designer should also be a concrete expert. Some facts
to be kept in mind are:
• In the United States, there are 118 cement plants, each producing
a variety of “unique” products under broad specifications. From
personal experience on a research project, five Type I cements from
different plants ranged in 28-day strength from 2738 to 4975 psi
(19 to 34 MPa).
• There are 420 coal-burning plants in this country, and 28 per-
cent of their fly ash is acceptable for use in concrete in accor-
dance with ASTM C618. These products react differently with
various cements, and the result is dependent on the quantities
used. This is particularly important with respect to alkali aggre-
gate reaction and sulfate resistance (and, possibly, delayed ettringite
• Thousands of aggregate sources are available for use. Unfor-
tunately, aggregate is not an inert filling. In addition to some
aggregates reacting with the cementious materials, there are other
characteristics that can cause problems.
96 Selection of concrete materials
Concrete in its most simple form consists of cement, water, and aggregates.
In modern practice, chemical admixtures are almost always used, particu-
larly for pavements. The use of supplementary cementitious materials, also
called mineral admixtures, is also very common, because these materials
reduce the cost and improve the performance and durability of concrete.
Three excellent overall references on concrete are Kosmatka et al. (2002),
Mindess et al. (2003), and Neville (1997).
Cement is the hydraulic glue that holds concrete together. In US practice,
Portland cements are numbered using the Roman numerals I through V.
Type I is a general purpose cement suitable for all uses where no special
properties are required. In much of the United States it is by far the most
common cement. Type II cement is used where it is important to protect
against moderate sulfate attack. Sulfates are found in soils and groundwater,
particularly in the western states of the US, and may attack concrete made
with type I cement. In regions where sulfates are commonly found, type II
cement is the more common type, and not type I. Some cements meet both
type I and II and are designated type I/II. Type III cement is ground finer
to achieve higher early strength. Type IV cement has slower strength gain
for applications where heat of hydration must be minimized – it is now
rarely available because the same effect may be achieved, at lower cost,
with supplementary cementitious materials. Type V cement provides higher
sulfate resistance than type II for more severe environments (Kosmatka et al.
2002: 27–30). Portland cements are manufactured to meet ASTM C150,
Standard Specification for Portland Cement (ASTM C150 2005).
In Canada, Types I–V are termed types 10–50 (Mindess et al. 2003: 26).
Blended hydraulic cements also exist, with several designations depending
on whether blast furnace slag or pozzolans are added, along with hydraulic
cements and hydraulic slag cements (Kosmatka et al. 2002: 31–33).
Supplementary cementitious materials
Supplementary cementitious materials, or mineral admixtures, include fly
ash, slag, and silica fume, as well as other materials. Fly ash and slag
are commonly used in pavements. Typically, these materials retard early
strength gain of concrete, but improve the ultimate strength and durability.
Overall heat of hydration and the rate of heat buildup are both reduced.
Workability is improved, and the concrete surface is often easier to finish.
Durability is improved because the porosity of the concrete is decreased and
susceptibility to sulfate attack and ASR is reduced (Mindess et al. 2003:
Selection of concrete materials 97
Supplementary cementitious materials may have pozzolonic properties,
cementitious properties, or both. The pozzolonic reaction works with the
reaction products of cement hydration to improve strength and decrease
porosity of hardened cement paste and concrete (Mindess et al. 2003: 95).
Fly ash, the most widely used supplementary cementitious material
in concrete, is a byproduct of the combustion of pulverized coal in
electric power generating plants. It produces spherical glassy particles
that are finer than Portland cement. Two types of fly ash are available,
depending on the type of coal that was burned to make the ash. Class
F fly ash has pozzolonic properties, and Class C fly ash has both
pozzolonic and cementitious properties. Class F fly ash is typically used
at 15–25 percent by mass of the cementitious material, and Class C at
15–40 percent by mass.
(Kosmatka et al. 2002: 58–59)
Requirements for class C and F fly ash are provided in ASTM C618 (ASTM
Kohn and Tayabji (2003: 61) note that “Class C fly ash may be detri-
mental to the performance of concrete, causing premature stiffening of the
fresh concrete, thermal cracking, and/or reduced sulfate resistance (it) is
generally not effective in controlling expansions due to ASR.” Early stiff-
ening problems are more likely in hot weather with certain water reducing
admixtures. The potential for early stiffening may be assessed by making
trial batches at the highest temperatures anticipated on the project, and
measuring slump loss and setting times.
Ground granulated blast furnace slag (GGBFS), also called slag or slag
cement, is a by-product of metallurgical processes, generally the production
of iron from ore. Slags are classified as grade 80, 100, or 120 based on
reactivity, which is roughly 80, 100, or 120 percent of the 28-day strength
of a reference mortar made with pure cement (Mindess et al. 2003: 102–
103). Requirements for slag are provided in ASTM C989 (ASTM C989
2005). GGBFS should be distinguished from slag as an aggregate, which
has no cementitious properties.
Ternary blend mixtures, which use Portland cement, fly ash, and slag,
can produce very durable, low-permeability concrete. The Department of
Aviation for the City of Houston, Texas, had experienced problems of
durability of high early strength concrete. For a runway expansion at the
George Bush Intercontinental Airport (IAH) in 2002, a concrete with type
98 Selection of concrete materials
I cement (50 percent), class F fly ash (25 percent), and grade 120 slag (25
percent) was developed and extensively tested, and was predicted to have a
service life of 120 years (Sarkar and Godiwalla 2003).
Other supplementary cementitious materials
Another material, silica fume or microsilica, is often used in high perfor-
mance, low-permeability structural concrete but rarely if at all in pavements.
It is a by-product obtained during the manufacture of silicon metal and
alloys (Mindess et al. 2003: 95). It is more expensive than fly ash or slag and
less widely available, and the most likely application in pavements would
be for repair materials or thin bonded concrete overlays.
Other materials with potential use in paving concrete include rice husk
ash, metakaolin, natural pozzolans, and limestone filler. Rice husk ash is
not yet commercially available, but it has the potential to become another
important ingredient in concrete. The other three materials are not by-
products and have less potential for paving concrete (Malhotra 2006).
Aggregates and water
“Aggregates generally occupy 70 to 80 percent of the volume of concrete and
therefore can be expected to have an important influence on its properties”
(Mindess et al. 2003: 121). Aggregate is not simply an inert filler in concrete,
and its properties deserve careful consideration.
Aggregates are granular materials, usually natural rock (crushed rock
or natural gravels) and sands. Aggregates are classified as normal weight,
heavyweight, and lightweight, based on specific gravity. For concrete pave-
ments, normal weight aggregates are generally used because they are most
available. Aggregates for concrete must meet ASTM C33 Standard Speci-
fication for Concrete Aggregates (ASTM C33 2003). Aggregate properties
that affect concrete pavement performance include shape and texture, size
gradation, absorption and surface moisture, specific gravity, unit weight,
physical durability, chemical durability, and strength. Strength of the aggre-
gate particles rarely governs concrete strength, because the lower strength
of the paste or the aggregate-paste bond is likely to govern instead.
Aggregate shapes may be rounded or angular, with rounded materials
occurring naturally and angular materials produced by crushing and pro-
cessing. Within those two main divisions, aggregate shapes may be further
classified as spherical, irregular, highly irregular, flat or oblate/flaky, and
elongated. Textures may be glassy, smooth, granular, rough, crystalline, or
honeycombed. Rounded aggregates are more workable, but angular parti-
cles may develop higher flexural strength, which is important for pavements
(Mindess et al. 2003: 122–125).
Selection of concrete materials 99
Grading of an aggregate is determined by a sieve analysis, where the mass
of an aggregate sample retained on each of a number of standard sieves
is recorded. Two key parameters are the maximum aggregate size and the
shape of the gradation curve.
Absorption and surface moisture are of significance for calculating water
that aggregate will add to or subtract from paste, and are used in mixture
proportioning. Specific gravity is used to establish weight–volume relation-
ships, also for mixture proportioning. Unit weight differs from specific
gravity in that it includes not only the volume of the particles but the vol-
ume of the space between them when they are densely packed (Mindess
et al. 2003: 133–140). These properties are all necessary when proportion-
ing concrete mixtures by either the ACI 211.1 or 211.3 procedures (ACI
Committee 211 1991, 2002).
Physical durability of aggregates refers to soundness and wear resistance.
Aggregates are unsound if they deteriorate due to volume changes caused by
repeated cycles of freezing and thawing or of wetting and drying. Unsound
aggregates lead to surface popouts and D-cracking, discussed in Chapter 3.
Wear resistance of aggregate plays some part in wear resistance of concrete
under traffic, particularly in areas where studded tires are allowed (Mindess
et al. 2003: 140–142).
For concrete pavements, the wear resistance of fine aggregates is more
important than that of coarse aggregates for retaining skid resistance over
time (Huang 2004: 408). Aggregates with poor wear resistance lead to
polished pavement surfaces with poor skid resistance. It also seems logical
that the wear resistance of coarse aggregates would also be an important
factor in the performance of aggregate interlock joints over time.
“Most chemical-durability problems result from a reaction between reac-
tive silica in aggregates and alkalis contained in the cement” (Mindess et al.
2003: 142). These encompass ASR and alkali-carbonate reaction, and lead
to map cracking as discussed in Chapter 3. Fly ash, class F in particular, and
slag have been used to control ASR. Other measures include the use of low-
alkali cements and, when possible, the avoidance of susceptible aggregates
(Mindess et al. 2003: 149–151).
It has been recognized that the concrete linear coefficient of thermal
expansion (CTE) is an important performance parameter. This coefficient
determines how much joints and cracks open and close, and how much
concrete slabs curl due to temperature gradients. The concrete thermal
coefficient may range from 7 4–13 / C 4 1–7 2 / F . Since aggregates
make up such a large portion of the concrete, they effectively determine the
thermal coefficient for the concrete. Limestone has a low thermal coefficient
of 6 / C 3 3 / F , while sandstone has a higher thermal coefficient of
11–12 / C 6 1–6 7 / F (Mindess et al. 2003: 460).
Therefore, for a given temperature differential, concrete made with sand-
stone will attempt to move nearly twice as much as concrete made with
100 Selection of concrete materials
limestone, and will develop twice as much stress if the movement is
restrained. Joints must be designed to accommodate the larger displace-
ments. In addition, the temperature-induced curling of the slab will be twice
It may not be economically feasible to change coarse aggregate sources
on a paving project to reduce the concrete CTE. However, reducing the
joint spacing will decrease curling stresses and the risk of cracking (Hall
et al. 2005: 22).
For pavements, it is generally preferable to use the largest available coarse
aggregate size, limited to 1/3 of the thickness of the pavement. This is
because using the largest available aggregate reduces the proportion of paste,
thus reducing shrinkage. Most ready-mix concrete equipment can handle
aggregates up to 50 mm (2 in) in size. One caveat is that if the aggregate is
susceptible to freeze-thaw damage, or D-cracking, a reduction in aggregate
size will improve durability (Mindess et al. 2003: 125–127). For aggregate
interlock pavement joints, use of larger maximum size aggregate should
improve load transfer.
Use of a continuously or densely graded aggregate will also reduce paste
requirements, since the smaller aggregate fills gaps in the larger aggregate.
Uniformly graded or gap graded aggregates require more paste. Pervious
concrete, unlike conventional concrete, uses a uniformly graded coarse
aggregate (Mindess et al. 2003: 126–131).
ASTM C33 sets limits for fine and coarse aggregates separately. For fine
aggregates, the particle distribution is represented by a fineness modulus
FM, which is the sum of the cumulative percentage retained on seven stan-
dard sieves (150 m–9.5 mm or No. 100-3/8 in), divided by 100. The FM
is typically between 2.3 and 3.1, with a smaller number indicating finer
sand. FM determines the effect of the fine aggregate on workability, which
is important for mixture proportioning (Mindess et al. 2003: 126–131).
Traditionally, natural sands have been used for concrete, but where these
deposits are being depleted, manufactured sands made from crushed rock
are used instead.
Hall et al. (2005: 20–21) suggest instead using a well-graded coarse sand
with an FM in the range of 3.1–3.4, particularly with the high cement
contents often used in airfield pavement construction. Coarser sands reduce
Selection of concrete materials 101
Optimized combined aggregate grading
Aggregate grading research for soils, base, asphalt, and other applica-
tions has proven that the best performance is derived from that blend of
equi-dimensional particles that are well-graded from coarsest to finest.
Optimum combined aggregate grading is important for portland cement
concrete because it minimizes the need for the all-important second
mix component—the paste—and has a significant effect on the air-void
structure in the paste. The paste volume should be no more than is
necessary to provide lubrication during placement and bind the inert
aggregate particles together to resist the forces that will affect the mass
during its service life Gap grading (especially at the No. 4 and 8
sieves) and excessive fine sand and cementitious materials content were
found to cause problems. Corrections to fill gaps in the aggregate grad-
ing led to significant reductions in water, improvements in mobility and
finishability, and increases in strength.
(Shilstone and Shilstone 2002: 81)
The nos 4 and 8 sieves are 2.36 and 4.75 mm, respectively. The 1.16 mm
and 600 m (nos 16 and 30) sieves are also important.
Standard coarse and fine aggregate grading specifications such as those
published by ASTM and public agencies seldom facilitate development of
well-graded combined aggregate. ASTM C-33-03 (ASTM C33 2003), para-
graph 1.3 makes provision for the specifier to cite that standard for qual-
ity of materials, the nominal maximum aggregate size, and other grading
requirements. This allows the specifier to cite the coarseness factor chart
(Figure 5.1) and limits within the parallelogram in zone II for combined
aggregate grading. The one proportioning the mixture can use locally avail-
able non-standard or asphalt standard aggregate to fill voids.
Shilstone and Shilstone (2002) discuss aggregate gradation in detail. More
detailed information is provided by Shilstone (1990). A key feature of
the Shilstone approach is the use of the combined aggregate relationship
nomograph, shown in Figure 5.1.
The x-axis of the chart represents the coarseness factor of the combined
aggregates. This is the percentage of aggregate retained on the 2.36 mm (no.
8) sieve that is also retained on the 9.75 mm (3/8 in) sieve. The y-axis of the
chart is the combined aggregate workability factor. This is the percentage of
aggregate passing the no. 8 sieve, adjusted for cementitious content. To adjust
for the cementitious material content, add or subtract 2.5 percentage points
on the y-axis for every 43 kg/m
of cementitious material more or
less than 335 kg/m
(Shilstone and Shilstone 2002: 82).
The chart provides a trend bar and five zones. “The diagonal bar is
the Trend Bar that divides sandy from rocky mixtures. Zone I mixtures
segregate during placement. Zone II is the desirable zone. Zone III is an
extension of Zone II for 0.5 in (13 mm) and finer aggregate. Zone IV has too
102 Selection of concrete materials
Concrete mixture design
Combined aggregates relationships
Coarseness factor, combined aggregates
Percent retained on no. 8 sieve that is also retained on 3/8" sieve
40 20 0
Figure 5.1 Combined aggregate relationship (coarseness factor) chart (courtesy:
Shilstone and Shilstone 2002).
much fine mortar and can be expected to crack, produce low strength, and
segregate during vibration. Zone V is too rocky” (Shilstone and Shilstone
2002: 82). Paving concrete should fall into zone II since the coarse aggregate
is almost always larger than 13 mm (1/2 in).
The Shilstone Companies (undated) suggest the following guide specifi-
cation for highway pavement concrete:
This guide is meant to provide a basis for development of concrete
pavement mixtures using locally available aggregate. It is based upon
the objective of optimizing the combined aggregate grading to minimize
the need for paste (water, cementitious materials, and entrained air).
A. The minimum concrete (compressive) (flexural) strength shall be
_____ [MPa] psi.
Selection of concrete materials 103
B. Cementitious materials shall include portland cement and may
include Fly Ash or Ground-Granulated Blast Furnace Slag as appro-
priate for the local conditions.
C. Admixtures, if used, shall meet the requirements of ASTM C-494
and ASTM C260 and be compatible with the cementitious materi-
als. Develop an air content of _____ % ±11/2 %
D. The aggregate shall comply with the Agency or ASTM C-33-04
specifications and meet the following criteria:
• The aggregate shall meet quality requirements of _____ (Agency
or ASTM C33).
• The nominal maximum aggregate size shall be [38 mm] 1–
• The grading of the combined aggregate shall fall within Zone
II when plotted on the Coarseness Factor Chart (Figure 5.1).
The supplier shall establish his mixture design within a paral-
lelogram indicating limits of allowable production variations.
When aggregate tests lead to results outside of the parallel-
ogram, adjust mixture proportions to fall within the design
• The grading of the combined aggregate shall be such that the
sum of the percent retained on 2 adjacent sieves shall not be
less than 13%.
• When aggregate tests lead to results outside of the limits of the
mixture design parallelogram, adjust mixture proportions to
fall within the design limits.
• When tested in accordance with ASTM C642, the permeable
pores shall be 13% or less.
Kohn and Tayabji (2003: 63) note that concrete produced with well-graded
aggregate combinations will have less water, provide and maintain ade-
quate workability, require less finishing, consolidate without segregation,
and improve strength and long-term performance. In contrast, gap-graded
aggregate combinations tend to segregate, contain more fines, require more
water, shrink more, and impair long-term performance.
Shilstone and Shilstone pointed out that the coarseness factor chart
is a guide. Two other graphics, percent retained on each sieve and the
0.45 power chart, define details not reflected in the three size group-
ings in the nomograph. Gaps in grading can occur in other sieve sizes
such as the 1.18 mm and 600 m (nos 16 and 30). Optimized mixtures
have produced excellent results for building construction, highways, and
104 Selection of concrete materials
The maximum density grading or 0.45 power chart is more widely used
in asphalt paving than in concrete paving. This relationship may be repre-
P = 100 d/D 0 45
where d = sieve size in question, P = percent finer than (passing) sieve
d, and D = maximum size of aggregate. This may need to be adjusted
for aggregate angularity, shape, surface roughness, size, and compaction
method (Barksdale 1991: 3-22–3-23). A gradation that follows equation 5.1
closely would use the least paste, but would probably need to be modified
to allow for workability.
Lightweight aggregates have been used in bridges and buildings to reduce
dead load. Since dead load is not significant for pavements, there has not
been perceived to be a benefit to the use of lightweight aggregate. There are,
however, potential advantages that have not been traditionally considered.
Some key references on lightweight aggregate concrete are provided by the
ACI, including ACI 211.2-98 Standard Practice for Selecting Proportions
for Structural Lightweight Concrete (Re-Approved 2004) (ACI Committee
211 1998) and ACI 213R-03 Guide for Structural Lightweight-Aggregate
Concrete (ACI Committee 213 2003). These documents focus on structural
concrete rather than pavement, but they identify some of the desirable
characteristics of lightweight aggregate (LWA) concrete that also apply to
• lower modulus of elasticity, which in pavements translates to less tensile
stress (cracking risk) for the same deformation or strain;
• flexural and splitting tension strengths comparable with conventional
• freeze-thaw durability may be equal to or better than that of conven-
• reduced risk of alkali-aggregate reactions;
• some types of LWA provide superior abrasion resistance.
In 1963 and 1964, a CRCP LWA concrete test section was built on an
interstate highway frontage road in Houston, Texas, along with a standard
aggregate CRCP test section for comparison. The sections were evaluated
in 1974, 1984, and 1988. A 24-year performance survey in Texas found
that the CRCP pavements built with lightweight aggregate concrete had
relatively less surface distress than standard aggregate sections (Won et al.
1989, Sarkar 1999). At 34 years, another detailed investigation was carried
Selection of concrete materials 105
out. The LWA section showed high durability, low permeability, and little
cracking and spalling (Sarkar 1999).
LWA has also been investigated as a very thin non-skid surface overlay
for concrete pavements. Natural sand, expanded shale LWA, and slag were
compared (Gomez-Dominguez 1978).
Research has recently focused on the use of a replacement of a portion of
fine normal weight aggregate with saturated lightweight aggregate, which
has much higher absorption, in order to improve concrete curing (Bentz
et al. 2005, Lam 2005, Mack 2006). Since pavements have high surface to
volume ratios and are exposed to the environment, and are thus hard to
cure, this concept seems to hold considerable promise for concrete pavement
Typical LWAs are expanded shales, slates, clays, and similar materials,
with dry unit weights of 550–1 050 kg/m
and 5–15 percent
absorption of water by weight. They are heated in rotary kilns and bloat
up similar to popcorn (Mindess et al. 2003: 158–159).
Waste materials as aggregates
As supplies of natural aggregates deplete and landfills fill up, interest in
recycling waste materials as aggregates increases. There is a need to proceed
with caution, however, because there would be little benefit to turning our
concrete pavements into “linear landfills” with all of the maintenance and
performance problems that the term implies.
Solid wastes that have been considered as aggregate for concrete include
mineral wastes from mining and mineral processing, blast furnace slags,
metallurgical slags, bottom ash, fly ash not meeting class C or F specifica-
tions, municipal wastes (including commercial or household), incinerator
residues, and building rubble (including demolished concrete). Factors that
must be considered when deciding whether to use these materials include
economy, compatibility with other materials, and concrete properties. The
latter two factors often rule out the use of waste materials (Mindess et al.
2003: 156–158). However, hard mineral wastes and slags offer some poten-
tial for improving surface friction if used as fine aggregate.
The RMC Research Foundation (2005) publication Ready Mixed Con-
crete Industry LEED Reference Guide discusses the environmental benefits
of incorporating post-consumer recycled content into concrete construction.
The importance of this has been reviewed in Chapter 1. The most com-
monly used aggregate substitute is crushed recycled concrete. Air-cooled
blast furnace slag may be used as an aggregate, but has no cementitious or
pozzolanic properties and should not be confused with GGBFS or “slag”
used as a cement replacement, as discussed above (RMC Research Founda-
tion 2005: 38). For commercial or industrial projects that are attempting to
106 Selection of concrete materials
achieve a specific level of LEED certification, it may be useful to consider
recycled materials as aggregate.
“Crushed recycled concrete aggregate generally has lower specific gravity
and higher water absorption than natural stone aggregate. New concrete
made with such aggregate typically has good workability, durability, and
resistance to saturated freeze-thaw action. Fine recycled aggregate should
only be used in very limited quantities strength using only coarse aggre-
gate replacement is similar to that of concretes using natural aggregates”
(RMC Research Foundation 2005: 38). Other cautions are that the crushed
concrete should come from a known source and be clean, for example, free
of chemicals, clay coating, and other fine materials.
Air-cooled blast furnace slag may be a dense and hard aggregate, and
therefore desirable from the standpoint of wear and abrasion resistance.
Crushed glass is generally not recommended as an aggregate because of the
risk of ASR.
On occasion, use of recycled materials has led to problems.
Heaving of pavements and a building foundation became progressively
worse on a project at Holloman Air Force Base (AFB) N.M. The cause of
heaving was identified as sulfate attack on recycled concrete used as fill
and base course below the buildings and pavements. This recycled con-
crete came from sulfate-resistant airfield Portland concrete pavement
that had existed for decades at Holloman AFB without distress. How-
ever, severe sulfate exposure conditions, ready availability of water, the
more permeable nature of the crushed recycled concrete, less common
thaumasite attack, possible soil contamination as a secondary source of
alumina, or some combination of these factors allowed sulfate attack to
develop in the recycled material even though it had not in the original
(Rollings et al. 2006: 54)
The traditional rule of thumb is that potable water is good for making con-
crete. It does not, however, follow that non-potable water cannot be used,
although there are limits on dissolved solids and organic material. Seawater
should be avoided for any concrete containing reinforcement (Mindess et al.
Chemical admixtures are used in concrete to affect either the fresh or
hardened concrete properties. While a wide variety of admixtures are avail-
able to the industry, concrete pavement almost always uses air-entraining
Selection of concrete materials 107
admixtures, with set-controlling admixtures (accelerators and retarders) and
water reducers or plasticizers used under specific circumstances. Admix-
ture technology is advancing rapidly, and new admixtures are always being
developed which may be useful for paving applications.
Air-entraining admixtures are used to protect concrete from damage due
to freezing and thawing. Their primary purpose is to develop an entrained
air void system of tiny spherical bubbles, 0.05–1.25 mm (0.002–0.05 in)
in diameter, throughout the concrete, with an average spacing of no more
than 0.2 mm (0.008 in). The air should be 9 percent of the mortar fraction,
or 7.5 percent of the total concrete volume for 9.5 mm (3/8 in) maximum
size coarse aggregate to 4 percent for 64.5 mm (21/2 in) aggregate. This
is because the air void system protects the cement paste, and with larger
coarse aggregate there is less paste. Air entrainment also makes concrete
more workable (Mindess et al. 2003: 168–176).
Concrete pavements are exposed to the environment, and unless the cli-
mate makes freezing and thawing very unlikely, air-entraining admixtures
should be used. Some admixture manufacturers provide products specifi-
cally tailored for paving concrete.
Set-accelerating admixtures hasten the normal processes of setting and
strength development of concrete. Calcium chloride is a popular accelerator
because of its low cost, but it has the major disadvantage of increasing the
rate of corrosion of reinforcement, tie bars, and dowels. Non-chloride accel-
erators are available for reinforced concrete applications (Mindess et al.
2003: 185–187). For paving applications, accelerating admixtures are likely
to be useful in cold weather or when a pavement repair or overlay must be
opened to traffic quickly.
Set-retarding admixtures delay set, allowing more time for placement, con-
solidation, and finishing. Subsequent strength development is not signifi-
cantly affected (Mindess et al. 2003: 182–183). For paving applications,
retarding admixtures are likely to be useful in hot weather or when haul
distances between concrete production and placement are exceptionally
108 Selection of concrete materials
Three types of water reducing admixtures are currently available – low range
(regular), mid-range, and high range (superplasticers). Low-range water
reducers allow 5–10 percent water reduction, mid-range 10–15 percent,
and high range 15–30 percent. These materials, particularly the latter, may
be used to produce flowing concrete with very high slump (Mindess et al.
Concrete pavements are typically placed at low slump, particularly when
slipformed, so flowing concrete is not needed. However, water reducing
admixtures may be used to reduce water content, and thus the amount of
cement required to achieve a specific water/cement ratio. A reduction in
cement and paste reduces the amount of shrinkage and thermal deformation
of the pavement during curing. Some water-reducing admixtures also act
as set retarders. Water-reducing admixtures may be useful for fixed form
paving or for small areas of hand work.
Compatibility of materials
As more different materials are put into concrete, the compatibility of those
materials becomes more of an issue. Mindess et al. (2003: 167) note that
“effects that the admixtures may have on other concrete properties should
be taken into account.” Other admixtures may alter the effectiveness of
air-entraining admixtures, as may finely divided mineral admixtures such
as fly ash (Mindess et al. 2003: 172). Generally, admixtures from the same
manufacturer will have been tested for compatibility with each other and
are therefore less likely to present problems.
Kohn and Tayabji (2003: 62) note that “some concretes exhibit unde-
sirable characteristics because of incompatibility among different concrete
materials. Undesirable characteristics include:
1. Early loss of workability (early stiffening)
2. Delayed set (retardation)
3. Early-age cracking due to excessive autogenous and drying shrinkage
4. Lack of proper air-void system.”
Early stiffening problems may be attributed to individual cementitious mate-
rials, interactions between cementitious materials, admixtures, and tempera-
ture effects. The factors that result in incompatibility are poorly understood
and difficult to determine through testing, and many problems are triggered
by higher or lower temperatures (Kohn and Tayabji 2003: 62–63).
Selection of concrete materials 109
To minimize incompatibility problems, Kohn and Tayabji (2003: 63)
recommend using admixtures only from a single manufacturer and keep-
ing dosages under the manufacturer’s recommended maximums, and using
only cementitious materials that meet project specifications and/or ASTM
standards. In areas with significant seasonal temperature differences, it is
advisable to have separate mixture designs for hot and cold weather. As
stated earlier, Kohn and Tayabji (2003: 61) have noted that class C fly ash
may cause compatibility problems with certain water-reducing admixtures
in hot weather.
The FHWA Techbrief Protocol to Identify Incompatible Combinations of
Concrete Materials defines incompatibility as “interactions between accept-
able materials that result in unexpected or unacceptable performance”
(FHWA Techbrief 2006: 1). Some of the findings on incompatibility include:
• A number of relatively simple field tests are available to warn of poten-
• Use of a fly ash containing tricalcium aluminate may result in flash set
because of insufficient sulfate to control hydration.
• Some type A water-reducing admixtures accelerate tricalcium aluminate
• Increasing temperatures increase the rate of chemical reactions and may
make marginally compatible material combinations incompatible.
• Use of non-agitating transporters for paving concrete may exacerbate
false set problems.
• Conversely, delayed setting increases the risk of plastic shrinkage crack-
ing and makes timing joint sawing more difficult.
• Material chemistry can provide clues – fine cementitious materials with
high tricalcium aluminate or low sulfate contents or fly ashes with high
calcium oxide contents may cause problems.
• Possible field adjustments to correct problems include adjusting sup-
plementary cementitious material type, source, or quantity; adjusting
chemical admixture type or dosage; or changing the batching sequence
or mix temperature (FHWA Techbrief 2006).
Two FHWA reports provide more information on this topic (Taylor et al.
Van Dam et al. (2005) investigated durability of early-opening-to-traffic
paving concrete. Because these concretes must typically achieve flexural
strength in 6–8 or 20–24 hours, based on the construction window avail-
able, they use high cement contents and a wider variety and greater quantity
of admixtures. Therefore, there is a greater potential for cement/admixture
interactions that can lead to later durability problems (Van Dam et al.
110 Selection of concrete materials
Fiber-reinforced concrete has not been widely used for pavements. The
exception is bonded concrete overlays and UTW, which have made use of
both steel and synthetic fibers, although synthetic fibers have been much
more widely used. Fibers are intended to improve the flexural toughness
and fatigue performance of the concrete (ACI Committee 325 2006: 9). The
benefits, if any, of using fibers in concrete overlays and pavements have
proven difficult to quantify. Use of fibers in concrete is discussed in an ACI
Committee 544 Report on Fiber Reinforced Concrete (Reapproved 2002)
ACI 544.1R-96 (ACI Committee 544 1996).
Steel fiber-reinforced concrete has been used to design thinner pavements
with longer joint spacings, but this has led to difficulties. “During the 1980s
several steel fiber reinforced concrete airfield pavements were built at civil
and Navy airfields using the new methodology. These tended to be relatively
thin and large (sometimes only 100- to 150-mm (4- to 6-in) thick and 15
or even 30 m (50 and even 100 ft) between contraction joints). There were
soon reports of widespread corner breaks at these airfields the large plan
dimension of the slabs relative to their thin cross section required very little
differential shrinkage between the top and bottom of the slab to get curling
in the field Once opened to traffic, these slabs developed widespread
corner breaks” (Rollings 2005: 170–171).
Mixture design and
Once quality materials have been selected, as discussed in Chapter 5, it
is necessary to design a concrete mixture for the project that will meet
the requirements for fresh and hardened concrete properties, while keeping
economy in mind. The concrete must meet project requirements in both
the fresh and hardened state. In the fresh state, the chief characteristic is
workability. In the hardened state, requirements for strength and durability
must be met. If the fresh concrete properties are not satisfactory, the concrete
will not be placed, consolidated, and finished properly, and the hardened
properties will not matter.
The most commonly used method for proportioning concrete mixtures
is the ACI Committee 211 Standard Practice for Selecting Proportions
for Normal, Heavyweight, and Mass Concrete, 211.1-91 absolute volume
method (ACI 211 1991). This method is discussed in Chapter 10 of Mindess
et al. (2003: 221–242) and Chapter 9 of Kosmatka et al. (2002: 149–177).
This procedure uses the following steps (Mindess et al. 2003: 227–236):
• Assemble the required information. This includes:
sieve analysis (gradation distribution) of coarse and fine aggregates;
dry rodded unit weight of coarse aggregate;
bulk specific gravities and absorption capacities of coarse and fine
slab thickness (since the maximum coarse aggregate size must be
less than or equal to one-third of the least dimension); w
• Choose the slump – typically 25–75 mm (1–3 in) for pavements, higher
if fixed forms are used, possibly lower if the pavement is slipformed.
• Choose maximum aggregate size – one-third of pavement thickness,
although availability or D-cracking concerns may dictate a smaller
aggregate. In many areas, 19 or 25 mm (3/4 or 1 in) may be the largest
112 Mixture design and proportioning
size available. If larger sizes are available, the pavement performance
may be improved.
• Estimate the mixing water and air content. Less water is typically used
for paving concrete than for structural concrete because the desired
slump is lower. The amount may be further reduced with water reducing
admixtures. Use of an optimized aggregate gradation, as discussed in
Chapter 5, will also reduce the mixing water requirement. Air content
is based on the maximum size aggregate (and thus the paste proportion)
and whether the exposure is mild, moderate, or severe. ACI 211.1
provides tables for maximum coarse aggregate size up to 75 mm (3 in).
Pavements are often subjected to severe exposure conditions.
• Determine the w/c or water/cementitious materials (w/cm) ratio. This
is based on either strength or durability, whichever is lower.
• Calculate cement or cementitious materials content. This is determined
by dividing the water by w/c (or w/cm). This gives either the total
cement content, or total cementitious materials if fly ash and/or slag are
used. If fly ash or slag are used, they replace cement on either a weight
or volume basis – these are not equal because the specific gravities of
these materials are not equal to that of cement. Reducing water content
by using water-reducing admixtures also reduces the cement content
required for the same w/c ratio.
• Estimate the coarse aggregate content. This depends on the maximum
size of the coarse aggregate and the FM (or lubricating potential) of the
sand. With larger coarse aggregates, a larger volume of coarse aggre-
gate is used, as the larger aggregate particles replace smaller coarse
aggregate, fine aggregate, and cement paste. With lower FM fine aggre-
gate, more coarse aggregate may be used because less fine aggregate is
required to lubricate the mixture and provide workability.
• Estimate the fine aggregate content. At this point the masses of water,
cement, other cementituous materials, and coarse aggregate are known.
Using the respective specific gravities, the volumes of these materials per
cubic meter or cubic yard are known, plus the percent air. Everything
else in the concrete volume has to be fine aggregate. The volume of
fine aggregate and the specific gravity of the fine aggregate are used to
determine the mass.
• Adjust for aggregate moisture. The mixing water estimates developed
earlier are on the basis of SSD aggregate. If the aggregate has surface
moisture, it will add water to the mixture, and a larger quantity of
wet aggregate will be needed. If the aggregate is dry, it will subtract
• Prepare a trial batch. The batch weights determined up to this point
are estimates that need to be verified in the laboratory. Water-and air-
entraining admixtures will need to be adjusted to achieve the correct
slump and air content. Unit weight should be verified to determine the
Mixture design and proportioning 113
yield of the mixture. Trial batches are important – the steps outlined up
to this point represent the starting point and not the end of determining
a satisfactory mixture.
Recently, ACI Committee 211 has published the Guide for Selecting Pro-
portions for No-Slump Concrete, 211.3R-02 (ACI Committee 211 2002).
This document covers mixtures with slump less than 25 mm (1 in), includ-
ing roller compacted (appendix 3) and pervious concrete (appendix 6). The
charts provided in this document are limited to a maximum aggregate size
of 38 mm (11/2 in). This document does not appear to address conventional
paving concrete, which is generally proportioned by the methods previously
For paving concrete, the water and paste content should be minimized to
reduce shrinkage. A total water content of less than 145 kg/m3
and a total paste volume of less than 60 percent are preferred (Hall et al.
2005: 22). This may require the use of water-reducing admixtures. As
noted earlier, an optimized aggregate gradation also reduces the water
Workability refers to ease of placing, consolidating, and finishing freshly
placed concrete without segregation. Although it is often addressed by slump
test measurements, this rapid, cheap, and simple test does not measure all
of the factors that are necessary for satisfactory workability. For slipformed
concrete pavements, factors affecting workability include:
• segregation during transportation and placement;
• ease of consolidation;
• well-formed slipformed edges with little or no edge-slump;
• minimal or no hand finishing required (Kohn and Tayabji 2003: 57).
The desired slump is used to select the water content for trial batches,
following the procedure outlined above. Slipformed concrete needs to be
stiff enough to stand up on its own without the edges slumping as it emerges
from the paver, so typical slumps are 25–50 mm (1–2 in) or less. Edge-
slump often indicates too much water in the mixture. The slump of concrete
for fixed form paving may be higher.
Although workability is thought of as being governed principally by water
content, other factors also affect it:
• Aggregate – Size, grading, particle shape, water demand, variability.
• Cement – Cement content, water demand.
114 Mixture design and proportioning
• Fly ash (if used) – Effect on initial set, water demand, effect on
• Slag cements and GGBFS – Effect on finishing and saw cutting.
• Water – Total water demand.
• Admixtures – Air entrained concrete exhibits better workability;
water reducers reduce water demand while improving workability.
(Kohn and Tayabji 2003: 57)
Both ACI 211.1 and 211.3 use required compressive strength to select a
w/c or w/cm ratio. ACI 211.3 (ACI Committee 211 2002: 5–6) states that
“If flexural strength is a requirement rather than compressive strength, the
relationship between w/cm and flexural strength should be determined by
laboratory tests using the job materials.”
As a general rule of thumb, flexural strength is on the order of 10 percent
of compressive strength of concrete. It is relatively higher with crushed
aggregates, which provide better bond, and lower with rounded aggregates
such as gravel.
The historic emphasis on strength, however, will not necessary lead to
good pavement performance. “As Hardy Cross once wrote: Strength is
essential but otherwise not important” (Murray 2000: 30). Although Pro-
fessor Cross was most likely speaking of structural concrete, his statement
is even more true of concrete pavement. It can probably be stated with con-
fidence that no concrete pavement has ever failed in compression, although
it is possible that thin pavements subjected to overloads have failed in flex-
ure or in punching shear. In fact, many problems have been caused by the
addition of too much cement to paving concrete in a misguided attempt to
Concrete pavements are designed for fatigue. “Fatigue is the degradation
of a material’s strength caused by a cyclically applied tensile load that is
usually below the yield strength of the material. Fatigue is a concern because
a material designed to withstand a safe load one time may fail when the
same load is applied cyclically one time too many. The cyclically applied
load causes a crack to initiate and propagate from the areas of highest
stress concentrations. The material finally fails when the crack grows to
a sufficient length so that applied load causes a stress that exceeds the
material’s ultimate strength” (Titus-Glover et al. 2005: 30).
Design for fatigue is based on a stress ratio (SR) between traffic-induced
stress and the flexural strength of the concrete.
SR = /MOR (6.1)
where = load-induced tensile stress in the concrete, and MOR = modulus
of rupture or flexural strength of the concrete. At a stress ratio at or near
Mixture design and proportioning 115
one, the concrete will fail after very few cycles. With a low SR, many load
applications may be made.
Flexural strength of concrete, or MOR, is determined using a third point
(ASTM C78 2002) or center point (ASTM C293 2002) bending test. The
beams tested are 150 × 150 × 500 mm 6 × 6 × 20 in . Third point testing
(ASTM C78 2002) is preferred because the center third of the beam is in
pure bending, with no shear. Some agencies use center point testing instead
(ASTM C293 2002). Third point testing gives lower but more consistent
flexural strengths than center point testing (Mindess et al. 2003: 379). Other
tests that can be used include splitting tensile strength (ASTM C496 2004)
and compressive strength (ASTM C39 2005).
The test method used for concrete acceptance varies by agency. According
to the ACPA database of state practices as of 1999, 12 states used flexural
strength for acceptance of concrete, with nine of those using third point and
three using center point loading. One state used both third point flexural and
compressive strength. Of the others, 21 states used compressive strength,
and one state used splitting tensile strength. For US states using flexural
strength testing, the required MOR ranges between 3,100 and 4,500 kPa
(450 and 650 psi), measured at 7, 14, or 21 days (ACPA 1999c).
FAA requires a minimum allowable flexural strength of 4,136 kPa
(600 psi) at 28 days for airport pavements, although individual project spec-
ifications may be set higher. For pavements carrying only lighter aircraft,
gross weight limit 13,500 kg (30,000 pounds), 28-day compressive strength
may be used for acceptance with a minimum of 30.7 MPa (4,400 psi).
Requirements are provided by item P-501, Portland Cement Concrete Pave-
ment, of Standards for Specifying Construction of Airports, AC 150/5370-
10B (FAA 2005: P-501-8).
It should be noted that the MOR used for acceptance and the MOR used
for design are almost certainly not the same. Because any concrete below the
required MOR may be rejected, the contractor will furnish concrete with
a higher strength. Also, testing may be done as early as 7 days to provide
early feedback to the contractor and the engineer, but the fatigue life of the
pavement extends over decades. Therefore, a higher MOR should be used
for pavement design than for concrete acceptance.
For a given SR, a certain number of load repetitions are predicted before
the pavement fails in flexural fatigue. The following fatigue equations were
developed by Packard and Tayabji (1985) for the PCA design procedure
For SR ≥ 0 55 logNf = 11 737 −12 077 SR (6.2)
For 0 45 < SR < 0 55 Nf =
SR −0 4325
And for SR ≤ 0 45, the number of repetitions is unlimited.
116 Mixture design and proportioning
To achieve a longer fatigue life for a pavement, the SR should be reduced.
This is achieved either by reducing the flexural stress in the pavement for a
given load (by making it thicker) or by increasing the MOR.
To combine the fatigue effects of different loading magnitudes and con-
figurations, the SR from each vehicle is determined. Next, fatigue equations
such as 6.2 are used to calculate the allowable number of repetitions Nf
for each SR. Finally, Miner’s fatigue hypothesis is applied to sum up the
cumulative damage function (CDF) for fatigue:
Where i = the number of load groups or configurations, ni = the actual or
projected number of repetitions of load group i, and Nfi = the allowable
number of repetitions for load group i. The ratio ni/Nfi represents the
fraction of the pavement fatigue life consumed by load group i. The CDF
may be expressed as a ratio, in which case it must be ≤1 0, or it may be
multiplied by 100 and expressed as a percent.
A new concrete pavement fatigue model was developed for the ACPA
StreetPave concrete pavement design computer program. The main enhance-
ments were the inclusion of additional fatigue data that has become avail-
able since equation 6.2 was developed, and the inclusion of a reliability
parameter. The stress ratio and cumulative damage remain as defined in
equations 6.1 and 6.4. The revised fatigue expression is:
where P = probability of failure and therefore 1−P = probability of sur-
vival, and other variables are as previously defined. The fatigue relationships
represented by equations 6.2 and 6.5 are compared in Figure 6.1.
It was found that the PCA fatigue equation 6.2 is equivalent to approxi-
mately 90 percent reliability, which indicates that only 10 percent of pave-
ments should fail before the end of design life (Titus-Glover et al. 2005).
The StreetPave program is discussed in detail in Chapter 9.
For pavements, durability is almost certainly a more important issue than
strength. Pavements are exposed outside, often in harsh environments. In
areas such as the author’s home in Northeast Ohio, pavements, bridges, and
other infrastructure are routinely bathed in harsh deicing materials during
the winter. There are very few civil engineering materials that have their
properties improved by repeated treatments of brine, particularly during
Mixture design and proportioning 117
100 1,000 10,000 100,000 1,000,000 10,000,000 100,000,000
Number of repetitions
80 % reliability
50 % reliability
90 % reliability
70 % reliability
95 % reliablity
Figure 6.1 Comparison of PCA 1984 and StreetPave fatigue relationships.
repeated cycles of freezing and thawing. Freeze-thaw cycles and chlorides
present significant challenges for pavement durability. In addition to using
durable aggregates, a low w/c or w/cm ratio should be used. This ratio may
be lower than that required for strength.
Repeated cycles of freezing and thawing can damage concrete over time
unless it has a well-distributed system of finely divided air voids. The air
is entrained using the air-entraining admixtures discussed in Chapter 5.
Although the air void system in the hardened concrete is important, gen-
erally the total air content of fresh concrete is measured. The proper air
content may be determined using the tables in ACI 211.1 (ACI Committee
211 1991). It is possible to evaluate the air void system of hardened con-
crete using petrographic analysis, but this is expensive and rare except for
large projects or as part of forensic investigations.
118 Mixture design and proportioning
Kohn and Tayabji (2003: 60) note:
• Trial batches are necessary to determine the proper amount of air
• The concrete for the trial batch should be allowed to sit for an amount
of time representative of the haul to the project site, because 1 or 2
percent of the air may be lost during the haul.
• Increasing air content reduces concrete strength if other factors
• Slipform paving can reduce the air content 1 or 2 percent during con-
The freeze-thaw durability of roller compacted and pervious concrete
remains an issue of concern. ACI 211.3 (ACI Committee 211 2002: 13)
Although the resistance of RCC to deterioration due to cycles of freezing
and thawing has been good in some pavements and other structures,
RCC should not be considered resistant to freezing and thawing unless
it is air-entrained or some other protection against critical saturation
is provided. If the RCC does not contain a sufficiently fluid paste,
proper air entrainment will be difficult, if not impossible, to achieve.
In addition, a test method for measuring the air content of fresh RCC
has not been standardized.
This contrasts with the observations of Piggott (1999) on the favorable
long-term performance of RCC in cold regions.
On pervious concrete, ACI 211.3 (ACI Committee 211 2002: 25)
Freezing-and-thawing tests of pervious concrete indicate poor durability
if the void system is filled with water. Tests have indicated that dura-
bility is improved when the void structure is permitted to drain and the
cement paste is air-entrained. No research has been conducted on resis-
tance of pervious concrete to the aggressive attack by sulfate-bearing or
acidic water that can percolate through the concrete. Therefore, caution
should be used in applications where aggressive water may exist.
Therefore, the key is to ensure that the pervious concrete is not saturated
during freezing weather. The National Ready Mixed Concrete Association
(NRMCA) report Freeze Thaw Resistance of Pervious Concrete defines
three different exposure conditions – dry freeze and dry hard freeze, wet
freeze, and hard wet freeze. In dry freeze and dry hard freeze areas, such
as many high areas of the Western US, a 100–200 mm (4–8 in) layer of
Mixture design and proportioning 119
clean aggregate base should be provided under the pervious concrete. Wet
freeze areas, such as the middle part of the Eastern US, should use the same
precaution. Possible safeguards in the wet hard freeze areas (subjected to
long continuous periods below freezing) include a 100–600 mm (4–24 in)
layer of base, air entrained paste, and/or perforated PVC drainage pipes. A
pervious concrete pavement at Pennsylvania State University, in the hard
wet freeze area, has performed well over five winters (NRMCA 2004, ACI
Committee 522 2006).
Mindess et al. (2003: 505) note that “the use of an adequately air-entrained,
low w/c ratio, low permeability concrete is the best protection against salt
scaling.” These are the same mixture considerations needed to provide
freeze-thaw durability. As noted earlier, construction practices also have an
important effect on scaling.
Deicer-scaling resistance of concrete is greatly improved when these
fundamentals are followed:
1. Minimum cement content – 564 lb per cubic yard (335 kg per
2. Maximum water-cementitious materials ratio – 0.45
3. Low slump – not more than 4 in (100 mm) (unless a water reducer
4. Sound, clean, durable, well-graded aggregate
5. Adequate air void system
6. Proper proportioning, mixing, placing, and finishing.
(ACPA 1992a: 1)
Two other important elements are adequate curing and a period of air
drying. Curing is discussed in Chapter 15. A period of air drying greatly
improves scaling resistance – the pavement should be allowed to dry 30 days
before de-icers are used, although earlier exposure is possible for concrete
with w/c of 0.40 or less (ACPA 1992a).
Kohn and Tayabji (2003: 59) point out that “if the soils or groundwa-
ter contain sulfates, the cementitious material(s) need to be appropriately
resistant to sulfate attack and the water/cementitious materials ratio needs
to be reduced appropriately.” Appropriate cementitious materials include
pozzolans, slags, and cement with low C3A content. Type V cement has the
lowest C3A limit, followed by type II.
120 Mixture design and proportioning
Corrosion of reinforcement and dowel bars
Traditionally reinforcement and dowel bars for concrete pavements have
been made from mild steel, which is subject to corrosion. In areas subject
to freezing and thawing, epoxy coated dowels and reinforcement are now
often used. Epoxy coated dowels and tie bars are shown in Figures 2.4
Snyder (2005) investigated the use of passive cathodic protection to pro-
tect dowel bars and reported extensive test results. This system uses a
1.2 mm (50 mil) zinc sleeve mechanically bonded to a carbon steel dowel.
The zinc sleeve acts as both a barrier to corrosion and a sacrificial anode for
cathodic protection. These dowels were also evaluated through four million
cycles in an accelerated loading facility and provided load transfer efficiency
comparable to conventional dowels, indicating that the zinc coating did not
inhibit performance. Corrosion of unprotected carbon steel dowels seems
to be an important contributor to poor joint performance. This may be
manifested in joint lockup and failure of adjacent joints, and mid-panel
cracks. Other protection techniques, such as barrier techniques, corrosion
resistance, and non-corroding dowels, were found to be either ineffective
or prohibitively expensive. Although conventional dowels are probably sat-
isfactory for pavements with projected service lives on the order of 20
years, zinc coated dowels provide an alternative worthy of consideration
for long-life (e.g. 50 year) pavements.
Shrinkage and thermal deformation
The contraction and expansion of concrete pavement slabs due to shrink-
age and thermal effects are important for performance. Both the absolute
deformation and the relative deformation between the top and the bot-
tom of the slab are important. The absolute deformation, due to uniform
strain through the thickness of the slab, determines how much joints open
and close, and restrained contraction due to friction between the slab and
subbase or subgrade causes tensile stress in the slab.
Strain gradients due to temperature are called curling, and those due
to moisture are called warping. These cause cupping upward or downward
of the slab. Where the slab lifts off the subbase, it is poorly supported.
This can lead to corner breaks as shown in Figure 3.1, particularly for
During the daytime, the top of the slab is warmer than the bottom, and
the slab curls downward. The slab curls upward at night, and if the corners
lift off the subbase there is an increased risk of corner breaks. The slab goes
through one complete cycle in 24 hours.
Differential moisture changes in the concrete slab cause warping. During
curing of the concrete, it is generally easier for moisture to escape from the
Mixture design and proportioning 121
top of the slab than the bottom, and differential drying shrinkage leads to
a permanent upward cupped distortion of the slab, sometimes referred to
as “built-in curl” although “built-in warp” is a more accurate term.
Drying shrinkage and thermal deformations should both be minimized.
Since drying shrinkage occurs in the cement paste, the amount of paste
should be reduced by using larger maximum size coarse aggregate (if avail-
able and not subject to D-cracking) and by blending the aggregate to achieve
a dense gradation. The drying shrinkage of the paste itself may be mini-
mized by using the lowest possible water content, possibly through use of
water reducers. Thermal deformations are reduced by using aggregate with
a low coefficient of thermal expansion.
Some factors that influence shrinkage and premature cracking include
high water demand, gradation of combined aggregates, and the type
of coarse aggregate. High cement contents (more than 295 kg/m
) and fine sands (FM lower than 3.1) may increase water
demand. Aggregate gradation affects workability and amount of paste. Dif-
ferent coarse aggregates have different thermal coefficients, affecting ther-
mal deformations and temperature sensitivity. Also, some admixtures such
as calcium chloride as an accelerator and water reducers with accelerators
may increase drying shrinkage (Hall et al. 2005: 19–20).
Mixture proportioning example
Two sample mixture proportions are shown below. The first uses 38 mm (1
1/2 in) maximum size coarse aggregate, and the second uses 19 mm (3/4 in)
coarse aggregate. If available, the larger size coarse aggregate will reduce
Large size coarse aggregate
1 Required information: type I cement with a specific gravity of 3.15; fine
aggregate bulk specific gravity SSD = 2 63, fineness modulus 2.70;
coarse aggregate maximum size 38 mm (11/2 in), bulk specific gravity
(SSD) 2.68, dry-rodded unit weight 1 600 kg/m3
ment is 250 mm (10 in) thick. Required 28-day flexural strength is
4.1 MPa (600 psi) roughly corresponding to a compressive strength
of 31 MPa (4,500 psi) based on experience with local materials. The
pavement will be subject to freezing and thawing.
2 Choose slump: for slipform paving, slump is 25–50 mm (1–2 in).
3 Choose maximum aggregate size: 38 mm (11/2 in) is less than one-third
of 250 mm (10 in).
4 Estimate mixing water and air content: from ACI Committee 211
(1991) tables, mixing water is 145 kg/m3
. Mixing water
122 Mixture design and proportioning
may be reduced if water-reducing admixtures are used. Air content for
severe exposure conditions is 5.5 percent.
5 w/c ratio: from ACI Committee 211 (1991) tables, a w/c ratio of 0.44
is necessary to achieve the desired strength. The maximum permissible
w/c ratio based on durability is 0.50, so 0.44 should be used.
6 Calculate cement content: divide the water by the w/c ratio to get the
cement content of 330 kg/m3
7 Estimate coarse aggregate content: from ACI Committee 211 (1991)
tables, cross-index the maximum coarse aggregate size with the fineness
modulus of sand to find a volume of dry-rodded coarse aggregate per
unit volume of concrete of 0.73. Multiply this by the dry-rodded unit
weight of the coarse aggregate to obtain 1 168 kg/m3
1 971 lb/yd
8 Estimate the fine aggregate content: determine the volume of each
constituent material by dividing it by its unit weight. The constituent
materials so far add up to 0.74 cubic meter (20.1 cubic feet), so
the remainder, or 0.26 cubic meter (6.9 cubic feet) must be fine
aggregate. Multiply by the unit weight of fine aggregate to obtain
1 131 lb/yd
9 Adjust for aggregate moisture: the water, coarse aggregate, and fine
aggregate weights must be adjusted if the aggregates are not in SSD
10 Prepare and test trial batches.
Normal size coarse aggregate
Design for 19 mm (3/4 in) aggregate is adapted from Mindess et al. (2003:
1 Required information is the same except for the maximum aggre-
2 Slump is the same.
3 Maximum aggregate size is less than one-third of the pavement thick-
4 Estimate mixing water and air content: from ACI Committee 211
(1991) tables, mixing water is 165 kg/m3
. Mixing water
may be reduced if water-reducing admixtures are used. Air content for
severe exposure conditions is 6 percent. More water is required with
smaller size coarse aggregate.
5 w/c ratio is the same.
6 Calculate cement content: with more water and the same w/c ratio, more
cement will be necessary. The cement content 375 kg/m3
for an increase of 45 kg/m3
7 Estimate coarse aggregate content: from ACI Committee 211 (1991)
tables, cross-index the maximum coarse aggregate size with the fineness
Mixture design and proportioning 123
modulus of sand to find a volume of dry-rodded coarse aggregate per
unit volume of concrete of 0.63. Multiply this by the dry-rodded unit
weight of the coarse aggregate to obtain 1 008 kg/m3
1 701 lb/yd
8 Estimate the fine aggregate content: the constituent materials so far add
up to 0.72 cubic meter (19 cubic feet), so the remainder, or 0.28 cubic
meter (8 cubic feet) must be fine aggregate to make one cubic meter
(one cubic yard, 27 cubic feet) of concrete. Multiply by the unit weight
of fine aggregate to obtain 736 kg/m3
1 307 lb/yd
9 Adjust for aggregate moisture: the water, coarse aggregate, and fine
aggregate weights must be adjusted if the aggregates are not in SSD
10 Prepare and test trial batches.
Comparison with the previous example shows that with the smaller coarse
aggregate, more water and cement are needed. This will add to the cost of
the mixture, and increase shrinkage.
Batch adjustments for aggregate moisture condition
Continuing the previous example, assume that the coarse aggregate has
a surface moisture of 0.5 percent and the fine aggregate has a surface
moisture of 4.2 percent. Unless the quantities are adjusted, the concrete
mixture will have too much moisture, the slump will be too high, and the
strength and durability will be reduced. Therefore, the coarse aggregate
weight must be multiplied by 1+ surface moisture/100 percent, or 1.005, to
get 1 013 kg/m3
1 710 lb/yd
of the wet coarse aggregate. Similarly, the
fine aggregate must be multiplied by 1.042 to get 766 kg/m3
1 263 lb/yd
of the wet fine aggregate. Now, since 5 kg/m3
of the wet coarse
aggregate and 31 kg/m3
of the wet fine aggregate batched is
actually water, this must be subtracted from the mixing water added. There-
fore, the batch water becomes 129 kg/m3
. The moisture con-
dition of the aggregate must be monitored, and if it changes the proportions
must be adjusted again.
Batch adjustments for supplementary cementitious
If a portion of the cement is replaced by supplementary cementitious mate-
rials, the replacement may be in terms of either mass or volume, although
mass is commonly used. Since supplementary cementitious materials have
a different (usually lower) specific gravity from cement, the fine aggregate
content will also be adjusted (Mindess et al. 2003: 230–231).
As an example, assume that the 19 mm (3/4 in) aggregate mixture dis-
cussed above is to be modified for a 30 percent replacement of cement
124 Mixture design and proportioning
with fly ash with a specific gravity of 2.4. The new cement content is
. The mass of fly ash is 30 percent of the total
cementitious material, or 113 kg/m3
However, with a lower specific gravity the fly ash occupies a larger vol-
ume than the cement it replaces. The new cement volume is 0.083 cubic
meter (2.97 cubic feet) and the fly ash volume is 0.047 cubic meter
(0.97 cubic foot).
The coarse aggregate content is unchanged. This increases the vol-
ume of all of the constituents except the fine aggregate to 0.73 cubic
meter (19.7 cubic foot) so the volume of sand is reduced to 0.27 cubic
meter (7.3 cubic foot). Therefore, the revised weight of the sand will be
1 191 lb/yd
. With a fly ash replacement, trial batches become
important because the fly ash increases workability and it will probably be
possible to remove some water from the mixture.
Batch adjustments for water reducing admixtures
Adjustments for water-reducing admixtures are a little simpler. For exam-
ple, consider the adjustment of the original 19 mm (3/4 in) aggregate mixture
(with cement only) with a 10 percent reduction in water due to the use of
a low or mid-range water-reducing admixture. The batch water is reduced
to 149 kg/m3
. The cement content may now be reduced to
As with the adjustment for supplementary cementitious materials, the
coarse aggregate content is unchanged. This reduces the volume of all of
the constituents except the fine aggregate to 0.69 cubic meter (18.7 cubic
foot) so the volume of sand is reduced to 0.31 cubic meter (8.3 cubic foot).
Therefore, the revised weight of the sand will be 808 kg/m3
1 360 lb/yd
Once again, trial batches are necessary to evaluate the properties of the
Often it is necessary to repair or reconstruct concrete pavements in ser-
vice within very narrow time windows. In many cases, closure windows
may be overnight or over a weekend. Van Dam et al. (2005) refer to
concrete pavement mixtures that may be opened to traffic after short clo-
sures as early-opening-to-traffic (EOT) concrete. One important reference
on accelerated concrete pavement construction is ACI 325.11R Accelerated
Techniques for Concrete Paving (ACI Committee 325 2001). Another ref-
erence on the topic is Fast-Track Concrete Pavements, Technical Bulletin
TB004.02 (ACPA 1994a).
For airports under the FAA jurisdiction, item P-501-4.18, Portland
Cement Concrete Pavement, of Standards for Specifying Construction of
Mixture design and proportioning 125
Airports, AC 150/5370-10B (FAA 2005: P-501-25) requires a flexural
strength of 3,792 kPa (550 psi), or a wait of 14 days before opening the
pavement to traffic. For lighter load airfields using compressive strength,
the requirement is 24.13 MPa (3,500 psi). In airport construction, high
early strength concrete may be necessary for bridging areas where taxiways
cross or high traffic volume apron areas (Kohn and Tayabji 2003: 58).
If the facility can be closed down for a few days, even three or four,
then it will often be found that conventional concrete will achieve sufficient
strength and no special mixtures or materials will be necessary. In one
case, the construction of a new runway at Cleveland Hopkins International
Airport in Cleveland, Ohio, two concrete mixtures were developed. A high
early strength concrete was proposed for critical tie-ins to existing runways
and taxiways. Early in the project, problems were encountered with the use
of high early strength concrete, and it was found that with careful scheduling
the conventional concrete could be used for all construction, including the
tie-ins. Use of the conventional mixture simplified the construction (Peshkin
et al. 2006a,b).
For an overnight closure window, where the facility is closed in early evening
and reopened in early morning, the concrete must achieve adequate flexural
strength to carry traffic in 6–8 hours. The narrow closure window must
incorporate removal of existing pavement as well as placement and curing
of the new pavement. Typical specifications require either a compressive
strength of 8.3–24 MPa (1,200–3,500 psi) or a flexural strength of 1.8–
2.8 MPa (260–400 psi) (Van Dam et al. 2005: 9). Airports may require
5–7 MPa (750–1,000 psi) compressive strength at 4–6 hours for overnight
construction (Kohn and Tayabji 2003: 58).
Overnight closures are complicated by the fact that these are typically
pavements carrying heavy traffic, with heavy user costs and delays due to
construction. For freeways and toll roads, often only overnight closures are
Occasionally airport pavement reconstruction is limited to overnight clo-
sures. The airports in Charleston, South Carolina, and Savannah, Georgia,
each have two runways that cross. When the runway intersections needed
to be repaired, there were no alternate runways to handle aircraft. The
Charleston project in 1990 and the Savannah project in 1996 used similar
techniques. During short overnight closures, individual slabs were removed
and replaced with very fast setting concrete. If the concrete could not be
placed and cured in time, precast panels were installed as a temporary
pavement and removed during a subsequent closure. All of the pavement
slabs in the intersection were replaced during multiple overnight closures,
126 Mixture design and proportioning
allowing daytime aircraft traffic to continue uninterrupted. Complete case
study details are provided by Peshkin et al. (2006a,b).
Van Dam et al. (2005: A-1–A-2) provide examples of three mixture
designs that provided good performance for 6–8 hour EOT concrete as well
as three for 20–24 hour EOT concrete. These are shown in Table 6.1.
Many 6–8 hour EOT mixtures in the past have relied on proprietary
cements, but satisfactory mixtures may be made with conventional cement.
Degussa admixtures has developed a patented system 4 × 4™ to achieve
2.8 MPa (400 psi) at 4 hours. The system uses either type III cement or a
very reactive type I or I/II cement, plus extended set-controlling admixtures
to allow the mixture to be placed and consolidated and a non-chloride
accelerating admixture. The system was first employed by the California
Department of Transportation (CALTRANS) and has since been employed
for Interstate Highways in California, Alabama, and West Virginia, as well
as the Philadelphia International Airport (Bury and Nmai 2005).
For weekend closures, concretes that achieve the required flexural strength
in 20–24 hours are satisfactory. These are typically larger projects and
involve more construction and more demolition. Examples of mixture
designs that provide satisfactory performance under these conditions are
shown in Table 6.1. Opening strength requirements are typically the same
as those for overnight closures, but more time is available to achieve them.
Airports may require 14–21 MPa (2,000–3,000 psi) compressive strength
at 24 hours for overnight construction (Kohn and Tayabji 2003: 58).
Durability of EOT concrete
The durability issue presents a serious problem, because those pavements
that are so heavily trafficked that only short closure windows are available
are precisely those pavements that need to have durable concrete. Van Dam
et al. (2005: 19) note that “In comparison with 20- to 24-hour EOT con-
crete, 6- to 8-hour EOT concrete will have higher cement contents and lower
w/c ratios. Type III cement, accelerators, and water reducers are more often
used in 6- to 8-hour EOT concrete than in 20- to 24-hour EOT concrete. It
was clearly observed from the laboratory test results that the 6- to 8-hour
mixtures had less desirable durability characteristics than the 20- to 24-hour
mixtures. This observation was reflected in the overall poorer performance
in freeze-thaw and scaling tests, increased shrinkage, increased difficulties
in achieving desirable air-void system characteristics, increased amounts
of paste microcracking, decreased paste homogeneity, and increased
absorption. This is not to suggest that durable 6- to 8-hour EOT
concrete mixtures cannot be made; it simply points out the difficulty
Table 6.1 Sample concrete mixture designs for early opening to traffic (Van Dam et al.
Mixtures 1, 2, and 3, all of which were made using a vinsol resin air-entraining agent, provided good
performance for six- to eight-hour EOT concrete
Constituent/property Mixture 1 Mixture 2 Mixture 3
Type I cement 525 kg/m3
w/c ratio 0.40 0.36 0.40
Accelerator type Non-chloride Non-chloride Calcium chloride
Water reducer None None None
Fine aggregate (natural
Average slump 140 mm (5.5 in) 70 mm (2.75 in) 65 mm (2.5 in)
Average air content 5% 5% 5.6%
2.4 MPa (350 psi) 3.0 MPa (435 psi) 2.4 MPa (350 psi)
Mixtures 4, 5, and 6, all of which were made using a vinsol resin air-entraining agent, provided good
performance for 20- to 24-hour EOT concrete
Constituent/property Mixture 4 Mixture 5 Mixture 6
Type I cement 400 kg/m3
w/c ratio 0.43 0.40 0.43
Accelerator type Calcium chloride Non-chloride None
Water reducer None None None
Fine aggregate (natural
Average slump 85 mm (3.35 in) 50 mm (2 in) 150 mm (6 in)
Average air content 6.6% 5.7% 5.9%
3.4 MPa (490 psi) 3.8 MPa (550 psi) 3.6 MPa (520 psi)
128 Mixture design and proportioning
in achieving the desired characteristics of a durable mixture in these higher
early strength mixtures. Thus, there is a higher level of risk associated with
using a 6- to 8-hour EOT concrete than a 20- to 24-hour EOT concrete
that must be considered when selecting a specific mixture to reduce lane
closure time.” This suggests that if six- to eight-hour EOT concrete is to be
used, there should be extensive preliminary testing to ensure durability.
One example of poor durability of EOT concrete occurred at Houston
Hobby Airport in Texas. The intersection of runways 4-22 and 12R-30L
at Houston Hobby airport is heavily used and closures for repairs of this
area must be limited because of the impact on commercial operations: the
intersection carries 95 percent of the total aircraft traffic at the airport.
When the intersection is closed, Hobby has only one visual flight rules
(VFR) runway that can handle air carrier operations, and even short periods
of rain or fog shut down the airport.
The intersection was repaired in 16 days in 1994 using very high early
strength concrete. The original 150 mm (6 in) thick runway pavement at
the time of this repair was more than 50-years old and had been over-
laid several times to increase the section by 450 mm (18 in). The project
concrete consisted of significant quantities of type III cement and fly ash,
with a superplasticizer and an accelerating admixture. The specified flexural
strengths were 5.2 MPa (750 psi) at 24 hours and 5.9 MPa (850 psi) at 28
days. The 24-hour strength was much higher than the typical requirement
at 28 days. Because the original amount of accelerator used was too great
and the concrete lost workability before finishing could be completed, the
amount of accelerator was reduced, leading to decreased 24-hour strengths.
By the late 1990s, this repaired area had experienced significant deterio-
ration, resulting in operational warnings to pilots and emergency closures
for repairs. The problem was initially identified through pilot complaints
about rideability problems on runway 12R-30L. Although the center line
profile was smooth, the wheel track profiles for the main gear had an
abrupt transition to 1 percent slopes. Observed distresses included surface
cracking, differential joint movement, concrete expansion and shoving, and
full depth and lateral cracking. A forensic investigation found that the con-
crete used in the project had produced delayed ettringite crystal formations,
which expanded the volume of the concrete pavement. The movement was
so great that several light bases in the intersection were damaged by shear-
ing forces as the pavement expanded and slid relative to the base. Asphalt
adjacent to the intersection was cracked and heaved due to the pressure of
the expanding concrete (Sarkar et al. 2001).
Concrete pavement design is often thought of solely in terms of thickness
design, but there are other important elements. These include the type and
spacing of joints (if any) – both transverse joints for JPCP and longitudinal
joints for all pavement types. The design of the drainage system has been
discussed previously in Chapter 4.
Theoretical analysis of a concrete pavement is a surprisingly daunting
task: geometric and joint issues, material shrinkage factors, environ-
mental effects on the structure, uncertain in-situ material properties
and strengths, complex nonlinear material response, perplexing fatigue
behavior, moving loads, etc. Consequently, pavement design has tended
to evolve with relatively simple analytical and material models, and a
number of empirical and experience-based guidelines on joints, pacing,
etc. that tend to work and keep us out of trouble.
(Rollings 2005: 170)
“Any of the major designs – plain, reinforced, continuously reinforced, or
prestressed – will give good performance if the subgrade, subbase, jointing,
and use of steel, if any, are properly considered and provided for in the
design, and if traffic is reasonably well forecast” (Ray 1981: 8).
The determination of pavement thickness requirements is a complex
engineering problem. Pavements are subject to a wide variety of load-
ing and climatic effects. The design process involves a large number
of interacting variables, which are often difficult to quantify. Despite
considerable research on this subject, it has been impossible to arrive
at a direct mathematical solution for thickness requirements. For this
reason, pavement engineers must base pavement thickness on a theo-
retical analysis of load distribution through pavements and soils, the
analysis of experimental pavement data, and a study of the performance
of pavements under actual service conditions.
(FAA 2005: 23)
130 Design fundamentals
Any transitions between concrete pavement and adjacent asphalt pavement
sections or bridges should also be carefully designed. For CRCP pavements,
the design also includes the selection of the steel percentage, by volume.
CRCP reinforcement, transitions, and other special details are discussed in
Pavement support is generally reduced to a k-value, based on the soil
type. Table 4.1 may be used to select a k-value for the subgrade soil,
and Tables 4.2 through 4.5 may be used to adjust the value based on an
untreated aggregate or stabilized subbase.
While it is conservative to use a low k-value for thickness design, it is
not conservative to use a low value to determine joint spacing. Therefore,
if a stiff stabilized layer is used under the pavement – CTB, ATB, etc. – a
higher k-value must be used for joint spacing determination.
For most concrete pavement design procedures, the thickness of the pave-
ment is not very sensitive to the k-value. This is in contrast to flexible or
asphalt pavements, where thickness is highly dependent on the soil stiff-
ness. Therefore, the subgrade and subbase materials are not particularly
important for determination of pavement thickness, but are very impor-
tant for constructability, pumping, and frost susceptibility. These issues are
addressed in Chapters 4 and 13.
There are three approaches to dealing with traffic for pavement design. The
simplest, by far, is if only one vehicle type needs to be considered in the
design. If a mixed traffic stream must be considered, then the effects of
different axle groups may be considered separately, or all axle groups may
be converted to equivalent 80 kN (18 kip) single axles.
For some pavements, primarily airfield or industrial pavements, it may be
possible to use a single vehicle approach. This method is valid if a single
heavy vehicle or aircraft type dominates the traffic stream, and other loads
on the pavement are so light that they cause minimal damage. This is the
case if the lighter loads are not more than about 80 percent of the design
To design for a single vehicle, the pavement flexural stress for a trial
pavement thickness is determined. Next, the flexural stress is divided by the
modulus of rupture to obtain the stress ratio SR, and fatigue models such
Design fundamentals 131
as equation 6.2 or 6.5 are used to find the allowable number of repetitions.
The trial pavement thickness is then adjusted until the design will carry the
projected number of load repetitions.
Mixed traffic stream
Most highways and airports carry mixed traffic streams, and the single
vehicle assumption cannot be used. If this is the case, the design approach
adopted by the 1984 PCA method may be used. This design procedure
calculates the pavement damage caused by each vehicle type in the traffic
stream, and then adds up the damage over the projected life of the pavement
to ensure that it does not exceed some allowable value.
First, a trial pavement thickness is assumed. Next, the damage caused by
each type of vehicle in the mixed traffic stream is calculated, based on the
expected number of load repetitions for that vehicle type over the projected
life of the pavement. For highways, vehicles are typically grouped by type
(single, tandem, or tridem/triple axle) into 8.9 or 17.8 kN (2,000 or 4,000
Damage due to each vehicle increment is then added up and compared
to allowable maximums. For the 1984 PCA method, the limits are 100
percent fatigue damage and 100 percent erosion damage, computed using
equation 6.4. Either fatigue or erosion may determine the design thickness
The NCHRP/AASHTO M-EPDG applies a similar but significantly more
sophisticated approach. Damage is calculated for each load group over each
season. Total damage over the life of the pavement is then compared to
allowable maximums for transverse cracking, joint faulting, etc., and then
the design is adjusted if necessary (Applied Research Associates 2006).
For airport pavements, only a limited number of types of aircraft need
to be considered. The number of repetitions or coverages per type may be
predicted fairly accurately. The predicted air traffic is not likely to change
significantly, unless there is a change of airline tenants.
The FAA Advisory Circular Airport Pavement Design, AC 150/5320-6D
states that “the pavement design method is based on the gross weight of the
aircraft. The pavement should be designed for the maximum anticipated
takeoff weight of the aircraft. The design procedure assumes 95 percent of
the gross weight is carried by the main landing gears and 5 percent is carried
by the nose gear. The FAA Advisory Circular AC 150/5300-13, Airport
Design, lists the weight of many civil aircraft. The FAA recommends using
the maximum anticipated takeoff weight, which provides some degree of
conservatism in the design. This will allow for changes in operational use
and forecast traffic, which is approximate at best. The conservatism will be
offset somewhat by ignoring arriving traffic” (FAA 2004: 24).
132 Design fundamentals
Axle equivalency (ESAL) concept
The various editions of the AASHTO Design Guide for rigid and flexible
pavements, culminating in the 1993 Guide (AASHTO 1993) and 1998
Supplement (AASHTO 1998), have relied on the axle equivalency concept
to design pavements for mixed traffic. Axle equivalency factors have been
developed for various magnitudes of single, tandem, or tridem/triple axles by
determining the relative damaging power of each axle, in loss of pavement
serviceability, to that of an equivalent 80 kN (18 kip) single axle.
These equivalency factors are then multiplied by the number of axles in
each category to determine a number of 80 kN (18 kip) equivalent single
axle loads, or ESALs. The pavement is then designed to carry a specific
number of ESALs.
Equivalency factors are roughly proportional to the fourth power of the
axle load magnitude (Yoder and Witczak 1975: 154). Therefore, doubling
the load on an axle type causes 16 times as much pavement damage, as a
rule of thumb. This relationship is not exact, and varies by pavement type,
but is useful as an estimate.
There are two significant problems with using ESALs for pavement
design. The first is that AASHTO has developed different equivalency fac-
tor tables for flexible and rigid pavements, and the numbers are different
for different pavement thicknesses. This makes it difficult to compare nom-
inally equivalent designs for asphalt and concrete pavements, because even
if they are designed for the same traffic they will not be designed for the
same number of ESALs.
The second is that some lighter axles do essentially no damage to the
pavement, and thus should have an equivalency factor of zero. Using the
PCA fatigue equations, loads that produce a SR ≤0 45 do no damage and
therefore unlimited repetitions are allowed. However, the AASHTO ESAL
tables assign equivalency factors to those loads.
Curling and warping stresses
Stresses in rigid pavements are due to environmental effects and traffic loads.
Stresses due to traffic loads determine the fatigue life of the pavement, while
environmental effects due to curling and warping determine the maximum
joint spacing for the pavement. As noted in Chapter 2, stresses are resisted by
the flexural strength of the concrete, and not by any included reinforcing steel.
Reinforcing steel for JRCP and CRCP is simply used to hold cracks together.
Stresses due to curling and warping depend on the ratio between the
length of the slab L and the radius of relative stiffness . The radius of
relative stiffness is provided by equation 7.1:
12 1− 2 k
Design fundamentals 133
where E = the modulus of the elasticity of the concrete, D is the pavement
thickness, k is the modulus of subgrade reaction, and is the Poisson’s ratio
of concrete, typically taken as 0.15.
Because is in units of length, the ratio L/ is dimensionless. Huang
(2004: 151–152) provides an example of calculating the radius of relative
stiffness for a slab 200 mm (8 in) thick, with E = 27 6 GPa (4,000,000 psi)
and k = 54 2 MPa/m (200 psi/in). From equation 7.1, = 776 mm (30.6 in).
The slab edge-stress due to temperature curling is provided by:
CE t t
2 1− 2
where t = concrete thermal coefficient of expansion, discussed in
Chapter 5, and t = temperature difference between the top and bottom
of the slab. C is a correction factor for a finite slab, determined using L/ ,
with a chart developed by Bradbury (1938) (Figure 7.1).
Note that a stiffer base or subbase material (higher k) leads to a smaller ,
and thus higher L/ ratios for the same joint spacing, higher C coefficients,
and higher curling stresses. Also, with a stiffer k, the required pavement
thickness D will often decrease, which will reduce further still. Use of
improved, stiffer base and subbase layers and thinner pavements, without
correspondingly reducing joint spacing, will lead to a greater incidence of
mid-slab cracking due to curling and warping.
Curling stresses may be calculated for a slab 7.6 m (25 ft) long and
3.66 m (12 ft) wide using the example from Huang (2004: 151–152) above.
0 1 2 3 4 5 6 7 8 9 10 11 12 13 14
Slab length/radius of relative stiffness L/
Figure 7.1 Curling stress correction factors for a finite slab (after Bradbury 1938).
134 Design fundamentals
Lx/ = 9 81 and Ly/ = 4 71, so Cx = 1 07 and Cy = 0 63. If the temperature
differential between the top and bottom of the slab is 11 1 C 20 F and
the thermal coefficient of the concrete t = 9×10−6
/ C 5×10−6
/ F , then
the edge-stress due to curling is 1.48 MPa (214 psi) in the longitudinal
direction. If the slab length is reduced to 4.6 m (15 ft), then Lx/ = 5 89
and Cx = 0 93. The shorter slab length reduces the edge-stress to 1.28 MPa
Because thermal strain t = t t, equation may be modified for differen-
tial shrinkage sh between the top and bottom of the slab:
2 1− 2
Curling occurs in a daily cycle, with heating during the day causing curling
downward (positive temperature gradient) and cooling at night causing
curling upward (negative temperature gradient). The bottom of the slab,
against the earth, remains at a more constant temperature. Tensile stresses
are induced in the top of the slab during the day and in the bottom of the
slab at night.
In contrast, warping occurs one time as the pavement is curing and
drying. Generally it is easier for moisture to escape from the top of the slab
than from the bottom, particularly if curing practices are not adequate or
the subbase drains poorly. There will, therefore, be differential shrinkage
between the top and bottom of the slab. This builds a permanent upward
warp in the slab.
LTPP data has been used to investigate locked-in curvatures for more
than 1,100 JPCP 152 m (500 ft) test site profiles from 117 different sites.
The worst sections were found to have differential elevations between
the mid-slab and the joints of as much as 10 mm (0.4 in). The most
extreme curvatures occurred in pavements over low plasticity sandy-gravely
clay or clayey sand-gravel. Slabs with severe upward curvature are at risk
for excessive joint deflections, premature faulting and spalling, pumping,
and mid-slab cracking. Curvatures were much higher for pavements with
undoweled joints (Byrum 2000, 2001).
Clearly, differential elevations of this magnitude can affect pavement ride
quality. Pavement construction practices, particularly curing, are likely to
have an important effect on the magnitude of locked-in curvature, with
well-cured doweled pavements likely to have the least curvature.
Traffic loading stresses
The stresses caused by traffic loading on a concrete pavement slab depend
on the location of the load, among other factors. If the load is carried in
the interior of the slab, away from any corners, the stress level is generally
Design fundamentals 135
Corner loading –
Edge loading –
Interior loading –
Figure 7.2 Corner, edge, and interior loading.
low. Therefore, analytical solutions have been developed for loads applied
at corners, edges, and at the interior of concrete pavement slabs, as shown
in Figure 7.2.
Stresses from corner loading
Corner stresses are associated with corner breaks, while edge and interior
stresses are associated with mid-slab transverse cracking. Stresses depend
on the load applied and load configuration, slab thickness, modulus of
subgrade reaction k, and radius of relative stiffness .
The oldest and simplest corner stress equation can be developed directly
from equilibrium. This formula was developed by Goldbeck (1919) and
Older (1924) and is discussed by Huang (2004: 154–155). It is based on
some very conservative assumptions – the load is placed at the corner of
the slab, and there is no subgrade support k = 0 . It approximates the
situation that may occur with pumping under pavement corners, or curling
and warping that lifts the corner from the subgrade.
The formula is developed from the standard bending stress equation =
Mc/I. The failure plane is assumed to occur a distance x from the corner,
and forms a crack of length 2x. Therefore, if D is the slab thickness, c = D/2
and I = bh3
/12 = 2x D3
/12. The bending moment for the cantilever is Px.
Thus, the corner stress becomes:
136 Design fundamentals
This formula is conservative, because the load is distributed over the contact
area of the tire and thus the moment must be less. Furthermore, it is unlikely
that there would be no subgrade support under the corner at all. It is,
however, useful to note that stress decreases with the square of the pavement
This equation was updated by Westergaard (1926) and subsequently by
Ioannides et al. (1985), and is discussed by Huang (2004: 154–155).
c 0 72
1 772a 0 72
Where c = the side length of a square contact area and a = radius of a circle
with the same contact area. Westergaard and Ioannides et al. use h for slab
thickness instead of D, but D is used in equation 7.5 for consistency with
the rest of this book.
Because of the term in brackets, the corner stress calculated using equa-
tion 7.5 will always be lower than that calculated using equation 7.4. In
pavement stress calculations, the load may be considered to be evenly dis-
tributed as a uniform tire pressure p over a circle of radius a, so:
P = p a2
or a =
For a slab 200 mm (8 in) thick, and a single axle load equal to half an
ESAL or 40 kN (9,000 lb), equation 7.4 gives a corner bending stress of
3 MPa (435 psi). If the concrete has E = 27 6 GPa (4,000,000 psi) and
the subgrade k = 54 2 MPa/m (200 psi/in), then = 776 mm (30.6 in) as
calculated previously in this chapter. If the tire pressure is 620 kPa (90 psi),
then the radius a is 143 mm (5.6 in). The corner stress then is multiplied by
0.556, which is the term in brackets in equation 7.5, so the stress becomes
1.67 MPa (242 psi).
Stresses from edge-loading
For mid-slab cracking, the edge-loading stress is critical because it is much
higher than the stress due to interior loading. Westergaard developed several
stress equations. The final equation for a circular loading patch is provided
by Ioannides et al. (1985) and is discussed by Huang (2004: 157–158):
−0 034 (7.7)
This assumes a Poisson’s ratio of concrete = 0 15. Continuing with the
previous example slab and loading case [D = 200 mm (8 in), P = 40 kN
Design fundamentals 137
(9,000 lb), E = 27 6 GPa (4,000,000 psi), the subgrade k = 54 2 MPa/m
(200 psi/in), = 776 mm (30.6 in), and a is 143 mm (5.6 in)] we calculate
an edge-loading stress e = 2 36 MPa (343 psi). This stress is 42 percent
higher than the corner loading stress calculated above using equation 7.5.
This suggests that, as a general rule, edge-loading stress is higher than
corner loading stress, and thus mid-slab cracking is more likely than corner
breaks unless the pavement corners are heavily loaded or unsupported.
Also, dowels near corners help prevent corner breaks.
Stresses from interior loading
The Westergaard (1926) interior loading stress equation may be written as:
+1 069 (7.8)
Where b = a if a ≥ 1 724D, and otherwise
b = 1 6a2 +D2 −0 675D (7.9)
This equation is discussed by Huang (2004: 156–157). As with equation 7.7,
this assumes a Poisson’s ratio of concrete = 0 15. For the slab and loading
parameters discussed in the examples above, equation 7.9 applies because a
is 143 mm (5.6 in) and is not ≥ 1 724D, or 345 mm (9.65 in). Therefore, b =
134 mm (5.29 in) and the interior-loading stress i = 1 26 MPa (183 psi).
This is much lower than the edge-loading stress, and so the edge-loading
stress is used to analyze the risk of mid-slab cracking.
Combining stresses from curling, warping, and traffic
Obviously stresses due to curling, warping, and loading are present simul-
taneously and affect the performance of the pavement. Since the service life
of the slab is predicated on fatigue, the number of cycles or reversals of
each type of stress is important.
Over the life of a pavement, the stress cycles due to curling and warping
are much fewer than those due to loading. Temperature effects occur once
per day, with the top of the slab heating and cooling while the bottom
of the slab remains at a more constant temperature. Even over 20 years,
therefore, there are only about 7,300 fatigue cycles due to temperature.
Moisture warping occurs only once, as the pavement cures and dries out,
unless there are significant seasonal moisture changes that are not uniform
through the slab, which would not be a common occurrence.
138 Design fundamentals
In contrast, traffic loads produce fatigue stresses in pavements for any-
where from tens or hundreds of thousands of repetitions, for airports, up
to tens or hundreds of millions of repetitions for busy highways. Therefore,
in fatigue analysis, curling and warping stresses are generally ignored.
In Yoder and Witczak’s classic textbook, they state “It is important to
note that warping stresses are not considered when determining thickness of
pavement. The philosophy that governs the design, simply stated, is ‘Joints
and steel are used to relieve and/or take care of warping stresses, and the
design, then, is based upon load alone when considering thickness.’ This
principle is so important that it must be clearly understood by the designer.
Recall that a joint is nothing more than a ‘designed crack’ ” (Yoder and
Witczak 1975: 125). In this passage, “warping” encompasses both curling
and warping as they are defined today.
At the time the paragraph above was written, lightly reinforced slabs with
only temperature steel (JRCP) were often used. Today, the philosophy for
JPCP is to ensure that the joint spacing is short enough to reduce curling
stresses. Therefore, with proper joint spacing, there is no explicit need to
consider curling and warping stresses in design. With CRCP, the closely
spaced cracks divide the pavement into miniature slabs short enough that
curling is not an issue.
Westergaard (1926) and Ioannides et al. (1985) also developed equations
for slab deflections due to corner, edge, and interior loading ( c e, and
i, respectively). These equations are discussed by Huang (2004: 155–158).
1 205−0 69
1 205−0 69
Deflections, particularly at slab corners, are important from the standpoint
of pumping. Slabs that deflect more apply more pressure and energy to
the subgrade, with a higher probability of ejecting pumpable water and
materials. This is the basis of the PCA 1984 erosion design.
On the other hand, it is not an efficient design practice to attempt to
solve pumping problems by increasing slab thickness. It is better to provide
dowels at joints and to provide a subbase. Doweled joints support slab
edges and corners, transferring loads to adjacent slabs through dowel shear
action. This is a more certain and probably more economical approach to
Design fundamentals 139
General stress and deflection calculation from finite
The analytical solutions developed by Westergaard and refined by Ioannides
and his colleagues represent idealized situations that rarely occur in practice.
The corner and edge solutions are very conservative. Even with the obsolete
practice of using narrow lanes only 2.7–3 m (9–10 ft) wide, it would not
be realistic to expect traffic to drive right along the edge of the pavement,
nor would it be safe.
Typically modern highways are designed with 3.7 m (12 ft) traffic lanes.
Therefore, for highway pavements neither edge-loading nor interior loading
really applies, and the actual stress condition is in between. It is always
conservative to design on the basis of edge-loading stress. Some highway
pavements use widened slabs for the outside lane that carries the most truck
traffic – typically widened lanes are 4.3 m (14 ft) wide. The definition of
a widened slab is “concrete pavement slab that is paved wider (usually at
least 18 in. [450 mm] wider) than a conventional 12 ft (3.7 m) traffic lane
to increase the distance between truck tires and slab edge, thereby reducing
edge stresses due to loading. Concrete shoulders that are tied to the travel
lane with bars also reduce edge loading stresses” (ACI Committee 325 2006:
3). Doweled transverse and longitudinal joints also reduce edge-stresses.
Due to the difficulty of computing stresses for various pavement and
loading geometries, finite element stress analysis programs have been devel-
oped. Early versions were used to develop the design tables and charts for
the PCA 1984 procedure. Other subsequent finite element programs include
JSLAB, ILLI-SLAB, KENSLABS, and EVERFE.
The program KENSLABS, which is provided with Huang’s pavement
design textbook, has many features in common with the other programs.
Key features are summarized in Chapter 5 of the textbook (Huang 2004)
and are listed below:
• Each pavement slab is divided into rectangular plate elements. The
number of elements per slab is determined from the grid geometry
input by the program user. A larger number of elements improves the
accuracy of the solution but requires more computation time, which is
generally not a problem with modern computers.
• The slab may have one or two layers. If there are two layers, they
may be bonded or unbonded. This may be used to model bonded
and unbonded overlays, or concrete pavement bonded to a base of a
different material such as asphalt or CTB. Each of the two layers may
be assigned its own modulus of elasticity and Poisson’s ratio.
• Three different foundation models may be used. The simplest is the liq-
uid, or spring foundation using k-values. A more realistic, and complex,
model is the solid foundation. The subgrade and subbase are modeled
as a single elastic halfspace, or Boussinesq model. The most complex
140 Design fundamentals
foundation is the layer model, also called a Burmister foundation. With
this foundation, the modulus of elasticity and Poisson’s ratio of each
layer (subgrade, subbase, base if any) are used directly. This behaves
as a multilayer flexible pavement under the slab. For most problems,
the liquid k-value foundation is sufficiently accurate. Gaps between the
slab and the foundation, representing pumping or subsidence, may also
• Dowel bars are modeled as transfer of shear and bending forces between
slabs. A shear spring constant may be specified, or the diameter and
spacing of the dowels as well as their material properties may be pro-
vided. It is also possible to model loose dowels, by specifying a gap
between the dowel and the concrete.
• Aggregate interlock joints are modeled as shear transfer across the joint
• Multiple slabs may be modeled – thus, load transfer across doweled or
aggregate interlock transverse joints or across tied longitudinal joints
may be included in the problem. A maximum of six slabs may be
• Traffic loads are represented as rectangular patches with uniform tire
pressure over each patch. Different pressures may be used for different
patches, and point loads may be applied at nodes.
• Temperature curling may be included in the problem. This feature may
also be used indirectly to model moisture warping.
• The output of the program includes stresses, strains, and deflections.
These may be reported at all nodes, or only at the nodes with the
highest values. Dowel bearing stresses may also be calculated.
Finite element programs appear to have satisfactory accuracy, and have
been shown to agree with analytical solutions. There are also limitations
to these tools, and the limitations of KENSLABS are described by Huang
Another rigid pavement finite element program is EVERFE. This is avail-
able at no cost on the web at http://www.civil.umaine.edu/EverFE/.
Thicker pavements can carry more loads, because flexural stresses are
reduced and the fatigue life of the pavement is increased. There are two basic
approaches to determining the proper thickness for a concrete pavement.
These are empirical and mechanistic designs. Empirical design is based on
the observed performance of pavements in the field, under normal or accel-
erated traffic loading. Mechanistic design relies on calculation of stresses
and strains. In reality, all design procedures combine both approaches to
Design fundamentals 141
The AASHTO design procedure up through the 1993 guide (AASHTO
1993) is empirically based. The design equations are based on regression
of the results of a two-year road test carried out in Ottawa, Illinois, in
the late 1950s, by AASHO (before the T for transportation was added).
The AASHO Road Test is discussed in Chapter 1. Loops with different
pavement designs were loaded by trucks with different axle weights and
configurations, and the distresses and serviceability of the pavements were
measured over time. Because approximately 20 years of traffic were applied
in 2 years, this represents an accelerated test. The basic equations were
modified in succeeding editions of the AASHTO Design Guide, often adding
adjustment factors based on mechanistic principles (Huang 2004: 568–570).
The problem with relying on empirical designs becomes evident when it is
necessary to extend them to new conditions – either new environments, new
pavement designs, or new vehicle types. The AASHTO design procedure
has, of course, been used for environments other than Ottawa, Illinois, and
triple axles and CRCP have been added to the design procedure, although
they were not part of the original road test. Furthermore, the pavements at
the AASHO Road Test were much more vulnerable to pumping than pave-
ments built with more recent details and construction techniques. Details of
the AASHTO 1993 and 1998 supplement design procedures are provided
in Chapter 8.
The PCA 1984 procedure (PCA 1984) is mechanistic. Two failure mecha-
nisms are identified, fatigue cracking and erosion (pumping), and the pave-
ment thickness is determined so that neither failure mode occurs before the
end of the required pavement life. This approach forms the basis for the
PCA and ACPA methods for airport and industrial pavement design also.
FAA airport pavement design procedures are also mechanistic.
The latest proposed AASHTO M-EPDG procedure combines both
approaches, as the name indicates. Results from finite element modeling are
used to determine stresses.
It should be noted that thicker pavements cannot compensate for defective
details, poor materials, or poor construction practices. Adequate thickness
is a necessary but not a sufficient condition for long pavement life.
Transverse joint design and spacing
Distortion of pavement slabs due to curling and warping has been discussed
previously. With greater joint spacing and longer slabs, the slab corners lift
and flexural stresses at the midpoint of the slab increase.
The joint design problem breaks down into several elements:
• Selection of an appropriate joint spacing. Some agencies have used
variable spacing to reduce the likelihood of rhythmic excitation of
142 Design fundamentals
• Determination of whether aggregate interlock joints or doweled joints
will be used.
• If doweled joints are used, what diameter of dowels to use.
• Determination whether the joint is transverse to the centerline of the
pavement or skewed.
In the past, keyed joints have been used. These are described in Chapter 2.
Problems occur when either the key or the top and bottom of the slab
above the slot break off. Yoder and Witczak (1975: 582) reported that they
should not be used for slabs less than 225 mm (9 in) thick, or for airfields
with heavy traffic. In current practice, keyed joints are avoided and tied or
doweled joints are used instead.
With JPCP, the joint spacing should be short enough to prevent high curling
stress buildup. This was discussed earlier in the section on calculation of
curling and warping stresses. Smith et al. (1990) found that joint faulting
and transverse cracking increase with longer joint spacing. Cracking, in
particular, increases when joint spacing exceeds 5.5 m (18 ft) for pavements
with random joint spacing. This trend would be expected to hold true
for pavements with uniform joint spacing. “Nussbaum and Lokken (1978)
recommended maximum joint spacings of 20 ft. (6.1 m) for doweled joints
and 15 ft. (4.6 m) for undoweled joints” (Huang 2004: 15).
The AASHTO 1993 Pavement Design Guide states
In general, the spacing of both transverse and longitudinal contraction
joints depends on local conditions of materials and environment the
spacing to prevent intermediate cracking decreases as the thermal coef-
ficient, temperature change, or subbase frictional resistance increases;
and the spacing increases as the concrete tensile strength increases. The
spacing also is related to the slab thickness and the joint sealant capa-
bilities As a rough guide, the joint spacing (in feet) for plain concrete
pavements should not greatly exceed twice the slab thickness in inches.
For example, the maximum spacing for an 8-inch [200 mm] slab is 16
feet [4.8 m].
(AASHTO 1993: II-49)
This relationship may be expressed as:
S = 0 024 D (7.13)
where S = joint spacing in m and D = slab thickness in mm, or
S = 2D (7.14)
Design fundamentals 143
where S = joint spacing in feet and D = slab thickness in inches.
ACI Committee 325 (2002: 14) provides a chart of maximum joint spac-
ing as a function of pavement thickness and k-value. This is based on a
maximum L/ ratio of 4.44. For example, a 280 mm (11 in) slab with
a k-value of 12 MPa/m (44 psi/in) should have a maximum joint spacing
of 6.2 m (20 ft). In contrast, a 130 mm (5.1 in) slab on stiff support of
110 MPa/m (400 psi/in) should have a joint spacing of no more than 2 m
(6.6 ft). This maximum joint recommendation is clearly conservative. Smith
et al. (2002: 4–9) notes that the maximum recommended L/ for unbonded
overlays is 4.5–5.5 (ACI 325.13R 2006, ERES 1999). As Figure 7.1 shows,
the stress coefficient C is 0.64 for L/ = 4 5 and 0.85 for L/ = 5 5.
For highways, the joint spacing
varies throughout the country because of considerations of initial costs,
type of slab (reinforced or plain), type of load transfer, and local con-
ditions. Design considerations should include: the effect of longitudinal
slab movement on sealant and load transfer performance; the maximum
slab length which will not develop transverse cracks in a plain concrete
pavement; the amount of cracking which can be tolerated in a jointed
reinforced concrete pavement; and the use of random joint spacings.
For plain concrete slabs, a maximum joint spacing of [4.6 m] 15 feet
is recommended. Longer slabs frequently develop transverse cracks. It
is recognized that in certain areas, joint spacings greater than [4.6 m]
15 feet have performed satisfactorily. The importance of taking local
experience into account when selecting joint spacing (and designing
pavements in general) cannot be overstated. Studies have shown that
pavement thickness, base stiffness, and climate also affect the maxi-
mum anticipated joint spacing beyond which transverse cracking can be
expected. Research indicates that there is an increase in transverse
cracking when the ratio L/ exceeds 5.0.
As Figure 7.1 shows, the stress coefficient C is 0.75 for L/ = 5 0. Figure 7.3
shows maximum slab length as a function of pavement thickness D and
modulus of subgrade reaction k if L/ ≤5 0. A concrete modulus of elasticity
of 27.6 GPa (4 million psi) is assumed.
As an example, a 500 mm (20 in) thick pavement with slab support of
54 MPa/m (200 psi/in) could have a joint spacing up to 7.6 m (25 ft). If the
k is increased to 135 MPa/m (500 psi/in), then the joint spacing should be
reduced to 6.1 m (20 ft).
144 Design fundamentals
Often thicker airfield pavements [greater than 300 mm (12 in)] are built
with 7.6 by 7.6 m (25 by 25 ft) squares. Another option is to pave using
11.4 m (37.5 ft) paving passes and sawcut a longitudinal joint, which
reduces the number of paving passes required by a third and produces 5.7
by 6.1 m (18.75 by 20 ft) panels.
For airports, the trend has been to use stiffer base materials such as
Econocrete or bituminous base course. With stiffer base materials, there is
a greater risk of mid-slab cracking unless the joint spacing is also reduced.
Therefore, the 7.6 m by 7.6 m (25 by 25 ft) joint spacing may be excessive
with stabilized bases.
The FAA Airport Pavement Design, Advisory Circular (AC) 150/5320-
6D provides a chart for maximum joint spacing for unstabilized bases,
4 6 8 10 12 14 16 18 20
Slab thickness, in
k = 50 psi/in
k = 300 psi/in
k = 100 psi/in
k = 400 psi/in
k = 200 psi/in
k = 500 psi/in
Figure 7.3 Maximum joint spacing based on slab thickness D and modulus of subgrade
reaction k for L/ ≤5 0 in (a) U.S. customary units and (b) metric units.
Design fundamentals 145
100 200 300 400 500
Slab thickness, mm
k = 13.5 Mpa/m
k = 81 Mpa/m
k = 27 Mpa/m
k = 108 Mpa/m
k = 54 Mpa/m
k = 135 Mpa/m
Figure 7.3 (Continued)
which is provided in Chapter 10 as Table 10.3. For stabilized bases, the joint
spacing is limited to five times the radius of relative stiffness, equation 7.1
(FAA 2004: 87). Furthermore, although the FAA places a maximum value
of 135 MPa/m (500 psi/in) on the subgrade modulus for pavement thickness
design, the actual value should be used for calculating the radius of relative
stiffness. Hall et al. (2005: 15) suggest a maximum joint spacing of 6.1 m
(20 ft) for pavements more than 305 mm (12 in) thick. Shorter spacing
should be used for thinner pavements.
If maximum joint spacing is exceeded, the pavement slabs will often crack
between the joints. “On a runway in Texas 200-mm (8-in) thick concrete
pavement was placed in 4.6 by 5.7m (15 by 18.75 ft) slabs. Slabs of this
thickness are limited to a maximum joint spacing of 4.6 m (15 ft) by Air
146 Design fundamentals
Force practice. Almost every slab in this project quickly cracked to bisect
the 5.7 m (18.75 ft) length” (Rollings 2005: 168).
For crowned pavements, a joint should always be provided at the crown.
“Slabs that are crowned in the middle without a joint tend to crack down
the crowned axis of the slab. During the 1990s three Air Force runways and
taxi lanes were designed with unjointed crowned slabs by a government
design agency. In every case, the slabs cracked. One of the examples is
a concrete runway that developed a continuous 3,048-m (10,000-ft) long
centerline crack much to the disgust of the Air Force owner” (Rollings
2005: 168–169). It could be argued that a concrete slab “knows” what its
proper joint spacing should be, and if the designer doesn’t provide for the
joint the slab will crack.
Traditionally, with JRCP, longer joint spacings were used and it was
assumed that the slabs would crack and that the temperature steel would
hold the cracks together. In practice, these pavements have often performed
poorly, particularly at the longer joint spacings.
Variable joint spacing
Evenly spaced joints, if faulted, can induce harmonic motion in vehicle
suspensions at certain speeds. For this reason, some agencies have used
variable joint spacing. The ACPA (2006) notes that this type of motion
was primarily a problem with large cars on California freeways with 4.6 m
(15 ft) spacing of undoweled joints. In California in the 1960s and 1970s,
variable joint spacing of 4, 5.8, 5.5, and 3.7 m (13, 19, 18, and 12 ft)
became the standard. Because the 5.8 and 5.5 m (19 and 18 ft) panels
were found to be too long and prone to mid-slab cracking, the spacing was
changed to 3.7, 4.6, 4, and 4.3 m (12, 15, 13, and 14 ft). The AASHTO
Design Guide also discusses randomized or irregular spacing patterns and
suggests avoiding multiples of 2.3 m (7.5 ft) (AASHTO 1993: II-49).
Random joint spacings have been successfully used in plain undoweled
pavements to minimize resonant vehicle responses. When using ran-
dom joint spacings, the longest slab should be no greater than [4.6 m]
15 feet, to reduce the potential for transverse cracking. Some States
are successfully using a spacing of [3.7-4.6-4.0-4.3 m] 12 -15 -13 -14 .
Large differences in slab lengths should be avoided.
Pavement construction standards have improved, and there are few 1959
Buicks still on the road. If pavements are built smoothly with doweled joints
to prevent faulting, then there is probably little benefit to the use of variable
Design fundamentals 147
Aggregate interlock joints
Loads applied by traffic must be effectively transferred from one slab to
the next in order to minimize vertical deflections at the joint. Reduced
deflections decrease the potential for pumping of the base/subbase mate-
rial and faulting. The two principal methods used to develop load trans-
fer across a joint are: aggregate interlock; and load transfer devices,
such as dowel bars Aggregate interlock is achieved through shearing
friction at the irregular faces of the crack that forms beneath the saw
cut. Climate, and aggregate hardness have an impact on load transfer
efficiency. It can be improved by using aggregate that is large, angu-
lar, and durable. Stabilized bases have also been shown to improve
load transfer efficiency. However, the efficiency of aggregate interlock
decreases rapidly with increased crack width and the frequent appli-
cation of heavy loads to the point that pavement performance may be
affected. Therefore, it is recommended that aggregate interlock for load
transfer be considered only on local roads and streets which carry a
low volume of heavy trucks.
Early concrete pavements were all built with aggregate interlock joints.
As pumping and faulting of joints began to cause problems on heavily
trafficked pavements, dowels were introduced.
Nevertheless, there remains a role for aggregate interlock joints in con-
crete pavements. Aggregate interlock joints work well with low-speed traf-
fic, relatively light loads, and shorter joint spacing. This corresponds to
thinner pavements – ACI Committee 325 (2002: 15) suggests that dowels
are not necessary for pavements less than 200 mm (8 in) thick. This is
supported by ACPA (1998: 26–27) for plain concrete pavements, although
it is suggested that thinner reinforced pavements with longer joint spacing
require dowels. There is also an issue of constructability – it is more difficult
to place dowels accurately in thinner pavements.
Aggregate interlock joints transfer load through shear of the irregular
interlocking faces of adjacent slabs. Generally, joints are sawn 1/4−1/3 of
the way through the slab, and then the slab is allowed to crack naturally.
The load transfer is aided by the stiffness of supporting layers, such as a
stabilized subgrade or subbase.
Efficiency of aggregate interlock joints depends on the following factors:
• The width of the joint or crack opening. This is directly related to slab
length. ACI Committee 325 (2002: 14) suggests that 5.5 m (18 ft) is a
practical maximum for undoweled joints.
• The opening width also depends on drying shrinkage and the thermal
coefficient of the concrete. Lower shrinkage and thermal coefficients
148 Design fundamentals
• Maximum size of the coarse aggregate, because when the crack forms
and goes around the particles it will be rougher. Larger coarse aggregate
also means less paste and less shrinkage.
• Hardness of the coarse aggregate, because harder stones will not break
down under traffic.
One advantage of aggregate interlock joints in regions where deicing salts
are used to remove snow and ice is that a pavement with no reinforcement
or dowels is not susceptible to corrosion of embedded steel. This makes the
pavement both cheaper to build and more durable.
Dowels are used in transverse joints to prevent pumping and faulting. Dow-
els differ from tie bars in that they are lubricated to allow the joints to
open and close without longitudinal stress buildup, while preventing dif-
ferential vertical movement across the joint. Dowel bars are generally used
for all pavements 200 mm (8 in) or more in thickness (ACI Committee 325
2002: 15). When dowels are used, they are typically 460 mm (18 in) long
and spaced 300 mm (12 in) on center across the slab, for 11 dowels in a
typical 3.66 m (12 ft) highway pavement lane. In contrast, when dowels
are installed in an existing pavement with dowel bar retrofit, as discussed
in Chapter 17, generally only three are put in each wheel path for a total
of six across the lane.
The FHWA recommends the use of dowel bars on all highway pavements.
Dowel bars should be used on all routes carrying more than a low vol-
ume of heavy trucks. The purpose of dowels is to transfer loads across
a joint without restricting joint movement due to thermal contraction
and expansion of the concrete. Studies have shown that larger dowels
are more effective in transferring loads and in reducing faulting.
Dowel bar diameter
Proper minimum dowel size is based on having sufficient diameter to resist
shear and bending forces transmitted from one slab to another, and to
reduce the bearing stress of the steel dowel against the concrete to an
acceptable value. Generally, the concrete bearing stress is the critical design
parameter. If it is too high, the dowel will wear away the concrete and
In theory, the allowable dowel-bearing stress should be a function of
the concrete compressive strength, and it would be possible to use smaller
Design fundamentals 149
diameter dowels with higher strength concrete. In practice, recommen-
dations have traditionally been based on the thickness of the pavement,
because thicker pavements are assumed to carry larger numbers and heav-
ier vehicle loads. In the past 19 and 25 mm (3/4 and 1 in) dowels were
recommended for thinner pavements, but in current practice the mini-
mum recommended dowel diameter is 32 mm (1.25 in) for 200 mm (8 in)
For highway pavements
It is recommended that the minimum dowel diameter be D/8, where D
is the thickness of the pavement. However, the dowel diameter should
not be less than [32 mm] 1 1/4 inches. It is also recommended that
[450 mm] 18-inch long dowels be used at [300 mm] 12-inch spacings.
Dowels should be placed mid-depth in the slab. Dowels should be
corrosion-resistant to prevent dowel seizure, which causes the joint to
lock up. Epoxy-coated and stainless steel dowels have been shown to
adequately prevent corrosion.
Table 7.1 shows recommended dowel diameters, lengths, and spacings for
different pavement thicknesses, from 200 mm (8 in) pavements to 50 mm
(2 in) dowels for 400 mm (16 in) thick pavements.
Smith and Hall (2001) recommend a different approach to dowel bar
diameter selection for highways based on the traffic level. If the pavement
is designed to carry less than 30 million ESALs, 30 mm (1.25 in) dowel bars
are recommended. Dowels 38 mm (1.5 in) in diameter should be used for
pavements carrying between 30 and 90 million ESALs. For traffic over 90
million ESALs, the bar diameter should be 41 mm (1.625 in). Since thicker
pavements are needed to carry heavier traffic, the two recommendations
produce similar dowel diameters.
Table 7.1 Dowel bar diameter recommendations (ACPA 1998: 27, ACI Commit-
tee 2002 325: 15)
Slab thickness, mm
Dowel length, mm (in) Dowel spacing, mm
<200 <8 Dowels not required
200 (8) 32 (1.25) 450 (18) 300 (12)
250 (10) 32 (1.25) 450 (18) 300 (12)
280 (11) 38 (1.5) 450 (18) 300 (12)
300 (12) 38 (1.5) 450 (18) 300 (12)
350 (14) 44 (1.75) 500 (20) 300 (12)
400 (16) and up 50 (2) 600 (24) 450 (18)
150 Design fundamentals
Skewed joints represent another approach to addressing the problem of
joint faulting. The idea is that by skewing joints, only one wheel crosses
the joint at a time, making faulting less objectionable (Yoder and Witczak
Skewed joints and variable spacing may be combined.
Skewed joints with randomized spacings, say 13-19-18-12 ft. (4.0-
5.8-5.5-3.7 m), have also been used. The obtuse angle at the outside
pavement edge should be ahead of the joint in the direction of traffic,
since that corner receives the greatest impact from the sudden impact
of wheel loads. The advantage of skewed joints is that the right and
left wheels do not arrive at the joint simultaneously, thus minimizing
the annoyance of faulted joints. The use of randomized spacings can
further reduce the resonance and improve the riding comfort.
(Huang 2004: 179)
The AASHTO Design Guide also discusses skewed joints and notes that
they may reduce deflections and stresses at joints, and provide a smoother
ride for vehicles (AASHTO 1993: II-49).
While they do not affect joint spacing, skewed joints have been used
in plain pavements to provide a smoother ride. A skew of [0.6 m] 2
feet in [3.7 m] 12 feet is recommended, with the skew placed so that
the inside wheel crosses the joint ahead of the outside wheel. Only one
wheel crosses the joint at a time, which minimizes vehicle response and
decreases stresses within the slab. Skewed joints are most commonly
used when load transfer devices are not present. While skewed joints
may be used in conjunction with load transfer devices, studies have not
substantiated that skewing doweled joints improves pavement perfor-
mance and are not recommended. Dowels in skewed joints must be
placed parallel to the roadway and not perpendicular to the joints.
On new JPCP, skewed joints can be effective in reducing faulting on
nondoweled pavements, but have no effect when used on properly dow-
eled pavements (Yu et al. 1998; Khazanovich et al. 1998). Furthermore,
JPCP designs with skewed joints constructed on a stiff base (treated
cement or lean concrete) are prone to corner breaks.
(ACI Committee 325 2006: 4)
It is notable that skewed joints do not prevent joint faulting, but only
mitigate its effects. It is more reliable to use conventional perpendicular
transverse joints with dowels.
Design fundamentals 151
Longitudinal joints and tie bar design
As noted in Chapter 2, longitudinal joints are often used between highway
traffic lanes. Tie bars may be placed across longitudinal joints between
traffic lanes and between traffic lanes and a concrete shoulder. They differ
from dowel bars in that they do not have to allow movement. Also, traffic
does not cross these joints except when changing lanes, so load transfer is
not a major concern. One common tie bar design is 13 mm (#4) conventional
reinforcing bars 910 mm (36 in) long, spaced at 760–1020 mm (30 to 40 in)
intervals. Tie bar length is governed by bond stress (Huang 2004: 171).
Most steel available today for tie bars would be classified as Grade
60, with 413 MPa (60,000 psi) yield stress. “When using Grade 60 steel,
[16 mm] 5/8-inch by [1 m] 40-inch or [13 mm] 1/2-inch by [0.8 m] 32-inch
tiebars should be used. These lengths are necessary to develop the allowable
working strength of the tie bar. Tie bar spacing will vary with the thickness
of the pavement and the distance from the joint to the nearest free edge”
Huang (2004: 170) provides an equation for calculating the required area
of steel per unit length As of the pavement slab:
As = cDL fa
= 0 13DL mm2
/m = 469×10−6
Where c = unit weight of concrete (23 6×10−6
, or 0 0868 lb/in
D = slab thickness (mm, in), L = distance from the longitudinal joint to a
free edge (m, ft), fa = average coefficient of friction between the slab and
subgrade, usually taken as 1.5, and fs = the allowable stress in the steel
(2/3 of the yield stress, conservatively 276 MPa or 40,000 psi with modern
steel). To calculate the bar spacing, divide the cross-sectional area of a single
bar by the required area of steel per unit length of the slab.
As an example, determine the spacing for 13 mm (#4) bars for a 250-
mm thick pavement with two lanes of total 7.32 m (24 ft) to the outside
edge. The required As = 238 mm2
/m 0 113 in2
/ft . Each bar has a cross-
sectional area of 127 mm2
0 20 in
, so the required spacing is 533 mm
Figure 3.13 of the AASHTO Design Guide provides two charts for esti-
mating tie bar spacing based on the slab thickness and the distance to the
closest free edge of the pavement. Charts are provided for 13 mm (#4) and
16 mm (#5) bars. Tie bar spacing of greater than 1.2 m (48 in) is not rec-
ommended. For the example given above, the recommended tie bar spacing
is 400 mm (16 in) (AASHTO 1993: II-62–II-64). Table 7.2 may also be
used to select tie bar spacing.
Recommended tie bar lengths are 800 mm (32 in) for 13M/#4 bars, 1 m
(39 in) for 16M/#5 bars, 1.18 m (46 in) for 19M/#6 bars, and 1.35 m
(53 in) for 22M/#7 bars (ACPA 1998: 29–30).
154 Design fundamentals
Tiebars should not be placed within [380 mm] 15 inches of trans-
verse joints. When using tiebars longer than [810 mm] 32 inches with
skewed joints, tiebars should not be placed within [450 mm] 18 inches
of the transverse joints. The use of corrosion-resistant tiebars is recom-
mended, as corrosion can reduce the structural adequacy of tiebars. It
is recommended that longitudinal joints be sawed and sealed to deter
the infiltration of surface water into the pavement structure. A [9.5 mm
wide by 25 mm deep] 3/8-inch wide by 1-inch deep sealant reservoir
should be sufficient.
Highway pavement design
High speed, heavy duty highways are an important concrete pavement
application. Concrete pavement has been an essential component of the
interstate highway system in the United States as well as similar systems
around the world.
For many years in the United States, the AASHTO 1993 Design Guide
and its predecessors have been used to design both asphalt and concrete
pavements. Other available concrete pavement design methods include the
PCA 1984 procedure and the AASHTO 1998 Supplement procedure. These
are expected to be replaced by the M-EPDG, but full implementation of the
new procedure will be dependent on local calibration studies and may take
AASHTO 1993 design guide
Based on the results of the AASHO Road Test, AASHTO published design
guides in 1972, 1986, and 1993. These were all similar in overall concept but
incorporated various modifications to account for different environmental
conditions and new technologies. The development of the design equations
is discussed by Huang (2004: 568–570).
The basic AASHTO Design Guide rigid pavement design equation, in US
customary units, is (AASHTO 1993: II-45):
log10 W18 = ZRS0 +7 35 log10 D +1 −0 06+
4 5−1 5
D +1 8 46
156 Highway pavement design
+ 4 22−0 32pt
ScCd D0 75
D0 75 −
where W18 = traffic carried in ESALs, ZR = the standard normal deviate for
the desired reliability, S0 = overall standard deviation, D = slab thickness in
inches, PSI = design change in serviceability index = po −pt po = initial
serviceability index, pt = terminal (final) serviceability index, Sc = flexural
strength of the concrete (psi), Cd = drainage coefficient, J = load transfer
coefficient, Ec = modulus of elasticity of concrete, in psi, and k = modulus
of subgrade reaction in psi/in.
This equation must be solved for D, the design slab thickness in inches.
The following sections discuss the input values for the design equation, and
methods for solving the equation.
The easiest way to use this equation in SI units is to convert Sc and Ec/k,
solve the equation, and then multiply D in inches by 25.4 to get mm. To
convert Sc in kPa to psi, multiply by 0.145. To convert the ratio Ec/k in
[MPa/(MPa/m] to [psi/(psi/in)], multiply by 39.3.
The AASHTO Design Guide (1993) provides detailed instructions for deter-
mining the inputs for equation 8.1.
Traffic in ESALs W18
Axle equivalency factors that may be used to convert single, tandem, and
tridem axles to ESALs are provided in appendix D of the Design Guide, in
tables D.10 through D.18 (AASHTO 1993: D-12–D-20). The equivalency
factors depend on the type of axle (single, tandem, and tridem), the axle load
magnitude (in 8.9 kN or 2 kip increments), the slab thickness D in inches (6
through 14 in in 1 in increments), and the pavement terminal serviceability
index pt (2.0, 2.5, or 3.0).
In theory, this must be an iterative process, because the design thickness
D depends on W18, which depends on the axle equivalency factors, which in
turn depend on D. In practice, it is generally possible to estimate the pavement
Highway pavement design 157
thickness in advance to determine which table to use, based on how heavy the
projected traffic is.
Approximate equivalency factors can be calculated using the 4th power
rule. Examination of the equivalency factor tables shows that 129 kN (29
kip) tandem axles and 173 kN (39 kip) tridem axles are each approxi-
mately equivalent to 80 kN (18 kip) single axles. Therefore, an approximate
equivalency factor EF in SI units may be calculated:
EF = P1/80 4
or P2/129 4
or P3/173 4
where P1 P2, and P3 = load in kN on a single, tandem, or tridem axle,
respectively. In US customary units, the relationship is:
EF = P1/18 4
or P2/29 4
or P3/39 4
where P1 P2, and P3 = loads in kip.
If the projected traffic is not known accurately, it is possible to simply esti-
mate the number of ESALs. Because equation 8.1 is logarithmic, small errors
in calculation of ESALs are not likely to make a great difference in the required
pavement thickness D. After all, how easy is it to predict how many tandem
axles of a given weight will be using a given highway over the next 20 years?
Pavement performance is variable. If it were possible to perfectly predict the
average life of pavements, and design on that basis, then 50 percent of pave-
ments would fail before the end of their expected design lives. Although this
carrying heavy traffic variability demand a higher level of reliability.
Reliability is an important topic and is therefore covered in full chapters
in pavement design textbooks by Yoder and Witczak (1975: Chapter 13)
and Huang (2004: Chapter 10). There are two approaches to reliability.
One approach, used by the PCA 1984 method and traditional structural
engineering procedures, is to use a factor of safety. This is discussed fur-
ther below. The other approach is to assign a specific reliability – for
example, an 85 percent probability that the pavement will not fail before
20 years. Failure is defined as falling below the terminal serviceability
The reliability term in equation 8.1 is the product ZRS0. The overall
standard deviation S0 should be selected based on local conditions, and
may be estimated as 0.35 based on the AASHO Road Test as compared
to 0.45 for flexible pavements, and should be between 0.30 and 0.40 for
rigid pavements. If variability of traffic is considered, 0.39 should be used,
and 0.34 if traffic is not considered (AASHTO 1993: I-62, II-9–II-10).
Therefore, it is probably best to use 0.39 for design.
158 Highway pavement design
Table 8.1 Reliability and standard normal deviate ZR (AASHTO 1993, I-62 and II-9)
Functional classification Recommended level of reliability
Percent ZR Percent ZR
Interstate and other
85–99.9 −1 037
80–99.9 −0 841
Principal arterials 80–99 −0 841
75–95 −0 674
Collectors 80–95 −0 841
75–95 −0 674
Local 50–80 0 50–80 0
−0 841 −0 841
The desired reliability and corresponding standard normal deviate ZR
range from 50 to 80 percent and ZR = 0 to −0 841 for local roads to
85–99.9 percent and ZR = −1 037 to −3 750 for interstate and other free-
ways. Suggested values of reliability and corresponding ZR are shown in
Initial and terminal serviceability po pt PSI
The initial serviceability po depends on how smoothly the pavement can be
built, and the terminal serviceability pt depends on how rough the agency
is willing to let the pavement get before undertaking major rehabilitation.
Based on the results of the AASHTO Road Test, rigid pavements may be
constructed to an initial serviceability po of 4.5, which is 0.3 points higher
than flexible pavements. At terminal serviceability pt of 2.0, 2.5, and 3.0,
respectively, AASHTO estimates that 85, 55, and 12 percent of people
would find the pavement objectionable (AASHTO 1993: II-10).
Flexural strength of concrete Sc
The flexural strength of concrete Sc used in equation 8.1 is the average
28-day third point bending strength. Many agencies have minimum flex-
ural strength specifications for acceptance at 7, 14, or 28 days. Because
of the incorporation of reliability, discussed above, the minimum flexural
strength for acceptance should not be used for design, because the actual
pavement strength will always be greater. Actual flexural strength from test-
ing and construction records may be used or the design Sc may be estimated
as the acceptance strength plus an additional margin (AASHTO 1993:
Highway pavement design 159
Drainage coefficient Cd
As discussed earlier, drainage of concrete pavements is important. The
drainage coefficient Cd ranges from 0.70 to 1.25 based on the quality of
drainage (very poor to excellent) and the percent of time that the pavement
moisture levels approach saturation, from less than 1 percent to greater
than 25 percent. Drainage coefficients are provided in Table 8.2 (AASHTO
The effect of the drainage coefficient is to increase the required pavement
thickness to compensate for poor drainage. Obviously, this will not always
be an effective approach. If drainage is really a problem, it is better to fix
that problem rather than to try to build the pavement thicker to compensate.
Load transfer coefficient J
The load transfer coefficient J actually encompasses three different design
factors – whether or not load transfer devices (dowels) are used, whether
the shoulder is asphalt or tied concrete, and whether the pavement type
is JPCP/JRCP or CRCP. Within each category ranges are given. The total
range is from 2.3 (low end for CRCP with tied concrete shoulders) to 4.4
Table 8.2 Drainage coefficients Cd (AASHTO 1993, II-26)
Quality of drainage Percent of time exposed to moisture
levels approaching saturation
<1% 1–5% 5–25% >25%
Excellent 1.25–1.20 1.20–1.15 1.15–1.10 1 10
Good 1.20–1.15 1.15–1.10 1.10–1.00 1 00
Fair 1.15–1.10 1.10–1.00 1.00–0.90 0 90
Poor 1.10–1.00 1.00–0.90 0.90–0.80 0 80
Very poor 1.00–0.90 0.90–0.80 0.80–0.70 0 70
Table 8.3 Load transfer coefficients J by pavement type (AASHTO 1993, II-26)
Pavement type Shoulder
Asphalt Tied concrete
Load transfer devices
Yes No Yes No
JPCP, JRCP 3.2 3.8–4.4 2.5–3.1 3.6–4.2
CRCP 2.9–3.2 N/A 2.3–2.9 N/A
160 Highway pavement design
(high end for JPCP/JRCP, no dowels, and asphalt shoulders). Load transfer
coefficients are provided in Table 8.3 (AASHTO 1993: II-26).
The load transfer coefficient J has a strong effect on the design thickness.
The most common case is doweled JPCP with asphalt shoulders, with J =
3 2. For highway pavements that carry a substantial number of heavy truck
loads, particularly at high speeds, it is more logical to provide load transfer
devices than to increase the pavement thickness.
Concrete modulus of elasticity Ec
AASHTO recommends using the ACI relationship between compres-
sive strength of concrete and modulus of elasticity Ec (AASHTO 1993:
Ec = 4 730 fc MPa = 57 000 fc psi (8.4)
Modulus of elasticity Ec does not vary substantially across the narrow
strength range of paving concrete, and thus does not have a strong effect
on pavement thickness.
Modulus of Subgrade Reaction k
The AASHTO Design Guide procedure for determining the effective mod-
ulus of subgrade reaction k is complex, and follows these steps (AASHTO
• First, the subgrade k-value is estimated by dividing the resilient modulus
MR by 19.4, in US customary units.
• If the subgrade modulus varies substantially from season to season due
to freezing and/or moisture effects, a seasonally weighted k should be
• The k-value is then adjusted upward for the subbase type and thickness.
• The k-value is then adjusted downward for potential loss of support
due to erosion of the subbase.
• Finally, if bedrock lies within 3.05 m (10 ft) of the surface the k-value
is adjusted upward yet again.
The effect of all of these steps is a k-value usually fairly close to the original
estimate. Loss of support should be avoided by using non-pumping materials
under the slab, not by making the pavement thicker to compensate for
weak support. Furthermore, the slab thickness D is not very sensitive to the
k-value. The simpler methods for determining k outlined in Tables 4.1–4.5
Highway pavement design 161
Equation 8.1 is difficult to solve directly for D. The AASHTO Design Guide
provides a nomograph for determining the solution – with a sharp pencil
and a lot of care, a reasonable degree of accuracy may be achieved. The
equation may also be put into a spreadsheet or other equation solver, or a
Two software packages are available, DarWIN from AASHTO and Win-
PAS from the ACPA. Both packages provide design solutions for both
asphalt and concrete pavements. WinPAS is less expensive and is available
for US $495 from the ACPA bookstore (www.pavement.com). WinPAS may
be used to solve for the pavement thickness D, or for any other variable.
For example, it is possible to determine the reliability of a given pavement
design for a certain projected traffic.
The design example provided here is the example used in the AASHTO
Design Guide to illustrate the use of the nomograph (AASHTO 1993: II-
45), with one exception. The example uses a standard deviation S0 = 0 29,
which is lower than the recommended range, and WinPAS will not accept
this value. Therefore, S0 = 0 30 is used instead. The input values for the
design example are provided in Table 8.4. The design solution is shown
in Figure 8.1. WinPAS provides a design thickness of 9.77 in or 248 mm,
which rounded up to 10 in or 254 mm matches the value from the AASHTO
A few comments may be made. The subgrade value is low, and prob-
ably not compatible with the high level of reliability assumed, which is
Table 8.4 Input values for design example (AASHTO 1993, II-45)
SI units US customary
Modulus of subgrade reaction k 19 MPa/m 72 pci (psi/in)
Modulus of elasticity of
34.5 GPa 5,000,000 psi
Concrete flexural strength Sc 4.5 MPa 650 psi
Load transfer coefficient J 3.2
Drainage coefficient Cd 1.0
Standard deviation S0 0.29 (increase to 0.30)
Reliability and standard normal
95%, – 1.645
Initial serviceability 4.2
Terminal serviceability 2.5
Traffic in ESALs W18 5,100,000
Figure 8.1 WinPAS solution to design problem.
Table 8.5 Sensitivity analysis – effect of design parameters on thickness D
Input value Thickness D inches mm Percent change
Baseline case (Table 8.4) 9.77 248 N/A
Traffic 510,000 ESALs 6.69 170 −31.5
Traffic 4,080,000 ESALs −20% 9.45 240 −3.2
Traffic 6,120,000 ESALs +20% 10.05 255 +2.9
Traffic 51,000,000 ESALs 13.77 350 +40.9
Reliability 80% 8.97 228 −8.2
Reliability 99.9% 12 305 +22.8
Overall deviation 0.49 10.9 277 +11.6
Low strength concrete – S = 550 psi,
E = 3 700 000 psi
10.56 268 +8.1
High strength concrete – S = 750 psi,
E = 5 062 500 psi
9.07 230 −7.1
Load transfer J = 2 6, CRCP with tied
8.76 222 −10.3
Load transfer J = 4 1, no dowels 11.11 282 +13.7
Subgrade k = 50 psi/in 9.89 251 +1.2
Subgrade k = 200 psi/in 9.37 238 −4.1
Saturated >25% with very poor
drainage, Cd = 0 70
11.74 289 +20.1
Saturated <1% with excellent
drainage, Cd = 1 25
8.98 220 −8.1
High terminal serviceability 3.0 10.28 261 +5.2
Low terminal serviceability 2.0 9.42 239 −3.6
Highway pavement design 163
at the upper range even for an interstate highway. For this type of pave-
ment a subbase would be required, leading to a higher k-value. The load
transfer coefficient J corresponds to a doweled pavement (JPCP or JRCP)
with asphalt shoulders. Table 8.5 provides a sensitivity analysis show-
ing the effect of changing various design variables on the required design
It may be seen that traffic has a significant effect when increased or
decreased by a factor of 10, but less of an effect for smaller variations,
say plus or minus 20 percent. The required overall reliability, load trans-
fer coefficient, and drainage coefficient are relatively important. Overall
standard deviation S0, concrete strength and stiffness, modulus of subgrade
reaction k, and terminal serviceability do not have a major effect on design
AASHTO 1998 Supplement
In 1998, AASHTO published a Supplement to the AASHTO Guide for
Design of Pavement Structures, entitled Part II – Rigid Pavement Design &
Rigid Pavement Joint Design. Use of this procedure is illustrated in Figures
8.2 and 8.3. This Supplement provided an alternate to the 1993 design
procedure, and unlike the previous versions was not based on the AASHTO
Road Test results. Instead, the 1998 Supplement procedure was based on
the LTPP data base and NCHRP Project 1–30. Input values remain the same
as for the 1993 procedure, with the addition of the joint spacing. The design
is carried out using free spreadsheet software that may be downloaded from
The Supplement procedure provides a thickness design for JPCP, JRCP, or
CRCP pavement, and also provides a joint faulting check for JPCP or JRCP.
This reference is the source for the k-values provided in Table 4.1. Consid-
erable information is provided on determining the k-value, particularly for
moisture sensitive soils (AASHTO 1998: 2–16).
One additional key input required is the location of the project, and
the associated mean annual wind speed, mean annual air temperature,
and mean annual precipitation. These are provided for two to twelve
cities per US state, in Table 15. For example, Cleveland, Ohio has a
mean annual wind speed of 17.2 kph (10.7 mph), mean annual air tem-
perature of 9 9 C 49 6 F , and mean annual precipitation of 900 mm
164 Highway pavement design
Some further inputs are required:
• Joint spacing in feet. For JPCP, the actual joint spacing is used. For
JRCP, the joint spacing is used up to a maximum of 9.1 m (30 ft).
For CRCP, an arbitrary joint spacing of 4.6 m (15 ft) is used for slab
thickness calculation only.
• Whether the traffic lane is conventional width (3.66 m or 12 ft), con-
ventional width plus tied to a concrete lane, or widened to (4.27 m or
• Modulus of elasticity, thickness, and friction factor for the base.
Figure 8.2 Spreadsheet solution to AASHTO 1998 design example.
Highway pavement design 165
With the design example discussed above and a Cleveland location, the
required pavement thickness for a 4.6 m (15 ft) joint spacing is 267 mm
(10.59 in). Therefore, the thickness produced by the AASHTO 1998 Sup-
plement procedure is a little greater than that from the AASHTO 1993
Design Guide. Changing the design to CRCP does not produce a change in
pavement thickness. Thickness design is shown in Figure 8.2.
The next step in the process is to determine the required dowel diam-
eter. For slabs less than 7.6 m (25 ft) in length, the critical mean joint
Figure 8.3 Spreadsheet faulting check for AASHTO 1998 design.
166 Highway pavement design
Sensitivity analysis (effective subgrade support)
0 100 200 300 400 500 600 700 800
Modulus of rupture =
Elastic modulus of
concrete = 5,000,000
Elastic modulus of
base = 40,000 psi
Base thickness = 0 in
k-value of subgrade =
50 to 800 psi
Joint spacing = 15 ft
Reliability = 95 %
Standard deviation =
Slab thickness = 10.59
Figure 8.4 Sensitivity analysis for AASHTO 1998 design.
faulting limit is 1.5 mm (0.06 in). This also requires the input of the annual
temperature range in degrees, and mean annual freezing index in Fahren-
heit degree-days. For Cleveland, these may be estimated as 90 degrees and
656 F degree-days. With a drainage coefficient of 1 and a pavement age of
25 years, 25 mm (1 in) dowels fail but 32 mm (11/4 in) dowels barely pass.
The joint faulting check is shown in Figure 8.3.
Slab thickness sensitivity may also be performed automatically by the
spreadsheet for modulus of rupture, elastic modulus of the slab, elastic
modulus of the base, base thickness, k-value, joint spacing, reliability, and
standard deviation. Sensitivity analysis for k-value is shown in Figure 8.4.
The supplement also provides a design example, with three different solu-
tions. Solutions are provided for an undoweled JPCP with an aggregate base,
an undoweled JPCP with ATB, and doweled JPCP with aggregate base.
PCA 1984 design
Unlike the AASHTO 1993 and 1998 procedures, the PCA 1984 procedure
is mechanistically based. The charts and tables are based on finite element
calculations of pavement stresses and deflections.
The original guide was set up for hand calculations. The hand calculations
are described in detail by standard pavement textbooks such as Chapter 12
of Huang (2004) and Chapter 21 of Garber and Hoel (2002). The pro-
cedure is outlined below, but the tables and charts are not provided. It is
Highway pavement design 167
simpler to use PCAPAV or StreetPave software, discussed below. Because
the method is iterative, multiple design trials quickly become tedious with
hand calculations. A hand solution is discussed below, but it is very similar
to the StreetPave calculation presented in Chapter 9.
The PCA 1984 design procedure is also listed as an alternate method in
the 1993 AASHTO Design Guide (AASHTO 1993: C-1). Although the PCA
1984 procedure may no longer be widely used for highway pavement design,
it remains relevant for a number of reasons. The procedure provides insight
into the role of various design variables – pavement thickness, dowels, and
tied shoulders – into performance. It is particularly useful for lighter duty
pavements, and has been used to develop design tables for parking lots (ACI
Committee 330: 2001) and for streets and local roads (ACI Committee
325: 2002). An SI version of the Design Guide has been published by the
Canadian Portland Cement Association (CPCA 1999).
Pavements are designed to prevent failure due to either fatigue or erosion.
First, a trial pavement thickness is selected, along with joint and shoulder
details. Then, the fatigue and erosion damage caused by the projected traffic
is calculated, using equation 6.4. If both damage percentages are less than
100 percent, the design is satisfactory. It may, however, be overly conserva-
tive, so a thinner pavement may be tried. If either fatigue or erosion damage
exceeds 100 percent, a thicker pavement is tried.
The PCA 1984 method design inputs are similar to those for other proce-
dures. These include:
• The flexural strength of concrete, as measured through the third point
• Subgrade and subbase support (k-value). The PCA guide includes a rel-
atively simple chart, similar to Table 4.1, for determining the k-value
based on the ASTM soil classification, the AASHTO soil classifica-
tion, resistance value, bearing value, or CBR. The k-value may then be
adjusted upward for an untreated subbase or CTB. These adjustments
are shown in Tables 4.2 and 4.3.
• Doweled or undoweled (aggregate interlock) joints are selected.
• Tied concrete shoulders or no shoulders/asphalt are selected.
• Traffic over the life of the pavement is divided into single and tandem,
axles, and then divided into increments of 8.9 kN (2,000 lb) for singles
and 17.8 kN (4,000 lb) for tandems.
168 Highway pavement design
• Load safety factor – reliability is not addressed specifically in the PCA
1984 procedure. Instead, the axle loads are multiplied by a load safety
factor (LSF) of 1.2 for interstate and other multilane highways, or
1.1 for highways or arterial streets with moderate volumes of truck
First, a trial pavement thickness is assumed. Then fatigue and erosion anal-
ysis are carried out to find the percent damage.
Based on whether or not the pavement has tied concrete shoulders, one
of two charts is selected to determine the equivalent stress for single and
tandem axles. Because tied concrete shoulders convert the loading from
a near edge condition to a near interior condition, they reduce the stress
An example is provided in the 1984 PCA Guide. For example, with a
241-mm (9.5-in) doweled pavement and a subgrade modulus of 35 MPa/m
(130 psi/in), the equivalent stresses for single and tandem axles are 1.42 MPa
(206 psi) and 1.32 MPa (192 psi).
The equivalent stresses are divided by the concrete flexural strength of
4.48 MPa (650 psi) to get stress ratio factors of 0.317 and 0.295 for single
and tandem axles, respectively. Next, the stress ratio is used for each single
and tandem axle load to get an allowable number of repetitions for that axle.
In the example, the pavement is projected to carry 6,320 133 kN (30 kip)
single axles. For a major highway, these are multiplied by an LSF of 1.2 to
get 160 kN (36 kip). A nomograph is used to determine that the allowable
number of load repetitions for this axle is 27,000. Therefore, these axles
consume (6,320/27,000) or 23.3 percent of the pavement fatigue life.
This process is repeated for each single and tandem axle. At some point,
the number of allowable repetitions becomes unlimited and there is no need
to consider this axle or any lighter axles. For this pavement design, an
unlimited number of 98 kN (22 kip) single axles or 214 kN (48 kip) tandem
axles can be carried. Adding up the damage from all of the projected traffic
shows 62.8 percent fatigue damage for this design, less than 100 percent,
so the pavement is satisfactory for fatigue.
Erosion analysis is carried out in a similar manner. Four charts are pro-
vided for doweled or aggregate interlock joints, with and without concrete
shoulders. In the example provided in the 1984 PCA Guide, the pavement
Highway pavement design 169
has doweled joints, but no concrete shoulders. The erosion factors are 2.59
and 2.79 for single and tandem axles, respectively.
Using the nomograph, the allowable number of repetitions of a 160 kN
(36 kip) single axle is 1,500,000 for erosion. Therefore, 6,320 repetitions
of this axle weight consumes 0.4 percent of the pavement’s erosion life.
Adding up the damage from all of the projected traffic shows 38.9 percent
erosion damage for this design, less than 100 percent, so the pavement is
satisfactory for both fatigue and erosion.
PCAPAV and StreetPave software
If the original assumed design thickness is not satisfactory, the process must
be repeated, and hand calculations can become tedious. PCA developed
a DOS program, PCAPAV, to perform the designs. PCAPAV follows the
1984 PCA procedure exactly. The program automatically iterates until a
satisfactory solution is found. More recently, ACPA has developed the
Windows StreetPave program. This program is discussed in more detail in
Introduction to the mechanistic-empirical
pavement design guide
Under NCHRP Project 1-37A, research was carried out to develop a new
pavement design guide to supersede the 1993 guide. At present, the guide
has been completed and a research version is available on the web at
The new design guide is based on mechanistic-empirical principles. The
pavement is analyzed with numerical models, which were calibrated with
pavement performance data from the LTPP program. In essence, the LTPP
program is the “Road Test” on which the new guide has been based. The
procedure is completely software based and cannot be carried out manually.
Some specific points about the guide were made in a memoran-
dum distributed by the AASHTO Task Force overseeing its development
(AASHTO 2004). Some key excerpts from this three page memorandum
are quoted below.
• The M-E pavement design guide uses mechanistic-empirical numer-
ical models to analyze data for traffic, climate, materials, and pro-
posed structure and to estimate damage accumulation over service
life. It is applicable to designs for new, reconstructed, and rehabili-
tated flexible, rigid, and semi-rigid pavements. Performance predic-
tions are made in terms of distress and smoothness. The predicted
distresses for rigid pavement designs (are) faulting, cracking,
and continuously reinforced concrete pavement (CRCP) punchouts.
170 Highway pavement design
Design performance values can be compared with threshold values,
or comparisons of performance may be made for alternate designs
with varying traffic, structure, and materials.
• It must be understood that because the software is a tool for pave-
ment analysis it does not provide structural thickness as an output.
Nor, in its present form, does the M-E pavement design guide
lend itself directly to use as a tool for routine, day-to-day produc-
The design guide is available only in US customary units, and does not
address JRCP. The second point implies that the guide will be used primarily
to develop catalogs or tables of pavement designs for most applications.
Therefore, the guide will probably be used directly only for important
heavy duty highway pavements, or as a forensics tool to analyze pavement
There are a number of key features:
• It is an evaluation process like the PCA 1984 procedure, although
vastly more sophisticated. A pavement structure is proposed, and then
the projected distress and performance over the pavement service life
under the expected traffic and environmental conditions is modeled. If
necessary, the proposed design is adjusted until a satisfactory solution
has been achieved.
• Much more detailed input data is required than for earlier design pro-
cedures. Separate input modules are used for traffic and materials. The
software has a built-in climate model based on the location of the
Huang (2004: 716–727) provides additional details about the proposed
procedure in appendix F of his textbook, entitled “A Preview Of 2002
Pavement Design Guide”:
• The basic concrete pavement analysis module is the finite element pro-
gram ISLAB2000, a successor to ILLI-SLAB.
• Whenever possible, inputs for flexible and rigid pavements are the same
to make it easier to compare alternative pavement types.
• A hierarchical approach for determining design inputs is used. Level 1
inputs are very detailed and project specific, and more accurate, whereas
level 3 inputs will often be default values. Therefore, the designer will
use different amounts of data gathering effort based on the importance
of the project.
• The Guide eliminates the ESAL approach and calculates damage directly
from axle spectra, in a similar manner to the PCA 1984 method and
Highway pavement design 171
• The Enhanced Integrated Climate Model, developed by the FHWA, is
used to provide site specific environmental conditions.
• Pavement roughness in IRI is determined based on pavement distress
over time – for example, cracking, spalling, joint faulting, and other
The implementation of the M-EPDG by state agencies and the FHWA
will be a massive effort. At the time of this writing, the FHWA is spon-
soring workshops, generally one full day, for state highway agencies across
the United States. The workshops are described at http://www.fhwa.dot.
gov/pavement/dgit/index.cfm. Workshop topics include:
• climate considerations;
• traffic inputs;
• local calibration of performance models; and
• materials characterization.
Furthermore, because the models were developed based on national LTPP
data, many state agencies will be conducting research to further refine the
models based on their local conditions. As a result, full implementation of
the M-EPDG will probably take many years, and earlier design methods
(e.g. AASHTO 1993) are likely to remain in general use for some time
Light duty pavement design
Concrete pavements have been widely used for important, heavy duty high-
ways and airports. However, they also have an important place in lighter
duty applications, such as city streets, local roads, and parking lots. For
these applications, the long-term durability and reduced maintenance costs
of concrete pavements may be highly attractive, as well as reducing lighting
requirements at night and reducing heat buildup in warm climates. Con-
crete pavements with textured, patterned, or colored concrete may also be
integrated into the landscape and architecture of neighborhoods to improve
However, for lighter duty pavements the complex methods used for high-
ways and airports would be overkill. Moreover, although the AASHTO
1993 design procedure could be used for these pavements, light duty pave-
ments were not well represented in the AASHO Road Test data used to
develop the method. Furthermore, Huang (2004: 582–583) notes that the
use of the AASHTO 1993 method may produce dangerously unconservative
results for light duty pavements.
In order to develop appropriate light duty pavement designs, ACI Com-
mittees 325 and 330 applied the PCA 1984 method to develop simple design
tables. Also, the ACPA developed StreetPave design software to design
these types of pavements. ACPA has also developed Design of Concrete
Pavements for City Streets, Information Series IS184P (ACPA 1992b).
This chapter contains pavement design tables for parking lots, streets,
and local roads, generated using StreetPave. These are similar to the ACI
325.12R-02 and ACI 330R-01 tables. Because light traffic pavements are
reasonable applications for pervious concrete pavements, design tables for
pervious concrete are also provided.
Concrete intersections are also discussed. These are often used to replace
asphalt intersections that exhibit rutting and other deterioration. Rutting
is more likely with stopped or slowly moving heavy vehicles. Concrete bus
stops may be used for the same reason.
Project quality control and opening the pavement to traffic may be on
the basis of compressive strength, even though the pavement is designed
Light duty pavement design 173
on the basis of flexural strength. Various correlations between flexural
and compressive strength are proposed by ACI Committee 325 (2002),
ACI Committee 330 (2001), and the ACPA (1997). For intersections, the
pavement may generally be opened to traffic once the concrete has achieved
a flexural strength of 3 MPa (450 psi) or a compressive strength of 17 MPa
(2,500 psi) (ACPA 1997: 23).
ACI 325.12R and ACI 330 design guides
ACI Committee 325 published the Guide for Design of Jointed Concrete
Pavements for City Streets and Local Roads in 2002, and ACI Committee
330 published the Guide for Design and Construction of Concrete Parking
Lots in 2001. Both documents are written in dual US customary and SI
units. Maximum average daily truck traffic (ADTT) in two directions is
700 for parking lots and 1,500 for streets and local roads. In addition,
ACI Committee 330 has published the Specification for Unreinforced Con-
crete Parking Lots, ACI 330.1-03 (ACI Committee 330 2003). It includes
“requirements for materials, placing, texturing, curing, jointing, and open-
ing to traffic” (ACI Committee 330 2003: 1).
Because of the lighter traffic loads, undoweled JPCP pavements are often
used. Undoweled, unreinforced pavements also have the advantage of not
being susceptible to steel corrosion from deicing salts and other materials,
because there is no steel to corrode.
Reinforcement is generally only necessary for irregularly shaped panels
with aspect ratios of 1.7:1 or greater. Although reinforcement has been
used in the past with long joint spacing, it is generally better practice to
reduce the joint spacing. ACI 330R-01 states “The use of distributed steel
reinforcement will not add to the load-carrying capacity of the pavement
and should not be used in anticipation of poor construction practices” (ACI
Committee 330 2001: 8–9).
Typical design features
Minimum pavement thickness is generally 100 mm (4 in). Pavement thick-
ness for city streets and local roads may be as much as 200 or 225 mm
(8 or 9 in). Dowels are often used for pavements more than 200 mm (8 in)
thick. Dowels 32 mm (1.25 in) in diameter may be used for pavements up
to 250 mm (10 in) thick, as noted in Table 7.1.
City streets often have curbs and gutters tied to the pavement edge and
or placed integrally with the pavements. This reduces edge-stresses, and
makes it possible to build thinner pavements. Curbs and gutters can also
be built first and used as side forms to construct city street or parking lot
174 Light duty pavement design
not recommended for low-volume design applications. Design options such
as unbound bases, thickened edges, widened outside lanes, or tied curbs and
gutters can be very cost effective” (ACI Committee 325 2002: 7).
With the traffic weights, volumes, and speeds typically carried by low-
volume pavements, pumping is generally not a problem if drainage is ade-
quate. Positive surface drainage of 2 or 2.5 percent also helps prevent
moisture problems (ACI Committee 325 2002: 7). In urban areas, drainage
for city streets and parking lots is often provided by subsurface storm sewer
As with all concrete pavements, the heaviest axle loads tend to control
design and performance. Therefore, it is important to accurately estimate
the number of heavy trucks to be carried by the pavement, particularly
any in excess of legal load limits (ACI Committee 325 2002: 01). These
may be particularly important near industrial facilities. ACI Committee 325
(2002: 11) and ACI Committee 330 (2001: 6) provide the following facility
classifications (Table 9.1).
Design tables for these traffic levels are provided later in this chapter.
Table 9.1 Street and parking lot traffic classifications from ACI 325.12R-11 and ACI-
330R-6 (ACI Committee 325 2002: 11, ACI Committee 330 2001: 6)
VPD or ADT,
Heavy commercial vehicles
(two axle, six tire, and
Percent Trucks per day
Car parking only 0 0 Residential
Truck access lanes 1−10 Residential
Light residential 200 1−2 2−4 Residential
Residential 200−1,000 1−2 2−4 Residential
service lanes, bus,
Collector 1,000−8,000 3−5 50−500 Collector
Bus, truck parking 100−700 Minor arterial
Minor arterial 4,000−15,000 10 300−600 Minor arterial
Major arterial 4,000−30,000 15−20 700−1,500 Major arterial
Business 11,000−17,000 4−7 400−700 Major arterial
Industrial 2,000−4,000 15−20 300−800 Major arterial
Heavy truck parking 700 Major arterial
Vehicles per day or average daily traffic
Light duty pavement design 175
For parking lots, city streets, and local roads, jointing becomes an impor-
tant consideration. Unlike mainline highway pavements, which are straight
for long distances, light traffic facilities have to accommodate intersec-
tions, driveways, drainage structures, and utilities. Most of the joints are
contraction joints, but construction joints are also necessary, as well as
isolation or expansion joints to protect adjacent infrastructure. As a result,
laying out joint patterns for these pavements often requires considerable
Appendix C of ACI 325.12R-02 (ACI Committee 325 2002: 30–32) and
appendix C of ACI 330R-01 (ACI Committee 330 2001: 27–29) provide
examples of joint layouts for various types of facilities. Joint layout is
also discussed in Design and Construction of Joints for Concrete Streets,
Information Series IS061P (ACPA 1992c). Care should be taken that roof
drains from buildings do not drain directly onto parking lot joints, because
the large volumes of water moving at high speed can erode the supporting
layers away rapidly through the joint opening.
Typical joint spacing for pavements in this thickness range is 3–5 m
(12–15 ft). The joint spacing limits of Table 7.3 should not be exceeded.
One advantage of concrete pavements for city street and parking lot
applications is that pavement markings delineating lanes or parking spaces
may be incorporated into the joint pattern, making these features easier for
drivers to follow.
For low-speed facilities such as parking lots, joints may be created using
grooving tools while the concrete is still plastic, in the same manner as
pavements. This technique produces a hard rounded edge at the joint that is
easy to maintain, and any bump produced at the joint will not be noticeable
at low speeds. Joints may also be sawn, in the same manner as high speed
ACPA StreetPave design software
The StreetPave design program allows the engineer to design light duty
concrete pavements using either SI or US customary units. The program is
available from the ACPA (www.pavement.com) for US $100.
The calculation follows the PCA 1984 procedure with a few excep-
tions. Probably the most significant exception is the use of a variable
fatigue curve, based on the desired reliability and the allowable percentage
of cracked slabs. The fatigue relationship is shown in equation 6.5 and
Two other important changes are the addition of a comparable asphalt
pavement design and the addition of a life cycle cost module. Some of the
176 Light duty pavement design
other features and modules are discussed below. Help modules describe the
input parameters in detail.
The program’s global settings are intended to be changed rarely, if at all.
One is the system of units to be used, SI or US customary. Another is
the mean annual air temperature (MAAT), which is based on the project
location and is used only for the asphalt pavement design, using the Asphalt
Institute (AI) design method. The AI design method is discussed at length
in various transportation and pavement design textbooks, such as Chapter
20 of Garber and Hoel (2002) and Chapter 11 of Huang (2004) and will
not be discussed in detail here. An additional global input is the terminal
serviceability index, from the AASHTO design method, which is solely used
to estimate the number of ESALs for the AI design. This input defaults to
2.0 and has little effect on the pavement design.
One important global input is the percent of pavement slabs cracked at
the end of the service life. This ranges from 5 percent for interstate highway
type pavements, to 15 percent for state roads, arterials, collectors, and
county roads, to 25 percent for residential streets. The default value is 15
The percent of allowable cracked slabs is separate from reliability. With
25 percent cracked slabs and 85 percent reliability, there is no more than a
15 percent chance that the project will have more than 25 percent cracked
slabs at the end of its service life. Setting either a low percentage of cracked
slabs or a high reliability will make the design more conservative and more
costly. It will not adjust the asphalt design, so if high or low values of
cracked slabs or reliability are selected, the concrete and asphalt designs
will no longer be comparable.
The project-level inputs are specific to a given project. These include
the project information – project name, project description, route,
owner/agency, location, and design engineer. Two types of project may be
selected – either design of a new pavement, or analysis of an existing pave-
ment. For a new design, in addition to determining the required concrete
thickness, the designer may also elect to determine an equivalent asphalt
pavement thickness and compare life cycle costs.
Two additional key inputs are the pavement design life and the desired
reliability. Design life ranges from 10 to 40 years, with a default value of
20 years. The reliability recommendations of StreetPave are taken directly
from the AASHTO design procedure, as shown in Table 8.1.
Light duty pavement design 177
Probably the single most important traffic input is the traffic category, which
ranges from residential to collector to minor arterial to major arterial. At
each category, the maximum value of the single and tandem axle weights
is different. Table 9.2 shows the average daily traffic (ADT), average daily
truck traffic (ADTT), and maximum single and tandem axle assumed in each
Figure 9.1 and Table 9.3 show the number of single and tandem axles of
various weights (in kN) per 1,000 trucks. Designers may also define their
own traffic spectra, which may include tridem (triple) axles.
Other traffic inputs are the total number of lanes (in both directions),
directional distribution, design lane distribution, either ADTT or ADT and
percent trucks, and truck traffic growth per year. Directional distribution
is normally assumed to be 50 percent in each direction, unless there is
some reason truck traffic will always be heavier in one direction than the
Design lane distribution is the percent of trucks that travel in the outer
lane, and recommendations are provided in a help file and appear auto-
matically as defaults when the number of lanes is selected. For a four lane
highway, the default assumption is 90 percent of heavy trucks in the outer
lane and 10 percent in the inner or passing lane.
ADTT or ADT and percent trucks and estimated growth are typically
estimated by the designer. Default ranges are also provided for ADTT or
ADT and percent trucks, based on the traffic category. For example, the
default ADTT of 1,000 for a major arterial is shown in Figure 9.1. The
truck traffic growth rate default value is 2 percent, with a typical range of
Table 9.2 StreetPave traffic categories from help file
Category Traffic Maximum axle loads – kN
Percent Per day
Residential 200–800 1–3 Up to 25 98 (22) 160 (36)
Collector 700–5,000 5–18 40–1,000 116 (26) 196 (44)
Minor arterial 3,000–12,000 lane,
28–30 500–5,000+ 133 (30) 231 (52)
Major arterial 3,000–20,000 lane,
28–30 1,500–8,000+ 151 (34) 267 (60)
178 Light duty pavement design
Figure 9.1 StreetPave traffic major arterial traffic category.
The pavement properties must be input for the concrete pavement, and also
for the asphalt pavement if a comparison between concrete and asphalt
pavement designs is desired. A submodule may be used to compute the
modulus of subgrade reaction. Other pavement property inputs include:
• Average 28-day concrete flexural strength (MOR), which may be esti-
mated from the 28-day compressive strength.
• Concrete modulus of elasticity, which is computed automatically from
• Whether load transfer dowels are used (yes/no flag).
• Whether edge-support is provided, either through a tied concrete shoul-
der, curb and gutter, or widened lane (yes/no flag).
The modulus of subgrade reaction (k-value) under the pavement may be
input directly. Alternatively, the resilient modulus of the subgrade may be
used, or it may be estimated from the CBR or R-value.
Up to three base/subbase layers may be placed between the slab
and the subgrade. These layers may be econocrete/lean concrete base,
CTB, hot-mix asphalt base, bituminous stabilized mixture, lime-stabilized
180 Light duty pavement design
• Resilient modulus of the subgrade, which is automatically calculated
from the composite modulus of subgrade reaction submodule.
• The subgrade resilient modulus coefficient of variation, which ranges
from 0.28 to 0.38 for projects with homogeneous soils and good
quality control, to 0.59–0.70 for projects with little quality con-
trol of soils, such as municipal or industrial paving with little or
no inspection. The default value is 0.38, taken from the AASHTO
Existing and new pavement analysis
Once all of the inputs have been completed, either an existing pavement
analysis or a new pavement analysis is performed. For an existing pavement
analysis, the concrete thickness is input and either total erosion and fatigue
damage are calculated, or the year in which the pavement will theoretically
fail is calculated.
The new pavement analysis calculates the minimum required thickness
of the concrete pavement, and recommends a thickness rounded up to
the nearest 13 mm (1/2 in). Also, a maximum transverse joint spacing in
meters (feet) is calculated. If dowel bars were selected, the required dowel
diameter is also provided. If an asphalt pavement comparison is required,
the thickness of the asphalt pavement is also calculated.
The new pavement analysis module also provides sensitivity analysis of
the effects of k-value, reliability, concrete strength, percent slabs cracked,
or design life on the required pavement thickness. A six-page design and
analysis summary report is provided for each design.
Life cycle cost
The life cycle cost analysis module allows the comparison of the present
worth of future maintenance costs as well as the initial construction cost
between the concrete and asphalt designs. The comparison is only valid, of
course, if both designs are equally conservative.
The life cycle cost module requires a number of specific inputs:
• Project information – project length, lane width, analysis period, and
either interest and inflation rates or discount rate.
• Densities of the asphalt surface, asphalt base, and aggregate base.
• Initial material costs for concrete material and placement, aggregate
base, and asphalt pavement layers.
• Concrete pavement maintenance and rehabilitation costs – annual main-
tenance, joint sealant, full depth repairs, partial depth repairs, and
Light duty pavement design 181
Figure 9.2 StreetPave life cycle cost module input screen.
• Asphalt pavement maintenance and rehabilitation costs – annual main-
tenance, crack sealing, milling, chip sealing, and seal coat.
• Maintenance and rehabilitation schedule – for each item of Mainte-
nance, Preservation, and Rehab, a year and quantity are selected.
Project inputs/costs are shown in Figure 9.2. Once these have been speci-
fied, the schedule is developed. The program then produces graphs of life
This design example produced using the StreetPave software generally fol-
lows the example from the PCA 1984 Design Guide. The design life is 20
years, and the reliability is 85 percent with 15 percent cracked slabs.
The traffic inputs are shown in Figure 9.3. The pavement is four lane,
with 50 percent directional distribution and 90 percent of the trucks in the
design lane. ADTT is 2,000. The maximum single axle load is 151.2 kN
(34 kip), and the maximum tandem axle load is 266.9 kN (60 kip). These
are higher than the PCA 1984 loads without the LSF, but lower than with
the 1.2 LSF, so they are roughly comparable.
182 Light duty pavement design
Figure 9.3 Design example traffic inputs.
Pavement properties are shown in Figure 9.4. To match the 1984 PCA
design example, the subgrade and subbase k-value is set to 35.1 MPa/m
(130 psi/in). Concrete flexural strength is 4.5 MPa (650 psi) and the concrete
modulus of elasticity is 30.4 GPa (4.4 million psi). Dowels are used, but not
tied shoulders. For this example, a comparable asphalt pavement design is
The pavement design is shown in Figure 9.5. The design concrete thick-
ness is 223.8 mm (8.8 in), which rounds up to 229 mm (9 in). This agrees
closely with the 141 mm (9.5 in) thickness of the 1984 PCA example.
The recommended maximum transverse joint spacing is 4.57 m (15 ft) and
32 mm (11/4 in) diameter dowels should be used.
Figure 9.6 shows the fatigue/erosion table. The pavement has 98.9 percent
fatigue life consumed, but only 11.76 percent of the erosion life consumed.
Dowels could actually be omitted for this pavement, and the erosion life
consumption would become 99.81 percent. However, given the magnitude
and number of the traffic loads, it is better to use dowels.
Most of the fatigue consumption is due to the heaviest single axles – the
1,517 151.2 kN (34 kip) and the 4,310 142.3 kN (32 kip) together consume
Light duty pavement design 183
Figure 9.4 Design example pavement inputs.
over 78 percent of the fatigue, with lighter single axles and tandem axles
contributing little. For doweled pavements, then, the highest single axle
loads are the most significant. There are unlimited allowable repetitions
for single axles 89 kN (18 kip) and lighter and tandem axles 195.7 kN
(44 kip) and lighter. In contrast, virtually all of the axles do a small amount
of erosion damage, with more erosion due to the tandem axles.
The design results also provide a discussion of rounding considerations.
These are shown in Figure 9.7. Rounding the design thickness up increases
the projected life to 33 years, or increases the 20-year reliability to 88.9
percent. Rounding the thickness down reduces the projected life to 8 years,
or reduces the 20-year reliability to 75.4 percent.
StreetPave can calculate sensitivity analysis for k-value, reliability, con-
crete strength, percent slabs cracked, or design life. Figure 9.8 shows
the sensitivity analysis for k-value. A decrease in k-value below approxi-
mately 27 MPa/m (100 psi/in) would require a thicker pavement, and an
increase to 47.5 MPa/m (175 psi/in) or higher would allow a thickness
184 Light duty pavement design
Figure 9.5 Concrete pavement design.
For a city street, the curb and gutter would provide edge-support. Repeat-
ing this design example with edge-support reduces the pavement thickness
from 229 mm (9 in) to 203 mm (8 in). Joint spacing and dowel bar diameter
are the same. If a 7.3 m (24 ft) four-lane pavement is widened to 7.9 m
(26 ft) to widen the truck lane by 0.6 m (2 ft) and provide edge-support,
the widening and reduction of pavement thickness cancel out so that no
additional concrete is required.
Light traffic pavement design tables
The following design tables were prepared using StreetPave software, fol-
lowing the format of ACI 330R-01 and ACI 325.12R-02. These are based
on 85 percent reliability and 15 percent cracked slabs allowed. These tables
apply to parking lots, city streets, and local roads. These tables should
produce design thicknesses close to those found in ACI 330R-01 and ACI
Table 9.4 provides design thicknesses for pavements with aggregate inter-
lock joints and no edge-support, given concrete strengths of 3.45–4.5 MPa
Figure 9.6 Design example fatigue and erosion table.
Figure 9.7 Rounding considerations.
186 Light duty pavement design
14 27 41 54 68 81 95 109 122 136 149 163
Effect of k-value on thickness
Figure 9.8 Sensitivity of slab thickness to k-value.
(500–650 psi) and k-values of 13.5–135 MPa/m (50–500 psi/in). Local
roads often lack edge-support.
Table 9.5 is similar to Table 9.4, but for pavements with edge-support
provided. This is generally the case for parking lots, city streets with concrete
curb and gutter, and pavements with wider edges. The edge-stresses are
reduced, so design thicknesses are decreased.
The use of dowels for all pavements in these tables was investigated. In
only two cases, shown in Table 9.5 for low subgrade support, high concrete
strength, and heavy traffic, was it possible to decrease the thickness. In all
other cases, the required pavement thickness did not change.
For low speed, relatively low truck volume pavements of this type, joint
faulting and pumping do not control the design. Therefore, strictly speaking
dowels are not necessary. They are often included for pavements more than
203 mm (8 in) thick to reduce faulting potential. In harsh climates where
corrosive deicing materials are used, it makes sense to eliminate the dowels
and to instead attempt to reduce faulting by using a stabilized base.
For the design example discussed earlier in this chapter, the ADTT of
2,000 is higher than the traffic provided in the design tables, and the k-value
of 35.1 MPa/m (130 psi/in) is also not in the tables. However, a comparison
may be made with an ADTT of 1,500 and a k of 27 MPa/m (130 psi/in).
For a concrete strength of 4.5 MPa (650 psi), Table 9.4 indicates a design
thickness of 241 mm (9.5 in) for unsupported edges and Table 9.5 indicates
Light duty pavement design 189
Minor 100 165 6 5 178 7 191 7 5 191 7 5
Arterial 300 178 7 191 7 5 191 7 5 203 8
700 178 7 191 7 5 203 8 216 8 5
Major 700 191 7 5 203 8 216 8 5 229 9
Arterial 1500 203 8 203 8 216 8 5 229 9
CBR = 50 135 MPa/m
Concrete flexural strength
kPa psi kPa psi kPa psi kPa psi
4,500 650 4,150 600 3,800 550 3,450 500
Traffic ADTT Required pavement thickness
mm in mm in mm in mm in
Residential 1 114 4 5 114 4 5 127 5 127 5
10 127 5 127 5 140 5 5 140 5 5
Collector 25 140 5 5 140 5 5 152 6 165 6 5
300 152 6 165 6 5 165 6 5 178 7
Minor 100 165 6 5 178 7 178 7 191 7 5
Arterial 300 165 6 5 178 7 191 7 5 203 8
700 178 7 191 7 5 191 7 5 203 8
Major 700 191 7 5 191 7 5 203 8 216 8 5
Arterial 1500 191 7 5 203 8 216 8 5 229 9
a design thickness of 203 mm (8 in). These are close to the values found
Pervious concrete pavement
The ACI A330R-01 and ACI 325.12R-02 design tables as well as Tables 9.4
and 9.5 are limited to concrete with a flexural strength of at least 3.4 MPa
(500 psi). Pervious concrete often has a lower flexural strength than this.
Therefore, the following design tables were developed to address the design
of pervious concrete pavements. Flexural strengths of 2.1–3.1 MPa (300–
450 psi) may be used (Table 9.6).
As with the earlier tables, a truck traffic growth rate of 2 percent per year
is assumed. The concrete modulus of elasticity E is assumed to be 6,750
times the flexural strength or modulus of rupture. The pervious concrete
pavement has no dowels, and is assumed not to have edge-support. If edge-
support were provided, the pavement thickness could be reduced.
At this time, the fatigue relationship for pervious concrete is not known.
As a result, these tables have been developed using 90 percent reliability
rather than 85 percent, to add conservatism to the design until better infor-
mation on the fatigue performance of pervious concrete becomes available.
194 Light duty pavement design
Table 9.6 (Continued)
Minor 100 241 9 5 254 10 280 11 305 12
Arterial 300 254 10 267 10 5 292 11 5 318 12 5
700 267 10 5 280 11 305 12 330 13
Major 700 280 11 292 11 5 318 12 5 356 14
Arterial 1500 280 11 305 12 330 13 356 14
CBR =10 54 MPa/m
Concrete flexural strength
kPa psi kPa psi kPa psi kPa psi
3,100 450 2,750 400 2,400 350 2,100 300
Traffic ADTT Required pavement thickness
mm in mm in mm in mm in
Residential 1 152 6 165 6 5 178 7 203 8
10 178 7 191 7 5 203 8 229 9
Collector 25 203 8 216 8 5 229 9 254 10
300 216 8 5 241 9 5 254 10 280 11
Minor 100 229 9 254 10 267 10 5 292 11 5
Arterial 300 241 9 5 267 10 5 280 11 305 12
700 254 10 267 10 5 292 11 5 318 12 5
Major 700 267 10 5 292 11 5 305 12 343 13 5
Arterial 1500 280 11 292 11 5 318 12 5 343 13 5
Additional conservatism is introduced into the design because the thickness
is rounded up to the nearest even 12.5 mm (1/2 in) increment for ease of
One efficient design concept is to combine pervious and conventional
concrete pavement on the same site. Consider, for example, a four-lane city
street with curb parking. The two center lanes, which carry most of the
traffic, are made of conventional concrete and crowned. The curb lanes
are made of pervious concrete, and are able to handle both the water that
runs off of the conventional concrete and the rain that falls onto them.
They handle less traffic than the two inner through lanes. This combines
the proven durability of conventional concrete streets with the drainage
capacity of pervious concrete.
Along asphalt city streets, intersections often exhibit considerable rutting
and shoving due to the starting, stopping, and turning motions of heavy
Light duty pavement design 195
At busy intersections, the added load and stress from heavy vehicles
often cause asphalt pavements to deteriorate prematurely. Asphalt sur-
faces tend to rut and shove under the strain of busses and trucks
stopping and turning. These deformed surfaces become a safety con-
cern for drivers and a costly maintenance problem for the roadway
(ACPA 1997: 1)
Asphalt is a viscoelastic material – therefore, rutting progresses more rapidly
under stopped or slowly moving heavy vehicle loads than under faster
Bus stops often exhibit similar distress. Also, because intersections receive
traffic from four directions, they carry up to twice the traffic as the city
streets that they connect. Replacing deteriorated asphalt intersections with
concrete can considerably reduce maintenance costs. A detailed 28-page
guide to concrete intersections has been published by the ACPA as TB019P,
entitled Concrete Intersections: A Guide for Design and Construction
In addition to paving the physical area of the intersection, it is generally
necessary to include the entire functional area where vehicles slow, stop,
and accelerate. This may include 30–60 m (100–200 ft) on either side of
the intersection, or it may be offset in the direction of approaching traffic
to provide 60–120 m (200–400 ft) on the approach, but only 15 m (50 ft)
past the intersection. With moderate traffic volumes and a low percentage
of heavy vehicles, 15–30 m (50–100 ft) on either side of the intersection
may be sufficient (ACPA 1997: 2).
Intersection pavement design thickness ranges from 100–125 mm (4–
5 in) for light residential up to 150–225 mm (6–9 in) for minor arterial and
175–275 mm (7–11 in) for major arterial streets. Traffic from all directions
coming into the intersection must be considered for the physical area, which
may require increasing the pavement thickness 13–25 mm (1/2–1 in) over
that in the functional area of the intersection (ACPA 1997: 3–4). Pavement
thickness may be determined using the design tables above, or by using
Jointing considerations are important, and are similar to those for city
street pavements, with a few additional considerations. Isolation joints are
generally necessary for skew intersections and for the perpendicular street at
T-intersections. They are also needed at manholes, drainage fixtures, pave-
ments, aprons, and structures. It is important to develop a good jointing
plan in advance, and make field adjustments as necessary. It is not uncom-
mon for the actual physical location of some features, such as manholes, to
vary somewhat from what is shown on the plans (ACPA 1997: 4–9). An
isolation joint is shown in Figure 2.4.
196 Light duty pavement design
Sample joint plans for typical intersection configurations are shown
on page 10 of TB019P, Concrete Intersections: A Guide for Design and
Construction (ACPA 1997). Additional details and configurations are pro-
vided in IS006.01P, Intersection Joint Layout, which provides a ten-step
example (ACPA 1996b).
It is often necessary to maintain traffic through intersections during con-
struction, so project phasing may be important. If possible, it is preferable
to detour traffic away from the intersection to simplify and speed construc-
tion. This depends on having available alternate routes to handle the traffic.
To maintain traffic through the intersection, construction may be divided
into four phases by lane, or into four phases by quadrant (ACPA 1997:
9–11). Figure 9.9 shows quadrant construction at an urban intersection in
downtown Cleveland, Ohio.
Intersections must often accommodate vehicle detector loops. Inductive
loop detectors are used to magnetically detect the presence of vehicles in
order to start or extend traffic signal green time. They require wire loops
embedded in the pavement. Often, 6-mm (1/4-in) wide saw cuts 50 mm
(2 in) deep are made in the pavement for wires, and then sealed. Loops may
also be cast into the pavement, although in this case it is important that
Figure 9.9 Quadrant construction at an urban intersection in Cleveland, Ohio (photo by
Light duty pavement design 197
they be placed a minimum of 50 mm (2 in) above any reinforcing steel and
offset as much as possible (ACPA 1997: 25).
RCC composite pavements
In some areas, including Columbus, Ohio, and Quebec, Canada, composite
pavements consisting of an RCC structural base with a thin asphalt overlay
as a riding surface have been used. An RCC composite pavement base
under construction is shown in Figure 2.10. In the Columbus area, this type
of pavement has proven to be more economical than either conventional
concrete or asphalt pavements.
A relatively simple design method has been developed for this type of
pavement (Delatte 2004). However, since the asphalt contributes little to
the structural capacity of the composite pavement, the designs provided in
this chapter in Table 9.4 are conservative and may be safely used.
Short, thin slab pavements
Covarrubias (2007) has recently developed a patented short, thin slab pave-
ment system capable of carrying heavy truck loads. In this system, small
square slabs are used, no more than half a lane in width. Slab dimen-
sions are similar to those used for thin whitetopping, as discussed in
Key features of the Covarrubias system include:
• Shorter slab dimensions, approximately 1.8 m (6 ft) square.
• Due to the small slab size, curling and warping stresses are very low.
The slabs therefore have full bearing on the base and are not at a high
risk of corner breaks.
• Due to the small slab size, only one wheel load is on a slab at a time,
so there are no negative bending stresses due to multiple wheel loads.
Slabs must be shorter than the distance between truck front and rear
• Joints cut using a thin 2 mm (0.08 in) saw blade, with an early entry
• Due to the small slab size and tight joints, no dowels or tie bars are used.
• Pins are used along the pavement edges to hold the transverse joints
• Drainable base is used to prevent distress from water penetrating
through the narrow joints. CTBs, ATBs or granular materials with less
than 6 percent fines may be used.
With this system, a short slab pavement only 150-mm (6-in) thick has
the same stress, and thus the same fatigue life, as a conventional 230-mm
198 Light duty pavement design
(9-in) thick pavement. This technology has been demonstrated with trial
sections in Puerto Montt and Temuco in Chile in January 2005 and 2006,
respectively. At these sites, slabs as thin as 80 mm (3.1 in) over granular
base have carried 70,000 standard axle loads to date. The concrete flexural
strength was 4.8 MPa (700 psi).
Airport pavement design
There are important differences between highway and airport pavements.
Yoder and Witczak (1975: 559) note
The number of repetitions of load is considerably less, but, on the
other hand, gross load on the airfield pavement is greater than on the
highway. Pumping can be a major problem on highways but is of lesser
importance for rigid airfield pavements. In addition, a major portion of
the load is applied just several feet from the edge of the rigid highway
pavement, but loads are primarily in the center of airfield slabs.
The FAA notes that
The design of airport pavements is a complex engineering problem
that involves a large number of interacting variables An airfield
pavement and the aircraft that operate on it represent an interactive
system that must be addressed in the pavement design process. Design
considerations associated with both the aircraft and the pavement must
be recognized in order to produce a satisfactory design. Producing a
pavement that will achieve the intended design life will require careful
construction control and some degree of maintenance. Pavements are
designed to provide a finite life, and fatigue limits are anticipated.
Poor construction and a lack of preventative maintenance will usually
shorten the service life of even the best-designed pavement.
(FAA 2004: 23)
In the past, some runway pavements were built with keel sections. Keel
sections use thicker pavement near the runway centerline, and thinner
pavement along the edges, because few aircrafts are expected at or near
the edges. To prevent abrupt changes and stress concentrations, the pave-
ment thickness is often tapered (Packard 1973: 20–21). Yoder and Witczak
(1975: 592) suggested that the outer edges could be reduced by 30
200 Airport pavement design
Variable or keel cross-sections are now less common. The FAA notes
Airport pavements are generally constructed in uniform, full width sec-
tions. Runways may be constructed with a transversely variable section,
if practical. A variable section permits a reduction in the quantity of
materials required for the upper paving layers of the runway. However,
more complex construction operations are associated with variable sec-
tions and are usually more costly. The additional construction costs
may negate any savings realized from reduced material quantities.
(FAA 2004: 27)
Design procedures for airfield pavements have been developed in the United
States by the FAA for civilian airfields and by the USACE for mili-
tary airfields. The FAA advisory circulars that pertain to design and
construction may be downloaded free from http://www.faa.gov/airports_
airtraffic/airports/resources/advisory_circulars/. The PCA also developed
procedures, which have later come under the ACPA purview. Packard
(1973) authored Design of Concrete Pavement, which was supplemented
by design charts for various aircraft types. The FAA allows the use of PCA
procedures, which have now been updated by the ACPA with AIRPave
Military airfields are not covered in this book. In the United States, mili-
tary airfields are designed and built using UFC 3-250-02 “Standard Practice
Manual for Rigid Pavements,” (UFC 2001a) and UFC 3-260-02 “Pavement
Design for Airfields” (UFC 2001b). These documents are available on the
web at http://22.214.171.124/report/doc_ufc.html.
It is important to understand that both civilian and military airport
pavement design procedures assume an interior loading condition. In rare
circumstances where aircraft wheels travel near an unsupported edge, these
procedures are not valid. For example, a 30 m (100 ft) diameter circular
power check pad was built at a military airfield. These pads are intended
to anchor high performance jet aircrafts in order to test engines. As the
aircraft exits the pad, the main gear traverses the outside slab edges, so the
interior loading condition design assumption was violated. The edge-slabs
failed rapidly with widespread cracking (Rollings 2005: 167–168).
Airport pavement bases and subbases
Base and subbase layers, including drainage layers, are widely used in civil-
ian and military airport pavements. Hall et al. (2005: 1–2) note
When specified, designed, and properly constructed, stabilized and per-
meable bases have a positive impact on pavement performance. How-
ever, to ensure success, the selection and specification of these layers
Airport pavement design 201
should be considered in the overall context of the rigid pavement design
and construction process.
Stated in another way, mere inclusion of these bases in the typical
section is not adequate to guarantee pavement performance under all
situations. On the contrary, if careful attention is not paid to how these
layers alter the early-age and long-term performance of pavements, they
could even prove not as beneficial as anticipated. Design details of
the PCC layers (thickness, joint spacing, etc.), PCC mixture properties,
ambient conditions at the time of paving, and curing and jointing of
the PCC layer interact with the base layer’s as-constructed stiffness,
thickness, and friction properties to create a unique set of circumstances
for each project which need to be carefully accounted for to ensure a
successful end product.
The Innovative Pavement Research Foundation report Stabilized and Drain-
able Base for Rigid Pavement: A Design and Construction Guide, Report
IPRF-01-G-002-021(G) (Hall et al. 2005) discusses the higher risks of
uncontrolled early-age cracking with certain base types and how to reduce
those risks. Some of these factors should be addressed during design,
and some during construction. Construction aspects are addressed in
Hall et al. (2005: 13) suggest that stabilized base layers should be 152–
203 mm (6–8 in) thick and permeable bases should be 102–152 mm (4–6 in)
thick for airfield pavements. In this thickness range, the bases may be placed
without segregation and permeable bases will have adequate permeability.
For airports, rigid pavement stabilized layers typically include Item P-304,
CTB, Item P-306 Econocrete Subbase Course or LCB, and Item P-401 or
P-403 ATB (FAA 2005). These materials are discussed in Chapter 4 of this
book, and their construction is discussed in Chapter 13.
Standard FAA design procedures are discussed in Chapter 3 of FAA
Advisory Circular AC 150/5320-6D (FAA 2004). These procedures are
intended to address airports serving aircraft with gross weights of 13,000 kg
(30,000 lb) or more. The same general procedures and considerations apply
to both flexible and rigid pavements, although the specific design methods
are different. For airports with only lighter aircraft, a separate and simpler
design method has been developed, which is discussed in a later section.
The FAA standard design procedures are intended to provide pavements
with structural lives of 20 years, although during that time there may be
a need for some rehabilitation and renewal of skid resistance (FAA 2004:
202 Airport pavement design
Determining equivalent annual departures of design
Standard gear configurations are assumed for single gear, dual gear, dual
tandem gear, and wide body aircraft. Triple dual tandem gear aircraft
are addressed separately by the new Chapter 7 – layered elastic design
procedures. Tire pressures vary between 515 and 1,380 kPa (75 and 200 psi)
(FAA 2004: 24).
The design is based on a single design aircraft type.
The forecast of annual departures by aircraft type will result in a list
of several different aircraft. The required pavement thickness for each
aircraft type in the forecast should be checked using the appropriate
design curve and the forecast number of annual departures for that
aircraft. The design aircraft is the aircraft type that produces the greatest
pavement thickness. It will not necessarily be the heaviest aircraft in
the forecast Since the traffic forecast is a mixture of aircraft having
different landing gear types and different weights, the effects of all
traffic must be accounted for in terms of the design aircraft. First,
all aircraft must be converted to the same landing gear type as the
design aircraft. The FAA has established factors to accomplish this
conversion. These factors are constant and apply to both flexible and
rigid pavements. They represent an approximation of the relative fatigue
effects of different gear types.
(FAA 2004: 24–25)
The conversion factors used to convert from one landing gear type to
another are shown in Table 10.1.
After converting the aircraft to the same landing gear configuration,
convert them to equal annual departures of the design aircraft:
Log R1 = Log R2 ×
R1 = equivalent annual departures by the design aircraft;
R2 = annual departures of the aircraft in question;
W1 = wheel load of design aircraft;
W2 = wheel load of the aircraft in question.
Wide body aircraft have significantly different landing gear assembly spac-
ings, so wide body aircraft are treated as 136,100 kg (300,000 lb) dual
tandem aircraft for computing equivalent annual departures, even when
they are the design aircraft (FAA 2004: 25).
Airport pavement design 203
As an example, Table 10.2 shows the annual departures for eight differ-
ent types of aircraft. The B727-200 is determined to be the design aircraft
because its 9,080 annual departures would require the greatest pavement
thickness. Therefore, the aircraft are all converted to dual wheel type by
using the appropriate factor from Table 10.1, and then the equivalent
annual departures are determined using equation 10.1. The equivalent
annual departures of a B727-200 are shown as 16,241 in Table 10.2.
For example, the 3,050 average annual departures of the B707-320B with
dual tandem gear type is multiplied by 1.7 to get 5,185 equivalent dual gear
departures. Next, apply equation 10.1 with W1 = 20,520 kg (45,240 lb)
and W2 = 17,610 kg (38,830 lb):
Log R1 = Log 5,185 ×
= 3 44
Table 10.1 Landing gear type conversion factors (FAA 2004: 25)
To convert from To Multiply departures by
Single wheel Dual wheel 0.8
Single wheel Dual tandem 0.5
Dual wheel Single wheel 1.3
Dual wheel Dual tandem 0.6
Dual tandem Single wheel 2.0
Dual tandem Dual wheel 1.7
Double dual tandem Dual tandem 1.0
Double dual tandem Dual wheel 1.7
Table 10.2 Forecast traffic and equivalent annual departures (FAA 2004: 26)
(a) Forecast departures
Aircraft Gear type Average annual
727-100 Dual 3,760 72,580 160,000
727-200 Dual 9,080 86,410 190,500
707-320B Dual tandem 3,050 148,330 327,000
DC-9-30 Dual 5,800 49,000 108,000
CV-880 Dual tandem 400 83,690 184,500
737-200 Dual 2,650 52,390 115,500
L-1011-100 Dual tandem 1,710 204,120 450,000
747-100 Double dual tandem 85 317,520 700,000
204 Airport pavement design
Table 10.2 (Continued)
(b) Equivalent annual departures
Aircraft Equiv. dual
Wheel load Wheel load
kg lb kg lb
727-100 3,760 17,240 38,000 20,520 45,240 1,891
727-200 9,080 20,520 45,240 20,520 45,240 9,080
707-320B 5,185 17,610 38,830 20,520 45,240 2,764
DC-9-30 5,800 11,630 25,650 20,520 45,240 682
CV-880 680 9,940 21,910 20,520 45,240 94
737-200 2,650 12,440 27,430 20,520 45,240 463
L-1011-100 2,907 16,1601
20,520 45,240 1,184
747-100 145 16,1601
20,520 45,240 83
Wheel loads for wide-body aircraft are taken as the wheel load for a 136,100 kg (300,000 lb) dual
tandem aircraft for equivalent annual departure calculations
Finally, 103 44
= 2 764 annual departures of the design aircraft (B727-100).
As noted previously, the wide bodied aircraft in the table (L-1011-100 and
B747-100) are treated as 136,100 kg (300,000 lb) dual tandem aircraft.
This is a very straightforward calculation to set up with a spread-
sheet. The weights of many aircraft are listed in FAA Advisory
Circular (AC) 150-5300-13 Airport Design (FAA 1989) or may be
found in the Aircraft Characteristics Data Base online http://www.
Design for frost and permafrost
Airfield pavement designs must consider climatic conditions, particularly
where adverse effects of seasonal frost or permafrost apply. Two approaches
are available for designing for seasonal frost. The first approach is to ensure
that the combined thickness of pavement and non-frost-susceptible material
is sufficient to eliminate or limit frost penetration into the subgrade. The sec-
ond approach is to provide a pavement strong enough to carry load during the
critical frost melting period. Three design procedures are available:
1 Complete frost protection – the depth of frost penetration is developed
using procedures in FAA AC 150/5320-6D Chapter 2, and the design
thickness of pavement is compared to this depth. If frost will penetrate
Airport pavement design 205
deeper than the pavement thickness, subgrade material must be removed
and non-frost-susceptible material provided. This is the most positive
and costly method of frost protection. In any case, frost protection is
normally limited to a maximum of 1.8 m (6 ft).
2 Limited subgrade frost protection – this method is similar to that above
but frost protection is only provided to 65 percent of the depth of
frost penetration. This method will not eliminate frost heave but will
generally keep it to a tolerable level.
3 Reduced subgrade strength – based on the soil frost groups defined in
FAA AC 150/5320-6D Chapter 2, the subgrade modulus is reduced
to 6.8–13.5 MPa/m (25–50 psi/in). This reduced value is then used to
determine the pavement thickness. This approach ignores the effects of
frost heave (FAA 2004: 27–29).
The design of pavements in permafrost regions must consider not only
the effects of seasonal thawing and refreezing, but also the effects of
construction on the existing thermal equilibrium. Changes in the sub-
surface thermal regime may cause degradation of the permafrost table,
resulting in severe differential settlements [and] drastic reduction of
pavement load carrying capacity.
(FAA 2004: 29)
Design approaches for permafrost include the complete protection method,
the reduced subgrade strength method, and the less common insulating
panel method. The first two methods are similar to those for ordinary frost
protection discussed in the previous paragraph (FAA 2004: 29–30). There
is no difference in the FAA design procedures for frost and permafrost
between rigid and flexible pavements.
FAA rigid pavement design
The FAA pavement design procedure may be carried out using design curves.
are based on the Westergaard analysis of edge loaded slabs. The edge
loading analysis has been modified to simulate a jointed edge condition.
Pavement stresses are higher at the jointed edge than at the slab interior.
Experience shows practically all load-induced cracks develop at jointed
edges and migrate toward the slab interior. Design curves are furnished
for areas where traffic will travel primarily parallel or perpendicular to
joints and where traffic is likely to cross joints at an acute angle. The
thickness of pavement determined from the curves is for slab thickness
only. Subbase thicknesses are determined separately.
(FAA 2004: 23)
206 Airport pavement design
Determining foundation modulus (k-value)
The k-value is established for the subgrade and then corrected for the
subbase to a higher value. A plate bearing test is preferred to establish the
subgrade k-value, but correlations such as those shown in Chapter 4 may
be used instead. The FAA notes that “Fortunately, rigid pavement is not
overly sensitive to k value, and an error in estimating k will not have a large
impact on rigid pavement thickness” (FAA 2004: 56).
For both granular and stabilized subbases, charts and tables from various
sources may be used to determine the composite k based on the subgrade
k and the thickness and type of subbase. Tables 4.2 through 4.5 from
Chapter 4 provide reasonable values.
Determining concrete slab thickness
Once the composite k under the concrete slab has been determined, the
concrete flexural strength is used to determine the concrete slab thickness
for a given aircraft type, gross weight of design aircraft, and number of
annual departures. The concrete flexural strength is based on the strength
that the concrete is required to have when it is opened to traffic, tested by
ASTM C78 (ASTM C78 2002). In other words, if the pavement will be 3
months old when opened to traffic, the acceptance of the concrete is on the
basis of 28-day flexural strength but the design should be on the basis of
Separate design curves or nomographs are provided for each aircraft type
on pages 59 through 83 of FAA AC 150/5320-6D. To use each chart, the
concrete flexural strength is the first input and a horizontal line is carried
across to the line representing the appropriate modulus of subgrade reaction
k. From that intersection point, a line is drawn vertically downward to the
line representing the gross aircraft weight. Finally, from that intersection
point a line is drawn horizontally to the right to intersect with the number
of annual departures and determine a design slab thickness. A dashed line
is provided on each chart to indicate the procedure (FAA 2004: 58).
With eight different aircraft in the forecast traffic, this procedure must be
carried out eight times – once for each aircraft, with its appropriate design
chart. This will produce eight different required slab thickness values. The
thickest value determines the design aircraft. Once the design aircraft has
been determined, the procedure outlined above is used to determine the
numbers of equivalent annual departures of the other seven aircraft types.
Since this manual procedure is obviously quite tedious, a spread-
sheet computer program R805faa.xls has been developed and
may be downloaded free from the FAA website, http://www.
faa.gov/airports_airtraffic/airports/construction/design_software/. The use
of the spreadsheet is illustrated in a design example below.
Airport pavement design 207
Critical and non-critical areas
FAA defines critical and non-critical areas for runway pavement. Critical
areas include taxiways and the center sections of runways, as shown in
Figure 3.1 of FAA AC 150/5320-6D. Non-critical areas include outer edges
of runways. In non-critical areas, the pavement thickness may be reduced
10 percent (FAA 2004: 58).
High traffic volumes
The design charts go up to 25,000 annual departures. Some airports have
more air traffic. With high traffic volumes, a stabilized subbase should
be used, and pavement thickness may need to be slightly increased. Joint
spacing may also be decreased to minimize joint movements and improve
load transfer, and high quality joint sealants should be specified (FAA
Joint spacing and configuration is an important element of the FAA design
procedure. Joints are classified as expansion, contraction, and construction
joints, as discussed in Chapter 2. If an unstabilized subbase is used under
the pavement, the maximum joint spacing listed in Table 10.3 may be used.
Pavements with extreme temperature differentials during placement or in
service should use shorter spacings (FAA 2004: 85–87).
If a stabilized subbase is used, the higher subbase k-values increase curling
and warping stresses. Therefore, the joint spacing should be limited to five
times the radius of relative stiffness of the slab (FAA 2004: 87). The radius
of relative stiffness is calculated using equation 7.1, and the maximum slab
length may be determined using Figure 7.3.
Joints are generally doweled, although the FAA AC 150/5320-6D allows
keyed joints for slabs 230 mm (9 in) thick or more. Keyed joints are not
Table 10.3 Maximum joint spacing for unstabilized base (FAA 2004: 87)
Slab thickness Transverse and longitudinal joint spacing
mm in m ft
150 6 3.8 12.5
175–230 7–9 4.6 15
230–305 9–12 6.1 20
>305 >12 7.6 25
208 Airport pavement design
Table 10.4 FAA dowel bar recommendations (FAA 2004: 88)
Slab thickness Dowel diameter Dowel length Dowel spacing
mm in mm in mm in mm in
150–180 6–7 20 3/4 460 18 305 12
210–305 8–12 25 1 480 19 305 12
330–405 13–16 30 11/4 510 20 380 15
430–510 17–20 40 11/2 510 20 460 18
535–610 21–24 50 2 610 24 460 18
recommended when wide-body aircraft use the pavement and the founda-
tion modulus is 54 MPa/m (200 psi/in) or less (FAA 2004: 87).
FAA recommendations for dowel bar diameter, length, and spacing are
based on the slab thickness. These recommendations are shown in Table 10.4.
These dowel diameters are smaller than those given in Table 7.1, so
the more conservative recommendations of Table 7.1 may be used instead.
Dowels are generally solid bars, but may be high-strength pipe plugged on
each end with a tight fitting cap or with a bituminous or mortar mixture. Tie
bars should be deformed bars 16 mm (5/8 in) in diameter spaced 760 mm
(30 in) on center (FAA 2004: 88).
Reinforced and CRC pavements
The FAA AC 150/5320-6D allows JRC and CRC airfield pavements in
addition to JPC. Reinforcement allows longer joint spacing, up to 23 m
(75 ft). Naturally joint openings will be larger and will require more care
to seal and maintain (FAA 2004: 89–93). CRC steel design for airport
pavements is addressed in Chapter 12.
Layered elastic pavement design
FAA airport pavement design procedures were substantially updated in
2004 to provide for new, larger aircraft, particularly the Boeing 777
and the Airbus A-380. Substantial changes were made to Section 3, rigid
pavement design, of Chapter 3, pavement design, and Chapter 7, lay-
ered elastic pavement design. Previously, design relied on curves developed
using the Westergaard stress equations, modified to model a jointed edge
The revised FAA AC 150/5320-6D states on p. 141 that
the design procedure presented in this chapter provides a method of
design based on layered elastic analysis developed to calculate design
thicknesses for airfield pavements. Layered elastic design theory was
Airport pavement design 209
adopted to address the impact of new gear and wheel arrangements
such as the triple dual tandem (TDT) main gear.
The Boeing 777 and the Airbus A-380 are examples of aircraft that
utilize this gear geometry. The TDT gear produces an airport pavement
loading configuration that appears to exceed the capability of the pre-
vious methods of design, which incorporate some empiricism and have
limited capacity for accommodating new gear and wheel arrangements.
This design method is computationally intense and is thus in the form
of a computer program called LEDFAA.
(FAA 2004: 141)
LEDFAA may be downloaded free from the FAA website, http://www.
faa.gov/airports_airtraffic/airports/construction/design_software/. Some of
the features of LEDFAA include:
• Designs may be carried out using either SI or US customary units.
• An extensive aircraft library is included and designers may adjust air-
• The basis of the design is layered elastic theory rather than the Wester-
• A pavement design life other than 20 years may be considered, although
this is a deviation from FAA standards.
• The aircraft traffic mix is not converted to equivalent departures of a
single design aircraft. Instead, for rigid pavements, the fatigue damage
caused by each aircraft is calculated. This is similar to the PCA/ACPA
1984 and StreetPave design method for highway pavements.
• Pavement materials are characterized by thickness, modulus of elas-
ticity, and Poisson’s ratio. Materials may be identified using their
FAA specification designations, such as P-209 for crushed stone base
• The program does not automatically check that layer requirements are
met – for example, the requirement for stabilized subbase layers under
rigid pavements with wide body aircraft in the traffic mix. This is left
to the designer (FAA 2004: 141–142).
Because of differences in philosophy between layered elastic design and the
previously used FAA design procedure, there are also limitations placed on
the use of LEDFAA by the FAA:
• If the aircraft traffic mix does not include aircraft with the TDT
gear configuration, the previously used procedure should be used
(i.e. Chapter 3 of FAA 2004) and the minimum pavement thickness
determined using that procedure applies.
210 Airport pavement design
• The procedure should not be used to determine thickness requirements
for an individual aircraft – the entire traffic mixture must be used.
• The program may not be used to evaluate existing pavements that
were designed using the previous FAA design procedure (FAA 2004:
The concrete pavement must be at least 152 mm (6 in) thick. Stabilized
subbases are required under rigid pavements serving aircraft with TDT
gear, with a minimum layer thickness of 102 mm (4 in). The subgrade is
assumed to be elastic and infinite in thickness and characterized by an elastic
modulus or k-value. The program converts an input k-value to an elastic
modulus. In US customary units, the subgrade E = 26 k1 284
143–144). Since the layered elastic design requires software, the procedure
is discussed in the following section.
Airfield pavement design software
The FAA provides software for the standard and layered elastic design
procedures. The ACPA has also developed a computer program, ACPA
AirPave, which is based on the PCA design procedure (PCA 1966).
AirPave can only determine stresses and allowable repetitions for a single
aircraft gear configuration at a time. However, the number of allowable
repetitions for each aircraft in the traffic stream may be determined using
AirPave, and then equation 6.4 may be used to compute the cumulative
damage for the pavement. If necessary, the design can then be adjusted.
Therefore, AirPave is convenient when designing an airfield pavement for
a single aircraft type, but the FAA procedures are more useful for mixed
traffic. The use of AirPave is very similar to RCCPave, which is discussed
in detail in Chapter 11.
Standard FAA design procedure (Chapter 3)
As noted above, the FAA has developed spreadsheet design software,
the program R805faa.xls, which may be downloaded free from the
FAA website, http://www.faa.gov/airports_airtraffic/airports/construction/
design_software/. The instructions file for the spreadsheet may be down-
loaded from the same website.
The basic program screen is shown in Figure 10.1. The eight design steps
are carried by activating the various input screens in order. Step 1 is the
basic airport and design information and does not affect the calculations.
Step 2 requires the input of the subgrade k-value, the subbase type and
thickness, and the necessary information for subgrade frost design if it is
required. Any of the frost design procedures discussed above may be used.
212 Airport pavement design
The frost design input screen is shown as Figure 10.2. Frost design may be
If the pavement is to be designed for frost, a number of additional inputs
are required, including the air freezing index in degree–days, the dry unit
weight of the soil, and the subgrade soil frost code (non-frost or F-1 through
F-4). These are used to calculate the depth of frost penetration. Alterna-
tively, the reduced subgrade strength may be used.
Continuing with step 2, the subgrade/stabilized subbase/aggregate sub-
base values are input. These are shown in Figure 10.3. The input subgrade
k-value of 27 MPa/m (100 psi/in) is automatically adjusted by the program
for the 150 mm (6 in) of stabilized base to 57 MPa/m (215 psi/in).
The concrete properties are input in step 3. The main input is the concrete
flexural strength. The Poisson’s ratio is assumed to be 0.15 and the concrete
modulus of elasticity is assumed to be 27.6 GPa (4,000,000 psi), although
these default values may be changed.
The projected aircraft forecast is entered in steps 4–6. Up to 21 different
aircraft types may be included. Aircraft types are entered one at a time, as
shown in Figure 10.4, which repeats the calculations shown in Table 10.2.
Figure 10.3 FAA R805FAA.xls rigid airport pavement design spreadsheet computation of
Airport pavement design 213
Figure 10.4 Determining critical aircraft.
For each aircraft type, the required inputs are the gear configuration,
maximum takeoff weight, and annual departures (columns 2 through 4). A
descriptive user name for each aircraft type (column 1) is optional. Some
aircraft are already provided in the library, such as the L1011 and 747-
100, and some are listed as gear configurations and an approximate gross
aircraft weight in thousands of pounds, such as DUAL TAN-300 which is
a dual tandem of approximately 136,000 kg (300,000 lb).
Once all of the aircraft have been entered, the pavement thickness for
each aircraft is calculated by clicking the step 5 button. This provides the
recommended critical aircraft, in this case the B727-200 as shown in both
Table 10.2 and Figure 10.4. Next, the step 6 button is clicked to accept the
critical aircraft and complete the design.
The program also offers an option to compute an overlay thickness,
which is discussed in Chapter 18. Step 8 provides a printed design sum-
mary. As part of the summary, charts illustrate how required pavement
thickness varies with the number of annual departures or with the pavement
flexural strength. Unfortunately for international users, the spreadsheet is
only available in US customary units, although the FAA design charts are
presented in both SI and US customary units.
Layered elastic design (Chapter 7)
LEDFAA can be downloaded from the FAA website, http://www.faa.gov/
airports_airtraffic/airports/construction/design_software/. The basic LED-
FAA input screen is shown in Figure 10.5.
214 Airport pavement design
Figure 10.5 LEDFAA basic input screen.
The program may be used to design new flexible or rigid pavements and
four types of overlays. Design examples are provided for each pavement
type. The basic input screen is used to select the pavement type and units
to be used (SI or US customary). An extensive help file is provided, as well
as an embedded software demonstration.
The pavement structure is input first. A new rigid pavement design is
copied into the design file from a file of samples stored in the program.
A sample rigid pavement section is shown in Figure 10.6.
Layer thicknesses are in mm if the program is used with SI units. The
concrete MOR is given in MPa, and the modulus of elasticity of each under-
lying layer is also given in MPa. One unusual aspect is that the modulus of
subgrade reaction k is given in kg/cm
rather than MPa/m, but since the
values are almost identical the traditional k in MPa/m should be input.
The basic rigid pavement structure stored within LEDFAA consists of
355.6 mm (14 in) of P-501 concrete pavement, 152.4 mm (6 in) each
of P-306 Econocrete and P-209 crushed aggregate, with elastic moduli of
4.8 GPa (700,000 psi) and 517 MPa (75,000 psi), respectively. The modulus
of subgrade reaction is 38 4 kg/cm
or MPa/m (141 psi/in), with an elastic
modulus of 103 MPa (15,000 psi).
Airport pavement design 215
Figure 10.6 Sample rigid pavement section from the LEDFAA samples file.
Once the structure has been selected, the layers may be modified by chang-
ing the thickness or modulus, or by selecting a different type of material,
such as replacing a P-306 econocrete subbase layer with P-304 CTB.
Once the structure has been modified, the designer selects the aircraft
button from the structure screen to input the aircraft traffic mix. An example
of an aircraft traffic mix is shown in Figure 10.7.
There are six built-in aircraft groups to select from – generic, Airbus,
Boeing, McDonnell-Douglas, other commercial, and military. A library of
aircraft is provided within each group. Once an aircraft type is selected
from the library and added, the aircraft type, gross taxi weight (in metric
tons or pounds), and a default number of 1,200 annual departures is added
to the list. If only a single aircraft type is selected, the program notifies the
user that this is a non-standard traffic mix.
The aircraft gross taxi weight may be modified, within limits. The number
of annual departures may be set at any number up to 100,000. For some
aircraft types, such as the DC-10-30 and MD-11, the wing and belly gear
are treated separately and a line for each is included in the table. Finally,
the aircraft traffic mix is saved, and the designer used the back button to
return to the Structure screen.
216 Airport pavement design
Figure 10.7 Aircraft traffic mix.
The design is completed by pressing the “Design Structure” button on the
Structure screen. The thickness of the top layer is changed until the CDF
for tensile stress at the bottom of the concrete is 1, based on the fatigue
damage from each aircraft type as calculated using equation 6.4.
FAA AC 150/5320-6D provides a rigid pavement design example using
design curves. The design aircraft has a dual tandem gear configuration and
a gross weight of 160,000 kg (350,000 lb). There are 6,000 annual equiva-
lent departures of the design aircraft, including 1,200 annual departures of
a B747 wide-body aircraft with a gross weight of 350,000 kg (780,000 lb).
The concrete flexural strength is 4.5 MPa (650 psi), and the subgrade
is a low plasticity clay with a modulus of subgrade reaction of 27 MPa/m
(100 psi/in). There is a 150-mm (6-in) thick stabilized subbase layer, which
increases the k-value to 57 MPa/m (210 psi/in). Use of the design chart
(Figure 3.19) provides a required thickness of 422 mm (16.6 in), which is
rounded up to 460 mm (17 in) (FAA 2004: 84).
The design may also be carried out using the spreadsheet program
R805faa.xls. The design aircraft may be input as either a DUAL TAN-300
Airport pavement design 217
or DUAL TAN-400 with the appropriate gross aircraft weight. The required
pavement thickness is slightly less, 404 mm (15.9 in), which due to rounding
will provide a savings of 25 mm (1 in) in the final pavement thickness. The
required dowel diameter, length, and spacing, from Table 10.4, are 30 mm
(11/4 in), 510 mm (20 in), and 380 mm (15 in), respectively. Because the
subbase is stabilized, the joint spacing is limited to five times the pavement
radius of relative stiffness.
If a pavement with the same flexural strength, support, and stabilized
subbase is designed for the forecast traffic and equivalent annual departures
shown in Table 10.2 and Figure 10.4, the required pavement thickness
would be 450 mm (17.7 in). The required dowel diameter, length, and
spacing, from Table 10.4, are increased to 40 mm (11/2 in), 510 mm (20 in),
and 460 mm (18 in), respectively.
LEDFAA provides a rigid pavement design example in its embedded help
file. The structure shown in Figure 10.6 is modified so that the concrete
flexural strength is 5.0 MPa (725 psi), the P-306 econocrete is replaced by
P-304 CTB with an elastic modulus of 3.45 GPa (500,000 psi), and the
modulus of subgrade reaction is changed to 32.6 MPa/m (120 psi/in). The
thickness of the subbase layers is not changed.
The aircraft traffic mix is shown in Table 10.5 and Figure 10.7. With the
TDT gear B-777-200 B in the traffic mix, the pavement cannot be designed
To complete the design, the program iterates to find a new concrete
pavement layer thickness of 406.7 mm (16 in). The two subbase layers are
not adjusted. Results of the design are shown in Figure 10.8.
For comparison, the second traditional/R805faa.xls example shown
above may be checked using LEDFAA. The sample rigid pavement structure
Table 10.5 Traffic mix for LEDFAA design example
No. Name Gross weight Annual
1 B-737-400 68,000 150,000 360
2 B-747-400 396,000 873,000 4,200
3 B-757 113,000 250,000 360
4 B-767-200 152,000 335,000 720
5 B-777-200 B 288,000 634,500 720
6 MD-82/88 68,000 150,000 600
7 DC-10-30 264,000 583,000 360
8 DC-10-30 Belly 264,000 583,000 360
9 MD-11 282,000 621,000 700
10 MD-11 Belly 282,000 621,000 700
11 L-1011 225,000 496,000 320
218 Airport pavement design
Figure 10.8 Example problem rigid pavement section as designed.
from Figure 10.6 is modified to change the concrete flexural strength to
4.5 MPa (650 psi), delete the P-209 crushed aggregate layer, and modify
the modulus of subgrade reaction to 27 MPa/m (100 psi/in). The traffic mix
is entered from the top half of Table 10.2.
The required pavement thickness calculated using LEDFAA is 461 mm
(18 in), which is thicker than the design required by the traditional method.
This aircraft traffic mix does not contain any TDT aircraft, so the result
from R805faa.xls should be used rather than that from LEDFAA.
Airport pavements for light aircraft
FAA defines pavements for light aircraft as “those intended to serve aircraft
weights of less than 30,000 pounds (13,000 kg). Aircraft of this size are usu-
ally engaged in nonscheduled activities, such as agricultural, instructional,
or recreational flying” (FAA 2004: 125).
Whether subbases are required depends on the gross aircraft weight.
Rigid pavements designed to serve aircraft weighing between 12,500
pounds (5,700 kg) and 30,000 pounds (13,000 kg) will require a
Airport pavement design 219
minimum subbase thickness of 4 inches (100 mm) except as shown in
Table 3–4 of Chapter 3. No subbase is required for designs intended
to serve aircraft weighing 12,500 pounds (5,700 kg) or less, except
when soil types OL, MH, CH, or OH are encountered. When the above
soil types are present, a minimum 4-inch (100-mm) subbase should be
(FAA 2004: 129)
Thickness design is straightforward. “Rigid pavements designed to serve
aircraft weighing 12,500 pounds (5,700 kg) or less should be 5 inches
(127 mm) thick. Those designed to serve aircraft weighing between 12,501
pounds (5,700 kg) and 30,000 pounds (13,000 kg) should be 6 inches
(150 mm) thick” (FAA 2004: 130). Although at first glance it seems unusual
not to take the modulus of subgrade reaction into account, the subgrade
and subbase construction requirements will ensure satisfactory support for
Jointing of light load rigid pavements is also relatively simple.
The maximum spacing of joints for light-load rigid pavements should
be 12.5 feet (3.8 m) for longitudinal joints and 15 feet (4.6 m) for trans-
verse joints Note that several differences exist between light-load
and heavy-load rigid pavement joints. For instance, butt-type construc-
tion and expansion joints are permitted when an asphalt or cement
stabilized subbase is provided. Also, half-round keyed joints are permit-
ted even though the slab thicknesses are less than 9 inches (230 mm).
Odd-shaped slabs should be reinforced with 0.05 percent steel in both
directions. Odd-shaped slabs are defined as slabs that are not rect-
angular in shape or rectangular slabs with length-to-width ratios that
(FAA 2004: 130)
FAA also allows a special tension ring design for light duty pavements no
more than 18.3 m (60 ft) wide. Interior joints may use keyways for load
The concept behind the jointing patterns shown is the creation of a
“tension ring” around the perimeter of the pavement to hold joints
within the interior of the paved area tightly closed. A tightly closed
joint will function better than an open joint. The last three contrac-
tion joints and longitudinal joints nearest the free edge of the pave-
ment are tied with [13 mm] #4 deformed bars, 20 inches (510 mm)
long, spaced at 36 inches (1 m) center to center. At the ends of the
220 Airport pavement design
pavement and in locations where aircraft or vehicular traffic would
move onto or off the pavement, a thickened edge should be con-
structed. The thickened edge should be 1.25 times the thickness of
the slab and should taper to the slab thickness over a distance of
3 feet (1 m).
(FAA 2004: 130)
Industrial pavement design
Industrial pavement facilities include rail and truck terminals, industrial
storage facilities, intermodal facilities, material handling yards, and ports.
Design of industrial pavements is similar to that of other types of pavements,
but there are important differences.
For example, the wheel loads on container and trailer-handling vehicles
may greatly exceed those of highway trucks and even of the heavi-
est modern aircraft; the required service life of the pavement may be
shorter than that required for highway and airport pavements; and the
pavement serviceability requirements may not have to be as strict as for
highway and airport pavements carrying high-speed traffic.
(PCA 1987: 1)
Industrial pavements may be made of conventional concrete pavement,
although the heavy duty load-carrying capacity and economy of RCC pave-
ments makes them ideal for this application. Vehicle speeds are generally
low, so pavement smoothness is less important than for highways or air-
port runways. Owners are generally interested in keeping construction and
maintenance costs low, so economical and durable pavements are favored.
This accounts for the increasing popularity of RCC pavements for these
The PCA has published IS234.01P, Design of Heavy Industrial Concrete
Pavements (PCA 1988). This addresses some of the specialized aspects
of industrial pavement design, and was adapted from design procedures
for concrete airport pavements. The PCA has also published IS233.01,
Structural Design of Roller-Compacted Concrete for Industrial Pavements
Like airport pavements, industrial pavements are designed to carry a
relatively predictable number of heavy vehicle loads. The design vehicle
may be heavy trucks parking at a facility, or heavy duty materials han-
dling equipment moving freight containers or other large items. Loads may
include large forklift trucks, straddle carriers, and log stackers, with wheel
222 Industrial pavement design
loads up to 578 kN (130 kip). Although the heavy point loads represent an
unusual design situation, other aspects of conventional concrete paving still
apply, such as joint design, subgrade and subbase preparation, and concrete
quality (PCA 1988: 1).
The estimation of expected traffic is important. Required information
includes the axle and wheel load magnitudes, wheel configurations in terms
of the number of wheels and spacing between wheels, and the number of
repetitions (PCA 1988: 5). It is also important to determine whether the
vehicle traffic is heavily channelized, or relatively evenly distributed across
Usually the vehicle having the heaviest wheel load will control the
design, but the design should also be checked for adequacy if other
vehicle wheel loads are almost as heavy and travel the pavement fre-
quently. The maximum wheel load is half of the heaviest axle load
for the vehicle at its maximum loading. This information is usually
available from the vehicle manufacturer.
(PCA 1987: 3)
With rounding up of the required pavement thickness for the heaviest
loads, the pavement will generally have sufficient fatigue capacity to han-
dle any lighter loads. Total fatigue consumption due to the heavier and
lighter loads can be checked using the pavement evaluation module for
each vehicle type, and adding up the fatigue damage percentage due to
each vehicle using equation 6.4 to determine the CDF. This is outlined
in the RCCPave help file, and described in the PCA guide (PCA 1988:
In some cases, it may be necessary to consider the weight of the loaded
containers themselves. Individual containers may weigh more than 289 kN
(65,000 lb) fully loaded, and may be stacked up to four high. In theory, this
would require a pavement thickness of 457–610 mm (18–24 in). However,
pavements in Halifax, Winnipeg, and Wando Terminal – Charleston have
been able to handle containers four high with 275–400 mm (11–16 in)
thick pavements. It is unlikely that all four containers would contain
the maximum weight. It is also possible that under sustained container
loads, some stress relief occurs due to creep (PCA 1988: 11–12). There-
fore, the thickness design based on the container handlers is generally
Point loads may also be important – if trailers are connected to dollies
while parked, the dollies will not distribute loads as well as rear dual
tires. This is only likely to control the design of lightly loaded industrial
pavements. In some cases, it is desirable to provide thicker pads, with
or without reinforcement, for smaller areas of the pavement subject to
Industrial pavement design 223
Conventional industrial pavements
Because of the similarities to airport pavement design, the ACPA AirPave
computer program may be used to design industrial pavements. Unfortu-
nately, this program does not have a library of industrial vehicles, so a user-
defined vehicle must be created. It is necessary to provide the gear/wheel
configuration, the contact area, the tire pressure, the number of wheels, and
the gross vehicle weight. Vehicle characteristics may be obtained from the
RCCPave computer program, discussed in the next section.
If a single design vehicle is used, this will be a relatively straightforward
procedure. Lighter vehicles can be checked to ensure that they will do
little or no fatigue damage. Using the Packard and Tayabji (1985) fatigue
relationships provided in equation 6.2, vehicles that impose a stress ratio
(SR) <0 45 will do no fatigue damage to the pavement.
RCC industrial pavements
The popularity of RCC pavements for industrial applications has been
increasing, because these pavements have low initial construction costs and
low maintenance costs (ACI Committee 325 1995). In the southeastern
US, automobile plant applications have included Saturn in Tennessee and
Honda and Mercedes in Alabama (Delatte et al. 2003). A 400 mm (16 in)
two-lift RCC pavement was constructed for the port of Norfolk, Virginia
The use of RCC for pavements at industrial facilities such as port and
intermodal container terminals is particularly appropriate because of
its ability to construct low-cost concrete pavements over large areas,
allowing flexibility in terminal operations over time. Two basic pave-
ment designs are used which incorporate RCC: 1) unsurfaced, where
high-strength concrete is used as the surface layer, and 2) asphalt sur-
faced, where lower-strength concrete is used as a pavement base and
an asphalt layer is used as the wearing surface RCC has been suc-
cessfully used at the Port of Boston, Port of Los Angeles, and for
container facilities at rail-truck intermodal yards in Denver, Colorado,
and Calgary, Alberta.
Single lift RCC pavements are limited in thickness to about 200–250 mm
(8–10 in). Thicker RCC pavements require two lift construction, preferably
with the second lift placed within 1 hour of the first lift. This is termed a
fresh joint or wet-on-wet construction. “Testing of core samples obtained
from RCC paving projects indicates that properly constructed multiple-lift
RCC pavements develop sufficient bond at the interface to be considered
224 Industrial pavement design
monolithic, except along edges that were unsupported during compaction”
(ACI Committee 325 1995: 13–14).
The original design procedures for RCC pavements closely followed pro-
cedures for conventional concrete pavements. Both the PCA and the USACE
developed RCC pavement design charts, which have been reproduced in
ACI 325.10R (ACI Committee 325 1995: 12–15).
No dowels are used for RCC joints, which rely on aggregate interlock.
When used, sawn transverse joints have been spaced 9.1–21.3 m (30–70 ft)
apart. Often joints are not sawn and the pavement is allowed to crack
naturally. Joints and cracks tend to remain tight. Maintenance costs for
RCC pavements are generally low.
The ACPA has developed a computer program, RCCPave, to design RCC
industrial pavements. It is computationally similar to AirPave, but uses a
different fatigue relationship specifically developed for RCC. It also has a
built-in library of industrial vehicles, including 80 kN (18 kip) single axles
with single and dual tires, 178 kN (40 kip) tandem axles with dual wheels,
and a variety of material handlers, as shown in Figure 11.1. User-defined
vehicles may also be created. This library may also be used to determine
vehicle characteristics for AIRPave to design a conventional concrete pave-
The RCCPave program may be used to design the thickness of a new
pavement or to evaluate an existing pavement. One important input is
Figure 11.1 RCCPave vehicle library.
Industrial pavement design 225
whether an interior or edge-loading condition should be used – in most
cases, most vehicle traffic will be away from the pavement edge and it
is reasonable to use the less conservative interior loading condition. This
same assumption is typically used for airport pavement design. The PCA
recommends increasing pavement thickness by 20 percent if vehicles will
travel near or at the pavement edge (PCA 1987: 2). Rather than increasing
pavement thickness, it makes more sense to extend the pavement width
about 0.6 m (2 ft) outside of the traveled way.
The designer must specify the desired pavement life and number of load
applications, along with the MOR and modulus of elasticity of the RCC
and the modulus of subgrade reaction. If the concrete MOR and/or mod-
ulus of elasticity are not known, they may be estimated from compressive
or splitting tensile strength. Modulus of subgrade reaction may be input
directly or estimated based on a fine or coarse-grained soil with or with-
out a subbase. The PCA recommends using the 90-day pavement flexural
strength for design because the number of load repetitions in the first 3
months of pavement life is likely to be low.
Industrial pavement design examples (RCCPave
These design examples have been modified from the PCA publication
on design of heavy industrial concrete pavements (PCA 1988: 8–9), and
redesigned using RCCPave software.
Design example 1 – container handler
The container handler has four wheels with a maximum single-wheel load
of 125 kN (28,000 lb). There are 40 repetitions per day of the container
handler, for a total of 292,000 repetitions over the 20-year life of the
pavement. The pavement flexural strength is 4.6 MPa (660 psi), and the
modulus of subgrade reaction is 27 MPa/m (100 psi/in). The design also
requires a modulus of elasticity, which has a default value of 27.6 GPa
(4 million psi). The modulus of elasticity has very little effect on the design,
so it is generally reasonable to use the default value.
This requires a user-defined input vehicle, with tire pressure of 758 kPa
(110 psi) and spacing between the tires of 300 and 1200 mm (12 and 48 in).
Based on interior loading condition, the required pavement thickness is
200 mm (8 in) versus 250 mm (9.9 in) found using the PCA 1988 procedure.
The design results are shown in Figure 11.2.
If edge-loading is selected instead, the required thickness becomes 300 mm
(12 in). Therefore, the PCA 1988 result is halfway between the two condi-
tions (PCA 1988: 8–9). If a 200 mm (8 in) RCC pavement is used, it may
be built in a single lift.
Figure 11.2 RCCPave design results for example 1.
Industrial pavement design 227
AirPave produces a less conservative design for this example. The pro-
gram does not calculate a pavement thickness – instead, the user checks
different thickness values. For each thickness value, a number of repeti-
tions is produced, which is compared to the desired number of repetitions.
AirPave requires a pavement thickness of 178 mm (7 in) for this design
example using interior loading.
Design example 2 – mobile gantry crane
Design example 2 uses a mobile gantry crane with a lift capacity of 40 tons.
The vehicle has eight wheels (four duals) and a maximum dual-wheel load
of 400 kN (90,000 lb). This closely matches one of the vehicles from the
RCCPave library, so a Clarklift C500/Y800 CH is selected.
There are 50 repetitions per day of the container handler, for a total
of 365,000 repetitions over the 20-year life of the pavement. The pave-
ment flexural strength is 4.4 MPa (640 psi), and the modulus of subgrade
reaction is 54 MPa/m (200 psi/in). The design modulus of elasticity is the
default value of 27.6 GPa (4 million psi). The design inputs are shown in
The required pavement thickness based on interior loading is 457 mm
(18 in), which is very close to the 431 mm (17 in) required thickness
Figure 11.3 RCCPave design inputs for example 2.
228 Industrial pavement design
calculated in the PCA 1988 Design Guide (PCA 1988: 9). For either thick-
ness, the pavement must be built in two lifts.
If this pavement is designed using AirPave, it is necessary to use a user-
defined vehicle to model the Clarklift C500/Y800 CH since only aircraft
are provided in the AirPave library. Once again, the AirPave results are less
conservative than the RCCPave results, with a 406 mm (16 in) pavement
required for interior loading. The input screen for AirPave is similar to
Figure 11.3, but only the pavement evaluation option is available, not
Industrial pavement case studies
Two case studies are presented below illustrating conventional and RCC
industrial pavement design and construction.
Conventional industrial pavement with shrinkage
Keith et al. (2006) reported a case study of an industrial distribution center
pavement made with shrinkage compensating concrete, long joint spac-
ing, and diamond-shaped plate dowels. Shrinkage compensating concrete
expands slightly during the first 1–7 days of curing, in order to offset sub-
sequent later shrinkage. It may be made using either special type K cement,
or with conventional type I, II, or V cement with an expansive admixture
that has the same effect.
A first phase of construction with shrinkage compensating concrete at
the Atlanta Bonded Warehouse Corporation (ABW) distribution center in
Kennesaw, Georgia, began in 1993. Twelve years after construction, the
pavement was still performing well. Despite joint spacing up to 32 m
(105 ft), there were few random cracks and no observed edge-curl. Although
the pavement cost more to build than conventional concrete pavements,
long-term maintenance costs were projected to be much lower.
Therefore, a second phase was constructed 7 years later with approxi-
mately 27 000 m2
300 000 ft
of new pavement. One placement set a
world record for more than 3 900 m2
42 000 ft
without interior joints.
Joint spacing for the new construction varied from 26 to more than 104 m
(85 to more than 340 ft).
There were some other unusual design features:
• Diamond square plate dowels, 115 by 115 by 6 mm (41/2 by 41/2 by
1/4 in), were used for load transfer. The dowels are encased in plastic
sleeves that may be attached to the concrete form work to ensure
accurate placement. With this spacing, all joints are construction joints
Industrial pavement design 229
and were built as expansion joints with polyethylene plank as filler.
Joints were sealed with silicone.
• Joints were located to prevent reentrant slab corners. To minimize
restraint against movement, catch basins and manholes were located
near the center of slabs when possible, or isolated with compressible
• Because shrinkage compensating concrete is very sensitive to curing, an
innovative plastic backed wet curing sheet was used.
• The pavement was designed to carry tractor-trailer loads, and slab
thickness was 150 mm (6 in).
• Two layers of plastic sheeting on top of a smooth base were used to
reduce friction between the slab and base.
• A tight aggregate gradation was also used to minimize shrinkage.
Diamond plate dowels provide an advantage over conventional dowel bars
in that they allow transverse movements parallel as well as perpendicular
to joints. Therefore, they allow slabs to slip relative to each other, while
providing load transfer. This is particularly important when new concrete is
cast next to hardened concrete, because dowel bars provide restraint to the
shrinkage of the new concrete and may initiate cracking. Although diamond
plate dowels have been used for floor slabs and industrial pavements, they
have not yet been adopted for highway or airfield pavements.
Norfolk international Terminal RCC port facility expansion
The Virginia Port Authority selected RCC for a large container storage and
handling area at the Norfolk International Terminals in Norfolk, Virginia.
The project is well documented in Norfolk International Terminal Selects
RCC for Port Facility Expansion (PCA 2006) which provided the informa-
tion for this case study. The port is the second largest in gross tonnage on
the east coast of the United States and requires continuing expansion. The
initial expansion included 10.5 hectares (26 acres) of pavement 420 mm
(16.5 in) thick, for a total of 43,800 cubic meters (57,300 cubic yards)
of concrete. RCC was estimated to be significantly cheaper than asphalt,
conventional concrete, or concrete paver blocks.
The heavy container handling equipment has wheel loads of 133–266 kN
(30,000–60,000 lb) per tire. The heavy wheel loads traveling continually
along the same path had heavily rutted the asphalt pavement. To carry the
traffic loads, the RCC was designed for a flexural strength of 3.1 MPa
(450 psi) and a compressive strength of 17.2 MPa (2,500 psi) at 7 days.
Because of the pavement thickness it was necessary to place the RCC in
two lifts. The second lift had to be placed within 1 hour of the bottom lift to
ensure bond. Cores extracted after 7 days indicated that the interface was
well bonded. The completed surface was water cured and then sealed with
230 Industrial pavement design
a bituminous tack coat before placing a 75 mm (3 in) asphalt overlay to
allow adjustments for future differential settlement of the underlying soils.
The final project cost was $50 US per square meter ($42 per square yard)
and the production rate was 5.4 days per hectare (2.2 days per acre). A
large paver was able to place RCC 9.1 m (30 ft) wide in one pass. The
Port was pleased with the work and planned a further 8.1 hectare (20 acre)
Transitions, special details, and
Transitions between concrete pavements and bridges and other structures
and CRCP reinforcement require special designs and detailing. Details
depend on whether movement is to be restrained or accommodated. If
movement is to be restrained, enough reinforcement and anchorage must be
provided to resist the forces that develop. If movement is to be allowed, the
joints must be detailed and maintained so that they open and c